This comprehensive textbook provides a modern, self-contained treatment for upper undergraduate and graduate level stude

*296*
*40*
*34MB*

*English*
*Pages 705
[706]*
*Year 2021*

- Author / Uploaded
- Woodward P.M.
- Karen P.
- Evans J.S.O.
- Vogt T.

*Table of contents : CoverHalf TitleSolid State Materials ChemistryCopyrightContentsPrefaceAcknowledgments1. Structures of Crystalline Materials 1.1 Symmetry 1.1.1 Translational Symmetry 1.1.2 Rotational Symmetry 1.1.3 Crystallographic Point Groups and Crystal Systems 1.1.4 Bravais Lattices 1.1.5 Introduction to Space Groups 1.1.6 Symmetry Elements That Combine Rotation and Translation 1.1.7 Space-Group Symbols 1.1.8 Description of a Crystal Structure 1.2 Databases 1.3 Composition 1.3.1 Coordination, Stoichiometry, and Connectivity 1.3.2 The Generalized 8−N Rule 1.4 Structural Principles 1.4.1 Packing of Spheres 1.4.2 Filling Holes 1.4.3 Network Structures 1.4.4 Polyhedral Structures 1.5 Structures of Selected Materials 1.5.1 The Spinel Structure 1.5.2 The Garnet Structure 1.5.3 Perovskite Structures 1.5.4 Silicates 1.5.5 Zeolites 1.5.6 Zintl Phases 1.6 Problems 1.7 Further Reading 1.8 References2. Defects and More Complex Structures 2.1 Point Defects in Crystalline Elemental Solids 2.2 Intrinsic Point Defects in Compounds 2.3 Thermodynamics of Vacancy Formation 2.4 Extrinsic Defects 2.5 Solid Solutions and Vegard’s Law 2.6 Kröger–Vink Notation 2.7 Line Defects in Metals 2.7.1 Edge Dislocations 2.7.2 Screw Dislocations 2.8 Planar Defects in Materials 2.8.1 Stacking Faults 2.8.2 Twinning 2.8.3 Antiphase Boundaries 2.8.4 Crystallographic Shear Structures 2.9 Gross Nonstoichiometry and Defect Ordering 2.10 Incommensurate Structures 2.11 Infinitely Adaptive Structures 2.12 Problems 2.13 Further Reading 2.14 References3. Defect Chemistry and Nonstoichiometry 3.1 Narrow Nonstoichiometry in Oxides 3.1.1 Point Defects in a Pure Stoichiometric Oxide 3.1.2 Point Defects upon Oxidation/Reduction of the Stoichiometric Oxide 3.1.3 Equilibrium Equations for Oxidative and Reductive Nonstoichiometry 3.1.4 Defect Equilibria for Schottky-Type Redox Compensation 3.1.5 Acceptor-Doped Oxides 3.1.6 Donor-Doped Oxides 3.1.7 Solid Solubility of Dopants 3.1.8 Cautionary Note on Defect Models in Pure Oxides 3.2 Wide Nonstoichiometry in Oxides 3.3 Point Defects and Diffusion 3.3.1 Point-Defect Movements 3.3.2 Random Hopping 3.3.3 Hopping Under a Driving Force 3.3.4 Hopping Under a Concentration Gradient 3.3.5 Hopping Under an Electric Field 3.3.6 Relationship between Conductivity and Diffusivity 3.3.7 Ambipolar Diffusion 3.3.8 Temperature Dependence of Diffusivity 3.3.9 Diffusivity and Redox Defect Equilibria 3.3.10 Outline of Non-Steady-State Diffusion 3.3.11 Cautionary Note on Diffusion in Real Materials 3.4 Problems 3.5 Further Reading 3.6 References4. Phase Diagrams and Phase Transitions 4.1 Phase Diagrams 4.2 Two-Component Phase Diagrams 4.2.1 Without Compound Formation 4.2.2 With Compound Formation 4.2.3 Solid-Solution Formation 4.3 Three-Component Phase Diagrams 4.4 Structural Phase Transitions 4.4.1 Classification of Phase Transitions 4.4.2 Symmetry and Order Parameters 4.4.3 Introduction to Landau Theory 4.4.4 Second-Order Transitions 4.4.5 First-Order and Tricritical Transitions 4.4.6 Phonons, Soft Modes, and Displacive Transitions 4.5 Problems 4.6 Further Reading 4.7 References5. Chemical Bonding 5.1 Ionic Bonding 5.1.1 Coulombic Potential Energy 5.1.2 Lattice Energy and the Born–Mayer Equation 5.1.3 Experimental versus Calculated Lattice-Formation Energies 5.2 Atomic Orbitals 5.2.1 Energies of Atomic Orbitals 5.2.2 Sizes of Atomic Orbitals 5.3 Molecular-Orbital Theory 5.3.1 Homonuclear Diatomics: H[sub(2)][sup(+)] and H[sub(2)] 5.3.2 The Heteronuclear Diatomic Case: HHe 5.3.3 Orbital Overlap and Symmetry 5.3.4 Combination of σ and π Bonding: O[sub(2)] 5.3.5 Symmetry-Adapted Linear Combinations (SALCs) 5.3.6 Simple Polyatomic Molecules: BeH[sub(2)] and CH[sub(4)] 5.3.7 Conjugated π Bonding: C[sub(6)]H[sub(6)] 5.3.8 Transition-Metal Complexes: [CrCl[sub(6)]][sup(3−)] and [CoCl[sub(4)]][sup(2−)] 5.3.9 High- and Low-Spin Configurations 5.3.10 Jahn–Teller Distortions 5.4 Bond Valences 5.5 Problems 5.6 Further Reading 5.7 References6. Electronic Band Structure 6.1 The Band Structure of a Hydrogen-Atom Chain 6.1.1 The Electronic Structures of Cyclic HN Molecules 6.1.2 Translational Symmetry and the Bloch Function 6.1.3 The Quantum Number k 6.1.4 Visualizing Crystal Orbitals 6.1.5 Band-Structure Diagrams 6.1.6 Density-of-States (DOS) Plots 6.2 The Band Structure of a Chain of H[sub(2)] Molecules 6.3 Electrical and Optical Properties 6.3.1 Metals, Semiconductors, and Insulators 6.3.2 Direct- versus Indirect-Gap Semiconductors 6.4 Representing Band Structures in Higher Dimensions 6.4.1 Crystal Orbitals in Two Dimensions 6.4.2 Crystal Orbitals in Three Dimensions 6.5 Band Structures of Two-Dimensional Materials 6.5.1 Graphene 6.5.2 CuO[sub(2)][sup(2)]− Square Lattice 6.6 Band Structures of Three-Dimensional Materials 6.6.1 α-Polonium 6.6.2 Diamond 6.6.3 Elemental Semiconductors 6.6.4 Rhenium Trioxide 6.6.5 Perovskites 6.7 Problems 6.8 Further Reading 6.9 References7. Optical Materials 7.1 Light, Color, and Electronic Excitations 7.2 Pigments, Dyes, and Gemstones 7.3 Transitions between d Orbitals (d-to-d Excitations) 7.3.1 Ligand- and Crystal-Field Theory 7.3.2 Absorption Spectra and Spectroscopic Terms 7.3.3 Correlation Diagrams 7.3.4 Selection Rules and Absorption Intensity 7.4 Charge-Transfer Excitations 7.4.1 Ligand-to-Metal Charge Transfer 7.4.2 Metal-to-Metal Charge Transfer 7.5 Compound Semiconductors 7.5.1 Optical Absorbance, Band Gap, and Color 7.5.2 Electronegativity, Orbital Overlap, and Band Gap 7.6 Conjugated Organic Molecules 7.7 Luminescence 7.8 Photoluminescence 7.8.1 Components of a Phosphor 7.8.2 Radiative Return to the Ground State 7.8.3 Thermal Quenching 7.8.4 Lanthanoid Activators 7.8.5 Non-Lanthanoid Activators 7.8.6 Energy Transfer 7.8.7 Sensitizers 7.8.8 Concentration Quenching and Cross Relaxation 7.8.9 Up-Conversion Photoluminescence 7.9 Electroluminescence 7.9.1 Inorganic Light-Emitting Diodes (LEDs) 7.9.2 Organic Light-Emitting Diodes (OLEDs) 7.10 Materials for Lighting 7.10.1 Fluorescent-Lamp Phosphors 7.10.2 Phosphor-Converted LEDs for White Light 7.11 Problems 7.12 Further Reading 7.13 References8. Dielectrics and Nonlinear Optical Materials 8.1 Dielectric Properties 8.1.1 Dielectric Permittivity and Susceptibility 8.1.2 Polarization and the Clausius–Mossotti Equation 8.1.3 Microscopic Mechanisms of Polarizability 8.1.4 Frequency Dependence of the Dielectric Response 8.1.5 Dielectric Loss 8.2 Dielectric Polarizabilities and the Additivity Rule 8.3 Crystallographic Symmetry and Dielectric Properties 8.4 Pyroelectricity and Ferroelectricity 8.4.1 Ferroelectricity inBaTiO[sub(3)] 8.4.2 Antiferroelectricity 8.5 Piezoelectricity 8.6 Local Bonding Considerations in Non-Centrosymmetric Materials 8.6.1 Second-Order Jahn–Teller Distortions withd[sup(0)] Cations 8.6.2Second-Order Jahn–Teller Distortions with s[sup(2)]p[sup(0)] Cations 8.7 Nonlinear Optical Materials 8.8 Nonlinear Susceptibility and Phase Matching 8.9 Important SHG Materials 8.9.1 KH2PO[sub(4)] 8.9.2 KTiOPO[sub(4)] 8.9.3 Niobates and Tantalates 8.9.4 Organic and Polymer NLO Materials 8.9.5 Borates 8.10 Problems 8.11 Further Reading 8.12 References9. Magnetic Materials 9.1 Magnetic Materials and Their Applications 9.2 Physics of Magnetism 9.2.1 Bar Magnets and Atomic Magnets 9.2.2 Magnetic Intensity, Induction, Energy, Susceptibility, and Permeability 9.2.3 Unit Systems in Magnetism 9.3 Types of Magnetic Materials 9.4 Atomic Origins of Magnetism 9.4.1 Electron Movements Contributing to Magnetism and Their Quantization 9.4.2 Atomic Magnetic Moments 9.4.3 Magnetic Moments for 3d Ions in Compounds 9.4.4 Magnetic Moments for 4f Ions in Compounds 9.4.5 Note on Magnetic Moments of 4d and 5d Metals in Compounds 9.5 Diamagnetism 9.6 Paramagnetism 9.6.1 Curie and Curie–Weiss Paramagnetism 9.6.2 Pauli Paramagnetism 9.7 Antiferromagnetism 9.8 Superexchange Interactions 9.9 Ferromagnetism 9.9.1 Ferromagnetic Insulators and Half-Metals 9.9.2 Ferromagnetic Metals 9.9.3 Superferromagnets 9.10 Ferrimagnetism 9.11 Frustrated Systems and Spin Glasses 9.12 Magnetoelectric Multiferroics 9.13 Molecular and Organic Magnets 9.14 Problems 9.15 Further Reading 9.16 References10. Conducting Materials 10.1 Conducting Materials 10.2 Metals 10.2.1 Drude Model 10.2.2 Free-Electron Model 10.2.3 Fermi–Dirac Distribution 10.2.4 Carrier Concentration 10.2.5 Carrier Mobility and Effective Mass 10.2.6 Fermi Velocity 10.2.7 Scattering Mechanisms 10.2.8 Band Structure and Conductivity of Aluminum 10.2.9 Band Structures and Conductivity of Transition Metals 10.3 Semiconductors 10.3.1 Carrier Concentrations in Intrinsic Semiconductors 10.3.2 Doping 10.3.3 Carrier Concentrations and Fermi Energies in Doped Semiconductors 10.3.4 Conductivity 10.3.5 p–n Junctions 10.3.6 Light-Emitting Diodes and Photovoltaic Cells 10.3.7 Transistors 10.4 Transition-Metal Compounds 10.4.1 Electron Repulsion: The Hubbard Model 10.4.2 Transition-Metal Compounds with the NaCl-Type Structure 10.4.3 Transition-Metal Compounds with the Perovskite Structure 10.5 Organic Conductors 10.5.1 Conducting Polymers 10.5.2 Polycyclic Aromatic Hydrocarbons 10.5.3 Charge-Transfer Salts 10.6 Carbon 10.6.1 Graphene 10.6.2 Carbon Nanotubes 10.7 Problems 10.8 Further Reading 10.9 References11. Magnetotransport Materials 11.1 Magnetotransport and Its Applications 11.2 Charge, Orbital, and Spin Ordering in Iron Oxides 11.2.1 The Verwey Transition in Magnetite, Fe[sub(3)]O[sub(4)] 11.2.2 Double-Cell Perovskite, YBaFe[sub(2)]O[sub(5)] 11.2.3 CaFeO[sub(3)] and SrFeO[sub(3)] 11.3 Charge and Orbital Ordering in Perovskite-Type Manganites 11.3.1 Spin and Orbital Ordering in CaMnO[sub(3)] and LaMnO[sub(3)] 11.3.2 The La[sub(1−x)]Ca[sub(x)]MnO[sub(3)] Phase Diagram 11.3.3 Tuning the Colossal Magnetoresistance 11.4 Half-Metals and Spin-Polarized Transport 11.4.1 Magnetoresistant Properties of Half-Metals 11.4.2 CrO[sub(2)] 11.4.3 Heusler Alloys 11.4.4 Half-Metals with Valence-Mixing Itinerant Electrons 11.5 Problems 11.6 Further Reading 11.7 References12. Superconductivity 12.1 Overview of Superconductivity 12.2 Properties of Superconductors 12.3 Origins of Superconductivity and BCS Theory 12.4 C60-Derived Superconductors 12.5 Molecular Superconductors 12.6 BaBiO3 Perovskite Superconductors 12.7 Cuprate Superconductors 12.7.1 La[sub(2)]CuO[sub(4)] “214" Materials 12.7.2 YBa[sub(2)]Cu[sub(3)]O[sub(7−δ)] “YBCO” or “123” Materials 12.7.3 Other Cuprates 12.7.4 Electronic Properties of Cuprates 12.8 Iron Pnictides and Related Superconductors 12.9 Problems 12.10 Further Reading 12.11 References13. Energy Materials: Ionic Conductors, Mixed Conductors, and Intercalation Chemistry 13.1 Electrochemical Cells and Batteries 13.2 Fuel Cells 13.3 Conductivity in Ionic Compounds 13.4 Superionic Conductors 13.4.1 AgI: A Cation Superionic Conductor 13.4.2 PbF[sub(2)]: An Anionic Superionic Conductor 13.5 Cation Conductors 13.5.1 Sodium β-alumina 13.5.2 Other Ceramic Cation Conductors 13.5.3 Polymeric Cation Conductors 13.6 Proton Conductors 13.6.1 Water-Containing Proton Conductors 13.6.2 Acid Salts 13.6.3 Perovskite Proton Conductors 13.7 Oxide-Ion Conductors 13.7.1 Fluorite-Type Oxide-Ion Conductors 13.7.2 Perovskite, Aurivillius, Brownmillerite, and Other Oxide Conductors 13.7.3 SOFC Electrode Materials and Mixed Conductors 13.8 Intercalation Chemistry and Its Applications 13.8.1 Graphite Intercalation Chemistry 13.8.2 Lithium Intercalation Chemistry and Battery Electrodes 13.8.3 Lithium-Ion Batteries with Oxide Cathodes 13.8.4 Electrochemical Characteristics of Lithium Batteries 13.8.5 Other Lithium Battery Electrode Materials 13.9 Problems 13.10 Further Reading 13.11 References14. Zeolites and Other Porous Materials 14.1 Zeolites 14.1.1 Representative Structures of Zeolites 14.1.2 Roles of Template Molecules in Zeolite Synthesis 14.1.3 Zeolites in Catalysis 14.1.4 Ion-Exchange Properties 14.1.5 Drying Agents, Molecular Sieving, and Sorption 14.1.6 AlPOs and Related Materials 14.2 Mesoporous Aluminosilicates 14.3 Other Porous Oxide Materials 14.4 Metal–Organic Frameworks (MOFs) 14.4.1 MOF Structures 14.4.2 Some Applications of MOFs 14.5 Problems 14.6 Further Reading 14.7 References15. Amorphous and Disordered Materials 15.1 The Atomic Structure of Glasses 15.2 Topology and the Structure of Glasses 15.3 Oxide Glasses 15.4 Optical Properties and Refractive Index 15.5 Optical Fibers 15.6 Nucleation and Growth 15.7 The Glass Transition 15.8 Strong and Fragile Behavior of Liquids and Melts 15.9 Low-Temperature Dynamics of Amorphous Materials 15.10 Electronic Properties: Anderson Localization 15.11 Metallic Glasses 15.12 Problems 15.13 Further Reading 15.14 ReferencesAppendices Appendix A. Crystallographic Point Groups in Schönflies Symbolism Appendix B. International Tables for Crystallography Appendix C. Nomenclature of Silicates Appendix D. Bond-Valence Parameters in Solids Appendix E. The Effect of a Magnetic Field on a Moving Charge Appendix F. Coupling j–j Appendix G. The Langevin Function Appendix H. The Brillouin Function Appendix I. Measuring and Analyzing Magnetic Properties Appendix J. Fundamental Constants of Exact Value References for AppendicesIndex*

Solid State Materials Chemistry This book explores the fascinating world of functional materials from the perspective of those who are tasked with inventing them, solid state chemists. Written in a clear and accessible style, this book provides a modern-day treatment of solid state materials chemistry for graduate and advanced undergraduate level courses. With over 330 problems and 400 original ﬁgures, this essential reference covers a wide range of materials in a holistic manner, including inorganic and organic, crystalline and amorphous, bulk and nanocrystals. The introductory chapters cover topics such as crystal structures, defects, diffusion in solids, chemical bonding, and electronic band structure. Later chapters focus on important classes of functional materials including pigments, phosphors, dielectric materials, magnets, metals, semiconductors, superconductors, nonlinear optical materials, battery materials, zeolites, metal–organic framework materials, and glasses. The technological applications and synthesis methods used to prepare the materials that drive modern society are highlighted throughout. Patrick M. Woodward is a Professor in the Department of Chemistry and Biochemistry and holds a courtesy appointment in the Department of Physics at Ohio State University. He is best known for his studies of the structures and properties of perovskite-related materials. He has served as chair of the Solid State Chemistry Gordon Conference (2018), Associate Editor of the Journal of Solid State Chemistry (2006–2011), and Vice President of the Neutron Scattering Society of America (2014–2018). He is co-author of the widely used general chemistry textbook, Chemistry: The Central Science (Pearson Education Limited, 2018). Patrick is a recipient of an NSF Career Award (2001), a Sloan Research Fellowship (2004), a Leverhulme Visiting Professorship (2017), and is a Fellow of the American Chemical Society (2020). Pavel Karen is a Professor in the Department of Chemistry at the University of Oslo. His interests include inorganic reaction chemistry, solid state synthesis methods, crystallography, phase relations and thermodynamics, and point-defect chemistry; all components of his teaching portfolio. He is interested in the relationship between structure and properties of less common inorganic solids, such as mixed-valence oxides. Crystal structures are studied by X-ray and neutron diffraction, local structures by Mössbauer spectroscopy, and valencemixing by calorimetry. He is co-author of the chapter Phase Diagrams and Thermodynamic Properties in the Handbook on the Physics and Chemistry of the Rare Earths, Volume 30, High-Temperature Superconductors (Elsevier, 2000). Pavel is a member of the American Chemical Society, the American Crystallographic Association, and of the International

Union of Pure and Applied Chemistry’s Division II and the Interdivisional Committee on Terminology, Nomenclature and Symbols. John S. O. Evans is a Chemistry Professor at Durham University where he served as Head of Chemistry from 2009 to 2014. His research interests are in the synthesis and properties of (mainly) inorganic materials, their structural chemistry, and their real-world applications. In recent years he has worked, inter alia, on negative thermal expansion, symmetry properties of phase transitions, new oxide-chalcogenides and energy-related materials. He has a longstanding interest in developing powder diffraction methods and is co-author of Rietveld Reﬁnement: Practical Powder Diffraction Pattern Analysis using TOPAS (De Gruyter, 2019). John was awarded the 1997 Meldola prize of the Royal Society of Chemistry, and was coawarded the 2015 Royal Society of Chemistry Teamwork in Innovation Award for work with industry. Thomas Vogt is the Educational Foundation Endowed Chair in the Department of Chemistry and Biochemistry, Director of the NanoCenter and adjunct Professor in the Department of Philosophy at the University of South Carolina. His work focuses on establishing structure–property relationships of solid state materials using X-ray and neutron scattering and electron microscopy. He is recognized as Fellow of the American Physical Society, the American Association for the Advancement of Science, the Institute of Advanced Study at Durham University, and the Neutron Scattering Society of America. Thomas received the Carolina Trustee Professorship of the Board of Trustees in 2018 as well as the University of South Carolina’s Educational Foundation Award for Research in Science, Mathematics, and Engineering in 2019.

Solid State Materials Chemistry Patrick M. Woodward Ohio State University

Pavel Karen Universitetet i Oslo

John S. O. Evans Durham University

Thomas Vogt University of South Carolina

University Printing House, Cambridge CB2 8BS, United Kingdom One Liberty Plaza, 20th Floor, New York, NY 10006, USA 477 Williamstown Road, Port Melbourne, VIC 3207, Australia 314–321, 3rd Floor, Plot 3, Splendor Forum, Jasola District Centre, New Delhi – 110025, India 79 Anson Road, #06–04/06, Singapore 079906 Cambridge University Press is part of the University of Cambridge. It furthers the University’s mission by disseminating knowledge in the pursuit of education, learning, and research at the highest international levels of excellence. www.cambridge.org Information on this title: www.cambridge.org/9780521873253 DOI: 10.1017/9781139025348 © Patrick M. Woodward, Pavel Karen, John S. O. Evans, and Thomas Vogt 2021 This publication is in copyright. Subject to statutory exception and to the provisions of relevant collective licensing agreements, no reproduction of any part may take place without the written permission of Cambridge University Press. First published 2021 Printed in the United Kingdom by TJ International Ltd, Padstow Cornwall A catalogue record for this publication is available from the British Library. ISBN 978-0-521-87325-3 Hardback Cambridge University Press has no responsibility for the persistence or accuracy of URLs for external or third-party internet websites referred to in this publication and does not guarantee that any content on such websites is, or will remain, accurate or appropriate.

Contents

Preface Acknowledgments 1 Structures of Crystalline Materials 1.1 Symmetry 1.1.1 Translational Symmetry 1.1.2 Rotational Symmetry 1.1.3 Crystallographic Point Groups and Crystal Systems 1.1.4 Bravais Lattices 1.1.5 Introduction to Space Groups 1.1.6 Symmetry Elements That Combine Rotation and Translation 1.1.7 Space-Group Symbols 1.1.8 Description of a Crystal Structure 1.2 Databases 1.3 Composition 1.3.1 Coordination, Stoichiometry, and Connectivity 1.3.2 The Generalized 8−N Rule 1.4 Structural Principles 1.4.1 Packing of Spheres 1.4.2 Filling Holes 1.4.3 Network Structures 1.4.4 Polyhedral Structures 1.5 Structures of Selected Materials 1.5.1 The Spinel Structure 1.5.2 The Garnet Structure 1.5.3 Perovskite Structures 1.5.4 Silicates 1.5.5 Zeolites 1.5.6 Zintl Phases 1.6 Problems 1.7 Further Reading 1.8 References

page xvii xix 1 1 2 3 5 5 8 9 11 12 13 14 15 17 18 19 22 28 32 38 38 39 40 44 46 47 48 51 51

v

vi

Contents

2 Defects and More Complex Structures 2.1 2.2 2.3 2.4 2.5 2.6 2.7

2.8

2.9 2.10 2.11 2.12 2.13 2.14

Point Defects in Crystalline Elemental Solids Intrinsic Point Defects in Compounds Thermodynamics of Vacancy Formation Extrinsic Defects Solid Solutions and Vegard’s Law Kröger–Vink Notation Line Defects in Metals 2.7.1 Edge Dislocations 2.7.2 Screw Dislocations Planar Defects in Materials 2.8.1 Stacking Faults 2.8.2 Twinning 2.8.3 Antiphase Boundaries 2.8.4 Crystallographic Shear Structures Gross Nonstoichiometry and Defect Ordering Incommensurate Structures Inﬁnitely Adaptive Structures Problems Further Reading References

3 Defect Chemistry and Nonstoichiometry 3.1 Narrow Nonstoichiometry in Oxides 3.1.1 Point Defects in a Pure Stoichiometric Oxide 3.1.2 Point Defects upon Oxidation/Reduction of the Stoichiometric Oxide 3.1.3 Equilibrium Equations for Oxidative and Reductive Nonstoichiometry 3.1.4 Defect Equilibria for Schottky-Type Redox Compensation 3.1.5 Acceptor-Doped Oxides 3.1.6 Donor-Doped Oxides 3.1.7 Solid Solubility of Dopants 3.1.8 Cautionary Note on Defect Models in Pure Oxides 3.2 Wide Nonstoichiometry in Oxides 3.3 Point Defects and Diffusion 3.3.1 Point-Defect Movements 3.3.2 Random Hopping 3.3.3 Hopping Under a Driving Force

54 54 55 58 61 63 65 66 66 66 67 67 68 72 74 75 78 80 81 85 85 87 87 87 88 89 90 93 94 94 96 98 99 101 103 104

Contents

3.3.4 Hopping Under a Concentration Gradient 3.3.5 Hopping Under an Electric Field 3.3.6 Relationship between Conductivity and Diffusivity 3.3.7 Ambipolar Diffusion 3.3.8 Temperature Dependence of Diffusivity 3.3.9 Diffusivity and Redox Defect Equilibria 3.3.10 Outline of Non-Steady-State Diffusion 3.3.11 Cautionary Note on Diffusion in Real Materials 3.4 Problems 3.5 Further Reading 3.6 References 4 Phase Diagrams and Phase Transitions 4.1 Phase Diagrams 4.2 Two-Component Phase Diagrams 4.2.1 Without Compound Formation 4.2.2 With Compound Formation 4.2.3 Solid-Solution Formation 4.3 Three-Component Phase Diagrams 4.4 Structural Phase Transitions 4.4.1 Classiﬁcation of Phase Transitions 4.4.2 Symmetry and Order Parameters 4.4.3 Introduction to Landau Theory 4.4.4 Second-Order Transitions 4.4.5 First-Order and Tricritical Transitions 4.4.6 Phonons, Soft Modes, and Displacive Transitions 4.5 Problems 4.6 Further Reading 4.7 References 5 Chemical Bonding 5.1 Ionic Bonding 5.1.1 Coulombic Potential Energy 5.1.2 Lattice Energy and the Born–Mayer Equation 5.1.3 Experimental versus Calculated Lattice-Formation Energies 5.2 Atomic Orbitals 5.2.1 Energies of Atomic Orbitals 5.2.2 Sizes of Atomic Orbitals 5.3 Molecular-Orbital Theory 5.3.1 Homonuclear Diatomics: H2+ and H2 5.3.2 The Heteronuclear Diatomic Case: HHe

vii

105 106 107 108 111 111 112 114 115 118 118 120 120 123 123 125 128 131 135 136 137 140 141 144 147 150 152 153 154 154 154 156 158 161 166 168 169 169 173

viii

Contents

5.4 5.5 5.6 5.7

5.3.3 Orbital Overlap and Symmetry 5.3.4 Combination of σ and π Bonding: O2 5.3.5 Symmetry-Adapted Linear Combinations (SALCs) 5.3.6 Simple Polyatomic Molecules: BeH2 and CH4 5.3.7 Conjugated π Bonding: C6H6 5.3.8 Transition-Metal Complexes: [CrCl6]3− and [CoCl4]2− 5.3.9 High- and Low-Spin Conﬁgurations 5.3.10 Jahn–Teller Distortions Bond Valences Problems Further Reading References

6 Electronic Band Structure 6.1 The Band Structure of a Hydrogen-Atom Chain 6.1.1 The Electronic Structures of Cyclic HN Molecules 6.1.2 Translational Symmetry and the Bloch Function 6.1.3 The Quantum Number k 6.1.4 Visualizing Crystal Orbitals 6.1.5 Band-Structure Diagrams 6.1.6 Density-of-States (DOS) Plots 6.2 The Band Structure of a Chain of H2 Molecules 6.3 Electrical and Optical Properties 6.3.1 Metals, Semiconductors, and Insulators 6.3.2 Direct- versus Indirect-Gap Semiconductors 6.4 Representing Band Structures in Higher Dimensions 6.4.1 Crystal Orbitals in Two Dimensions 6.4.2 Crystal Orbitals in Three Dimensions 6.5 Band Structures of Two-Dimensional Materials 6.5.1 Graphene 6.5.2 CuO22− Square Lattice 6.6 Band Structures of Three-Dimensional Materials 6.6.1 α-Polonium 6.6.2 Diamond 6.6.3 Elemental Semiconductors 6.6.4 Rhenium Trioxide 6.6.5 Perovskites 6.7 Problems 6.8 Further Reading 6.9 References

174 175 177 179 181 183 186 188 190 195 198 199 200 200 201 202 203 204 207 209 210 213 213 214 215 215 219 220 221 223 227 227 228 230 231 233 237 241 242

Contents

7 Optical Materials 7.1 Light, Color, and Electronic Excitations 7.2 Pigments, Dyes, and Gemstones 7.3 Transitions between d Orbitals (d-to-d Excitations) 7.3.1 Ligand- and Crystal-Field Theory 7.3.2 Absorption Spectra and Spectroscopic Terms 7.3.3 Correlation Diagrams 7.3.4 Selection Rules and Absorption Intensity 7.4 Charge-Transfer Excitations 7.4.1 Ligand-to-Metal Charge Transfer 7.4.2 Metal-to-Metal Charge Transfer 7.5 Compound Semiconductors 7.5.1 Optical Absorbance, Band Gap, and Color 7.5.2 Electronegativity, Orbital Overlap, and Band Gap 7.6 Conjugated Organic Molecules 7.7 Luminescence 7.8 Photoluminescence 7.8.1 Components of a Phosphor 7.8.2 Radiative Return to the Ground State 7.8.3 Thermal Quenching 7.8.4 Lanthanoid Activators 7.8.5 Non-Lanthanoid Activators 7.8.6 Energy Transfer 7.8.7 Sensitizers 7.8.8 Concentration Quenching and Cross Relaxation 7.8.9 Up-Conversion Photoluminescence 7.9 Electroluminescence 7.9.1 Inorganic Light-Emitting Diodes (LEDs) 7.9.2 Organic Light-Emitting Diodes (OLEDs) 7.10 Materials for Lighting 7.10.1 Fluorescent Lamp Phosphors 7.10.2 Phosphor-Converted LEDs for White Light 7.11 Problems 7.12 Further Reading 7.13 References 8 Dielectrics and Nonlinear Optical Materials 8.1 Dielectric Properties 8.1.1 Dielectric Permittivity and Susceptibility

ix

243 243 245 246 246 248 252 255 258 259 260 261 262 263 265 267 268 268 270 272 274 279 281 283 284 285 287 287 289 291 292 293 294 298 299 301 301 302

x

Contents

8.2 8.3 8.4

8.5 8.6

8.7 8.8 8.9

8.10 8.11 8.12

8.1.2 Polarization and the Clausius–Mossotti Equation 8.1.3 Microscopic Mechanisms of Polarizability 8.1.4 Frequency Dependence of the Dielectric Response 8.1.5 Dielectric Loss Dielectric Polarizabilities and the Additivity Rule Crystallographic Symmetry and Dielectric Properties Pyroelectricity and Ferroelectricity 8.4.1 Ferroelectricity in BaTiO3 8.4.2 Antiferroelectricity Piezoelectricity Local Bonding Considerations in Non-Centrosymmetric Materials 8.6.1 Second-Order Jahn–Teller Distortions with d 0 Cations 8.6.2 Second-Order Jahn–Teller Distortions with s2p0 Cations Nonlinear Optical Materials Nonlinear Susceptibility and Phase Matching Important SHG Materials 8.9.1 KH2PO4 8.9.2 KTiOPO4 8.9.3 Niobates and Tantalates 8.9.4 Organic and Polymer NLO Materials 8.9.5 Borates Problems Further Reading References

9 Magnetic Materials 9.1 Magnetic Materials and Their Applications 9.2 Physics of Magnetism 9.2.1 Bar Magnets and Atomic Magnets 9.2.2 Magnetic Intensity, Induction, Energy, Susceptibility, and Permeability 9.2.3 Unit Systems in Magnetism 9.3 Types of Magnetic Materials 9.4 Atomic Origins of Magnetism 9.4.1 Electron Movements Contributing to Magnetism and Their Quantization 9.4.2 Atomic Magnetic Moments 9.4.3 Magnetic Moments for 3d Ions in Compounds 9.4.4 Magnetic Moments for 4f Ions in Compounds 9.4.5 Note on Magnetic Moments of 4d and 5d Metals in Compounds

303 305 306 308 309 313 314 314 319 321 324 325 327 330 331 334 336 336 338 339 340 343 346 346 349 349 349 349 352 355 356 357 357 359 363 366 366

Contents

9.5 Diamagnetism 9.6 Paramagnetism 9.6.1 Curie and Curie–Weiss Paramagnetism 9.6.2 Pauli Paramagnetism 9.7 Antiferromagnetism 9.8 Superexchange Interactions 9.9 Ferromagnetism 9.9.1 Ferromagnetic Insulators and Half-Metals 9.9.2 Ferromagnetic Metals 9.9.3 Superferromagnets 9.10 Ferrimagnetism 9.11 Frustrated Systems and Spin Glasses 9.12 Magnetoelectric Multiferroics 9.13 Molecular and Organic Magnets 9.14 Problems 9.15 Further Reading 9.16 References 10 Conducting Materials 10.1 Conducting Materials 10.2 Metals 10.2.1 Drude Model 10.2.2 Free-Electron Model 10.2.3 Fermi–Dirac Distribution 10.2.4 Carrier Concentration 10.2.5 Carrier Mobility and Effective Mass 10.2.6 Fermi Velocity 10.2.7 Scattering Mechanisms 10.2.8 Band Structure and Conductivity of Aluminum 10.2.9 Band Structures and Conductivity of Transition Metals 10.3 Semiconductors 10.3.1 Carrier Concentrations in Intrinsic Semiconductors 10.3.2 Doping 10.3.3 Carrier Concentrations and Fermi Energies in Doped Semiconductors 10.3.4 Conductivity 10.3.5 p–n Junctions 10.3.6 Light-Emitting Diodes and Photovoltaic Cells 10.3.7 Transistors

xi

367 367 368 371 372 374 377 381 382 384 385 387 388 389 391 394 394 396 396 398 398 402 403 405 406 407 409 411 412 414 414 416 419 421 422 425 426

xii

Contents

10.4 Transition-Metal Compounds 10.4.1 Electron Repulsion: The Hubbard Model 10.4.2 Transition-Metal Compounds with the NaCl-Type Structure 10.4.3 Transition-Metal Compounds with the Perovskite Structure 10.5 Organic Conductors 10.5.1 Conducting Polymers 10.5.2 Polycyclic Aromatic Hydrocarbons 10.5.3 Charge-Transfer Salts 10.6 Carbon 10.6.1 Graphene 10.6.2 Carbon Nanotubes 10.7 Problems 10.8 Further Reading 10.9 References 11 Magnetotransport Materials 11.1 Magnetotransport and Its Applications 11.2 Charge, Orbital, and Spin Ordering in Iron Oxides 11.2.1 The Verwey Transition in Magnetite, Fe3O4 11.2.2 Double-Cell Perovskite, YBaFe2O5 11.2.3 CaFeO3 and SrFeO3 11.3 Charge and Orbital Ordering in Perovskite-Type Manganites 11.3.1 Spin and Orbital Ordering in CaMnO3 and LaMnO3 11.3.2 The La1−xCaxMnO3 Phase Diagram 11.3.3 Tuning the Colossal Magnetoresistance 11.4 Half-Metals and Spin-Polarized Transport 11.4.1 Magnetoresistant Properties of Half-Metals 11.4.2 CrO2 11.4.3 Heusler Alloys 11.4.4 Half-Metals with Valence-Mixing Itinerant Electrons 11.5 Problems 11.6 Further Reading 11.7 References 12 Superconductivity 12.1 12.2 12.3 12.4 12.5

Overview of Superconductivity Properties of Superconductors Origins of Superconductivity and BCS Theory C60-Derived Superconductors Molecular Superconductors

428 428 431 434 437 438 441 443 445 445 447 451 454 455 457 457 458 458 460 462 465 465 468 470 472 472 476 477 480 481 483 483 486 486 488 492 500 505

Contents

12.6 BaBiO3 Perovskite Superconductors 12.7 Cuprate Superconductors 12.7.1 La2CuO4 “214” Materials 12.7.2 YBa2Cu3O7−δ “YBCO” or “123” Materials 12.7.3 Other Cuprates 12.7.4 Electronic Properties of Cuprates 12.8 Iron Pnictides and Related Superconductors 12.9 Problems 12.10 Further Reading 12.11 References 13 Energy Materials: Ionic Conductors, Mixed Conductors, and Intercalation Chemistry 13.1 13.2 13.3 13.4

13.5

13.6

13.7

13.8

13.9 13.10 13.11

Electrochemical Cells and Batteries Fuel Cells Conductivity in Ionic Compounds Superionic Conductors 13.4.1 AgI: A Cation Superionic Conductor 13.4.2 PbF2: An Anionic Superionic Conductor Cation Conductors 13.5.1 Sodium β-alumina 13.5.2 Other Ceramic Cation Conductors 13.5.3 Polymeric Cation Conductors Proton Conductors 13.6.1 Water-Containing Proton Conductors 13.6.2 Acid Salts 13.6.3 Perovskite Proton Conductors Oxide-Ion Conductors 13.7.1 Fluorite-Type Oxide-Ion Conductors 13.7.2 Perovskite, Aurivillius, Brownmillerite, and Other Oxide Conductors 13.7.3 SOFC Electrode Materials and Mixed Conductors Intercalation Chemistry and Its Applications 13.8.1 Graphite Intercalation Chemistry 13.8.2 Lithium Intercalation Chemistry and Battery Electrodes 13.8.3 Lithium-Ion Batteries with Oxide Cathodes 13.8.4 Electrochemical Characteristics of Lithium Batteries 13.8.5 Other Lithium Battery Electrode Materials Problems Further Reading References

xiii

509 511 512 513 516 517 521 523 526 526

529 529 532 533 536 536 539 540 540 542 543 545 546 547 548 549 552 553 555 555 556 559 561 568 569 573 576 576

xiv

Contents

14 Zeolites and Other Porous Materials 14.1 Zeolites 14.1.1 Representative Structures of Zeolites 14.1.2 Roles of Template Molecules in Zeolite Synthesis 14.1.3 Zeolites in Catalysis 14.1.4 Ion-Exchange Properties 14.1.5 Drying Agents, Molecular Sieving, and Sorption 14.1.6 AlPOs and Related Materials 14.2 Mesoporous Aluminosilicates 14.3 Other Porous Oxide Materials 14.4 Metal–Organic Frameworks (MOFs) 14.4.1 MOF Structures 14.4.2 Some Applications of MOFs 14.5 Problems 14.6 Further Reading 14.7 References 15 Amorphous and Disordered Materials 15.1 15.2 15.3 15.4 15.5 15.6 15.7 15.8 15.9 15.10 15.11 15.12 15.13 15.14

The Atomic Structure of Glasses Topology and the Structure of Glasses Oxide Glasses Optical Properties and Refractive Index Optical Fibers Nucleation and Growth The Glass Transition Strong and Fragile Behavior of Liquids and Melts Low-Temperature Dynamics of Amorphous Materials Electronic Properties: Anderson Localization Metallic Glasses Problems Further Reading References

Appendix A: Appendix B: Appendix C: Appendix D: Appendix E: Appendix F:

Crystallographic Point Groups in Schönﬂies Symbolism International Tables for Crystallography Nomenclature of Silicates Bond-Valence Parameters in Solids The Effect of a Magnetic Field on a Moving Charge Coupling j–j

579 579 581 586 588 593 595 596 597 600 605 605 608 612 615 616 619 620 622 625 625 631 633 634 639 642 644 647 651 652 652 655 656 661 662 663 664

Contents

Appendix G: The Langevin Function Appendix H: The Brillouin Function Appendix I: Measuring and Analyzing Magnetic Properties Appendix J: Fundamental Constants of Exact Value References for Appendices Index

xv

665 666 670 672 673 674

Preface

Functional materials are an integral part of daily life. As an example, consider the materials that underpin smartphone technology. The integrated circuitry is made from complex patterns of semiconductors, metallic conductors, and insulators. Organic light-emitting diodes convert electrical signals from the processor into a vibrant high-resolution color display. The display is protected by a screen made from tough but lightweight Gorilla® glass, which is coated with a transparent conducting oxide to make the screen responsive to the touch of a ﬁnger. Magnetic materials are used in the speakers, a lithium-ion battery powers the device, speciﬁc dielectric materials are used to receive and isolate a call once the signal reaches a base station, and the list goes on. This book explores the fascinating world of functional materials from the perspective of those who are tasked with inventing them, solid state chemists. We therefore adopt the chemist’s deﬁnition of a material as a substance whose structure and properties are controlled at the atomic level to produce a speciﬁc function. Returning to our example, a modern smartphone contains over half of the non-radioactive elements on the periodic table. A few are used in their elemental form, but in most cases the desired function can only be achieved by combining elements to form compounds. With the periodic table as a palette, how does the chemist design and synthesize the mind-boggling variety of functional materials that future technologies depend upon? That question is the topic this book explores. The book is written speciﬁcally with teaching in mind and is intended primarily for use in upper-level undergraduate or graduate level courses. While our perspective is that of a chemist, the book is accessible to physicists and engineers as well. Mathematical details are given where they add deeper understanding, but the focus is always on relating the properties of a material to the characteristics of the atoms and molecules from which it is built. The ﬁrst six chapters cover the fundamentals of extended solids: crystal structures, defects, reactivity, phase diagrams, phase transitions, chemical bonding, and band structure. The remaining chapters, each of which is organized around a speciﬁc property or class of materials, show how the properties of modern functional materials can be understood from these fundamental concepts. Recognizing that the ﬁeld of solid state chemistry is much more expansive than can be covered in a single course, the later chapters are designed to be largely independent of each other. This organization provides the instructor freedom to tailor a course to cover those materials that are most relevant for their students. Coverage of inorganic and organic materials is interwoven throughout the book to place the emphasis on properties. To keep the scope at a manageable level, neither synthesis nor xvii

xviii

Preface

characterization are covered in detail. Instead, boxes on synthetic methods and characterization methods are placed throughout the book to highlight speciﬁc examples. In a similar vein, boxes are used to describe how the properties of nanoscale solids differ from bulk materials (Nanoscale Concepts), and to highlight important technological applications of materials (Materials Spotlight). Students learn by practice, and, in this spirit, we have included dozens of problems at the end of each chapter to allow students to test their understanding of the concepts covered in the chapter. Instructors can obtain a full set of worked solutions on request. We hope that this book will be a valuable source of learning for the next generations of solid state scientists and engineers and a resource for those who already work in this fascinating ﬁeld. Patrick Woodward Pavel Karen John Evans Thomas Vogt

Acknowledgments

We are indebted to several organizations and countless people for their support and encouragement. PMW would like to acknowledge the Leverhulme Foundation for supporting his stay at Durham University as a Visiting Professor during the 2017–2018 academic year. TV spent the beginning of 2018 as a Fellow at Durham University’s Institute of Advanced Study. He is grateful to Linda Crowe and the rest of the team at the institute, as well as David Wilkinson, Principal at St. John’s College, for their warm hospitality and for providing an environment so conducive to scholarly work. These overlapping stays in Durham were instrumental in making the ﬁnal push to ﬁnish this book. PMW is grateful for many years of support from the Solid State Materials Chemistry program of the National Science Foundation. PMW and JSOE thank Arthur Sleight for inspiration and early career mentoring. In these data-dominated times, PK is grateful to the now Professor Jiří Hanika for teaching Fortran programming in the 1970/1 course Computational Technology at the VŠCHT in Prague, and to the now Ing. František Hovorka, CSc, for the idea of taking an external typing course during the sophomore year 1967/8 at the SPŠCH Praha. We all would like to thank both colleagues and students who provided key feedback on early versions of the chapters. Finally, we thank our families for their patience and support over this long journey.

xix

1

Structures of Crystalline Materials

This book is about functional materials—those that perform a task or a technological operation. By the end of the book, we’ll see that all useful properties can ultimately be traced back to structure and dynamics at the atomic level of materials. Understanding structure is therefore of crucial importance. In this chapter we’ll investigate the structures of crystalline materials—those in which atomic arrangements are repeated periodically in three-dimensional (3D) space. Noncrystalline materials are covered in Chapter 15. In the ﬁrst section, we will discuss the symmetry and crystallography concepts that are important for the description of crystalline substances. A brief introduction to structure databases will follow. In the third section, we’ll cover the nomenclature and electron counting rules needed to understand the composition of solids; before learning in the fourth section how structures are built up by packing spheres, connecting coordination polyhedra, or via networks. In the ﬁfth and last section, we’ll discuss some structure types encountered later in the book. In addition to the ﬁgures and descriptions given in the chapter, readers might ﬁnd it useful to draw models of important structures with the included structural coordinates.

1.1

Symmetry In the ﬁrst section of this chapter, we’ll develop the language required to describe the structures of crystalline compounds. We know from everyday life that such materials frequently display an amazing regularity and symmetry on the macroscopic scale—salt crystals can grow as “perfect” cubes and many minerals and gemstones display wonderfully symmetric facets. The origin of this macroscopic symmetry can ultimately be traced back to the symmetry that’s present at the atomic scale (Å or 10−10 m). This local symmetry is replicated millions of times by translational symmetry to produce symmetric macroscopic objects. It’s perhaps worth stating at the outset that there is nothing “magical” about the high-symmetry structures materials adopt. As we will see in Chapter 5, local bonding 1

2

Structures of Crystalline Materials

interactions have inherent symmetry, and dense packing of such units is favorable energetically.

1.1.1 Translational Symmetry To describe a crystal structure, it is useful to introduce the concept of lattice; a spatial pattern of points of equal and equally oriented surroundings. We then deﬁne a motif, which might be a small group of atoms, a molecule, or a collection of several molecules. If we associate this motif with each of the lattice points, a crystal structure is built as shown in Figure 1.1. We can think of this “association” as re-drawing the motif at a constant displacement from each lattice point. The lattice is an operator of translational symmetry of crystal structures, of their periodicity. We can see in Figure 1.1 that the translational symmetry deﬁned by the lattice produces a structure in which the individual atoms in the motif achieve a sensible bonding environment. The small spatial segment that fully represents the entire structure upon periodic repetition is called the unit cell.1 We can use the analogy of tiles (2D) or bricks (3D) being stacked side by side. In 3D, the unit cell is a parallelepiped, a box whose sides are parallelograms. The size and shape of the unit cell is described with three lattice vectors a, b, c of lengths a, b, c, and angles α, β, γ. The angle α is between b and c, β between a and c, and γ between a and b. Together, a, b, c, α, β, γ are called lattice parameters or unit-cell parameters. Positions of atoms inside the unit cell are expressed with relative or fractional coordinates x,y,z in terms of fractions of the lattice vectors that deﬁne the unit cell. Fractional coordinates deﬁne the position (or radius) vector r from the unit-cell origin to the atomic position as r = xa + yb + zc. They can always be expressed on a 0 to 1 scale. Because of translational symmetry, a coordinate of 1.2 is equivalent to 0.2, or a coordinate −0.2 is equivalent to −0.2 + 1 = 0.8.

Figure 1.1 Association of an atomic motif with a lattice produces a crystal structure. 1

The following rules apply for choosing the unit cell: (a) its rotational symmetry is the same as that of the lattice, (b) the edges and angles are made as similar to each other as possible, (c) the number of right angles is maximized, and (d) the volume is minimized. Where applicable, the origin coincides with the inversion center of symmetry (Section 1.1.2). In some cases (Section 1.1.4), the cell contains more than one lattice point.

1.1

Symmetry

3

Figure 1.2 Description by indices of lattice planes and lattice directions with respect to the unit cell. An extra cell is drawn in order to show cases where planes facing the origin intercept the lattice vector at negative values.

Directions in the lattice are given with a [uvw] notation. When a line is drawn from the origin, parallel to the desired direction, then u,v,w are simply the relative/fractional coordinates of any point that line goes through, multiplied to give integer values. If it goes through ½,1,½, the direction is [121]. Symbols [242] and [484] would represent the same direction. A set of symmetrically equivalent lattice directions, such as [100], [010], [001], [−100], [0−10], [00−1] in a cubic lattice, is collectively referred to using angle brackets, ⟨100⟩. It’s often useful to deﬁne a set of parallel equidistant planes in a lattice. These are represented by an hkl notation. Starting with the plane that contains the origin, an hkl set of equidistant planes divides the unit-cell vector a into h sections, b into k sections and c into l sections (Figure 1.2). Dividing into 0 sections is possible and means that the set of planes is parallel with that axis. If the plane that faces the origin crosses a, b, or c at negative values, the appropriate h, k, or l of that set has negative sign (often put above the index, like h). An (hkl) symbol refers to a plane or to a crystal face (Miller indices). A set of their symmetryequivalent orientations is denoted in curly brackets, {hkl}.

1.1.2 Rotational Symmetry A point group2 is a set of symmetry operations that fulﬁll the mathematical requirements of being a group3 and act on an isolated geometrical object. The number of 2

3

At least one point of the object remains unshifted under point-group symmetry operations. Elementary knowledge of point-group symmetry may be an advantage for the reader; see Further Reading. A group must have a closure (combination of two elements yields an element of the group), fulﬁll the mathematic associative law (the result of combination of the elements is independent of the order they are applied), have an identity (an element that converts other elements into themselves), and have an inversion (every element has an inverse element; when combined together, they yield the identity element).

4

Structures of Crystalline Materials

Figure 1.3 Inversion center (symbol −1 or 1) at the origin operates on an object at the endpoint of the object’s radius vector r. The comma symbolizes a change in handedness (left- to right-hand relationship).

Figure 1.4 Operation of the twofold rotation axis (of symbols 2 in text and in graphics) on an object at the point r.

symmetry operations deﬁnes the order of the group; the higher the order, the higher the symmetry. The symmetry operations are performed by the elements of point symmetry; the identity, inversion center, mirror plane, rotation axis, and rotoinversion axis. All objects possess the identity; other symmetry elements may or may not be present. Let’s start with the inversion center. Figure 1.3 shows a point x,y,z represented by its radius vector r and the effect on that point of an inversion center at the origin of the coordinate system (shown by a small circle). Inversion moves x,y,z to −x,−y,−z. Mathematically, we can describe this transformation of r to r 0 with the equation r 0 = R ·r, where R is the matrix of the point-symmetry element, describing its operation.4 Inversion is given the symbol −1, often typeset as 1. Symmetry elements that unify a point in lattice space with another one by rotating it in steps of 1/n (n = 1, 2, 3, 4, 6) of the full circle are called n-fold rotation axes. The full-circle rotation (n = 1) is the identity, a twofold axis (n = 2) rotates by ½ of the full circle and has symbol 2, etc. As can be seen in Figure 1.4, twofold rotation around the z axis moves a point of fractional coordinates x,y,z to −x,−y,z. A rotoinversion axis is a single element, the operation of which combines rotation and inversion. However, the twofold rotoinversion axis −2, shown in Figure 1.5, operates like a mirror plane, m, as can be also demonstrated by 4

The three columns in this matrix are the products of the particular symmetry operation on the end-points of the respective unit-cell vectors (1,0,0), (0,1,0), and (0,0,1). This is conveniently used to set up the matrix.

1.1

Symmetry

5

Figure 1.5 Rotoinversion axis −2 is identical with mirror m.

multiplying together the matrices representing 2 and −1. Since m ≡ −2, all point-symmetry elements are in fact elements of rotational symmetry; the rotational axes 1, 2, 3, 4, 6 and the rotoinversion axes −1, −2, −3, −4, −6. Accordingly, the operation matrix of each of them has the symbol R.

1.1.3 Crystallographic Point Groups and Crystal Systems Due to the inﬁnite number of rotation axes, inﬁnitely many point groups are possible for isolated objects. However, in crystal structures, the translational symmetry of space ﬁlling is only compatible with a small number of rotation axes. Consider that we can tile a plane perfectly with identical rectangular tiles (twofold axis present), isosceles triangles (threefold), squares (fourfold), or hexagons (sixfold), but we can’t with pentagons (ﬁvefold) or heptagons (sevenfold), etc. This argument extends to the 3D space ﬁlled by the “bricks” of unit cells (Figure 1.1). The point groups with symmetry elements 1, 2, 3, 4, 6, 1, m (≡ 2), 3, 4, 6, which are compatible with translational symmetry, are called crystallographic point groups, also known as crystal classes. There are 32 crystallographic point groups and they are classiﬁed into seven crystal systems; cubic, tetragonal, hexagonal, trigonal, orthorhombic, monoclinic, and triclinic. Each crystal system is deﬁned by its minimum point-group symmetry (Table 1.1, see also Appendix A). If we take the cubic system as an example, the minimum-symmetry point group has symbol 23. It means that at each lattice point, the twofold axes along the x-, y-, and z-coordinate-system axes repeat the threefold axis of the symbol along all body diagonals of the adjacent cells. These threefold axes are easier to visualize and remember as the symmetry condition for the cubic crystal system. So if the actual crystal structure has four intersecting threefold axes, it is cubic. If you do not see intersecting threefold axes, the structure cannot be cubic even if the unit cell has right angles and equal edges.

1.1.4 Bravais Lattices As noted earlier, a lattice is a collection of points with identical surroundings. Having the highest rotational symmetry of each crystal system, 14 types of Bravais lattices are possible

6

Structures of Crystalline Materials

Table 1.1 Sorting 32 crystallographic point groups into seven crystal systems. Crystal system

Minimum symmetry

Higher-symmetry point groups

Triclinic Monoclinic Orthorhombic Tetragonal Hexagonal Trigonal Cubic

1 2, m 222 4, 4 6, 6 3, 3 23

1 2/m mm2, mmm 4/m, 422, 4mm, 4 2m, 4/mmm 6/m, 622, 6mm, 6m2, 6/mmm 32, 3m, 3m m3, 4 3m, 432, m3m

(Figure 1.6), which represent 14 types of translational symmetry in 3D lattice space5 of relative coordinates (Section 1.1.1). Some unit cells have lattice points only at the corners, and their lattices are called primitive Bravais lattices, labeled with symbol P. Others have lattice points located also at the centers of some or all unit-cell faces or at the unit-cell center, and these are called centered Bravais lattices. The body-centered lattice has symbol I (the cell has an additional lattice point at ½a + ½b + ½c relative to a P lattice). The face-centered lattices have symbol F when all unit-cell faces are centered. Symbol A, B, or C is used when just two opposite unit-cell sides are centered, along one direction, a, b, or c. Thus, C-centering6 adds an additional lattice point at ½a + ½b relative to a P lattice. A special type of centering, R, occurs in the hexagonal lattice, Figure 1.6. This R-centered lattice is equivalent to a P lattice with a rhombohedral7 unit cell, see Table 1.2. The rhombohedral lattice occurs only in those structures of the trigonal crystal system that carry the symbol R in their symmetry description. The remaining trigonal structures are described with a primitive hexagonal cell P. It is often convenient to express also the R structures on a hexagonal cell (not just the P). Having triple the volume of the rhombohedral cell, the hexagonal cell contains three rhombohedral lattice points: 0,0,0 and ⅔,⅓,⅓ with ⅓,⅔,⅔, shown in Figure 1.6 labelled as hR. Figure 1.7 gives an idea why only certain types of centering are possible for certain crystal systems. For example, a C-centered tetragonal cell could always be described with a smaller primitive cell, an F-centered tetragonal with a smaller I-centered cell. Similarly, a monoclinic B cell becomes a smaller P cell, monoclinic F cell becomes a smaller C cell, and a monoclinic I cell is equivalent to a C cell via an A cell rotated around b. However, there are cases where it is useful to choose a non-standard Bravais cell; for example in order to illustrate similarity between two structures. 5

6

7

The lattice space deﬁnes the orientation and angles of the coordinate-system axes applied to each unit cell of this space. While International Tables for Crystallography use the British-English forms “centre”, “centring”, and “centred”, the alternative spellings “center”, “centering”, and “centered” prevail in the USA. Terms like trigonal, tetragonal, and hexagonal originate in the rotational symmetry; the term rhombohedral implies that the Bravais cell is a rhombohedron, hence it refers to the lattice.

1.1

Symmetry

7

Figure 1.6 Standard settings of the 14 Bravais lattices. Lower-case letters: a = anorthic/triclinic, m = monoclinic, o = orthorhombic, t = tetragonal, h = hexagonal and c = cubic. Upper-case letters refer to centering. The primitive rhombohedral lattice is often described on its equivalent hR cell.

8

Structures of Crystalline Materials

Table 1.2 Metrics of lattices. Parameters not listed can take any values. Lattice

Conditions for lattice parameters

Triclinic (anorthic) Monoclinic Orthorhombic Tetragonal Rhombohedral Hexagonal Cubic

None* α = γ = 90° α = β = γ = 90° a = b, α = β = γ = 90° a = b = c, α = β = γ a = b, α = β = 90°, γ = 120° a = b = c, α = β = γ = 90°

* For limits on triclinic angles, see ref. [1].

Figure 1.7 Non-standard centering of monoclinic (top) and tetragonal Bravais cells (bottom). Drawing two cells reveals the true cell of the same crystal system.

1.1.5 Introduction to Space Groups We’ve seen that there are 32 crystallographic point groups and 14 Bravais lattices. Their combination gives a total of 230 space groups (we’ll see where this number comes from in Section 1.1.7). A space group deﬁnes both the translational symmetry (type of the Bravais lattice) and the rotational symmetry (point group) of the structure. Of the 230 space groups, 73 do not involve any symmetry other than that already present in the Bravais lattice and point group alone; these are called symmorphic space groups. The remaining 157 space groups are nonsymmorphic and possess translations by suitable fractions of lattice vectors, brought about by screw axes or glide planes. Before we explain these two terms, a note on symmetry operators. When discussing point groups, it was convenient to introduce the matrix operator R that acts on a point r of the relative-coordinate vector r such that r 0 = R · r. Because space groups

1.1

Symmetry

9

may include the above-mentioned additional fractional translations, this symbolic language is extended into a Seitz operator, (R | t) = R · r + t, which combines rotations (matrix R) and the possible translations (vector t). If we consider a symmetry element that involves no translations, such as the inversion 1, the Seitz symbol is (R | 0) hence (1 | 0). A rotational axis has a direction [uvw] that must be included. The Seitz symbol (2[001] | 0) then refers to a twofold rotation around the z axis. A plane has a direction as well—the direction of its normal vector that is oriented perpendicular to the plane. As an example, the mirror in the xy plane of Figure 1.5 has the Seitz symbol (m[001] | 0). The Seitz operators that include the fractional translations are explained in the subsection below.

1.1.6 Symmetry Elements That Combine Rotation and Translation The periodicity of crystal structures (their translational symmetry) means that the set of rotational symmetry elements repeats at each lattice point. This creates additional symmetry elements in between lattice points and may give rise to two types of symmetry elements that aren’t present in isolated molecules,8 screw axes and glide planes. A screw axis combines rotation with translation along the axis of rotation. An NM screw axis (M < N) rotates anticlockwise by 360/N degrees while shifting the image by a distance equal to an M/N fraction of the lattice periodicity along that axis. As an example, the twofold screw axis 21 in Figure 1.8 rotates by 180° and shifts by ½ of the vector c (the axis is along z). A 63 axis rotates by increments of 60° and each time shifts by 3/6 = ½ of c. Figure 1.9 shows the symmetry operations of axes 62 and 64, illustrating that screw axes NM and N(N−M) produce mirror images of each other. The “tailed hexagon” is the graphic symbol of the sixfold screw axes. A glide plane operates as a mirror plus a plane-parallel shift by half a vector length between two lattice points. When the shift is half of one lattice vector (either a, b, or c), the glide is called an axial glide plane a, or b, or c. The operation of the, say, c glide plane is a reﬂection

Figure 1.8 The screw axis 21[001] rotates 180° and shifts by ½ of the vector c. The graphical symbol of 21 parallel to the drawing plane is a half-arrow. 8

In the point groups used for isolated molecules, all symmetry elements intersect at a point; in space groups this is no longer true.

10

Structures of Crystalline Materials

Figure 1.9 Screw axes rotate anticlockwise. Axes 62 and 64 produce mirror images of each other. The 62 axis rotates by 60° and translates by 2/6 c, the 64 axis rotates by 60° and translates by 4/6 of the unit-cell length c. Due to translational symmetry, integers are subtracted from fractional coordinates ≥1, such as 3 /3 ≡ 0 or 10 /3 ≡ ⅓.

Figure 1.10 The glide plane c[100] creates a mirror image shifted by c/2.

followed by shift along c by half the c-length. This is shown in Figure 1.10 with the c-glide plane oriented in the direction of x.9 Note that an equally oriented plane with a translation along y would be called a b glide. In rare cases (ﬁve of the 230 space groups), centering creates a situation when the two alternative shift directions along a glide plane result in the same point. The symbol a, b, or c of such a glide plane is then changed to e (for equivalent or either), a double glide plane. When the shift length is half the sum of two lattice vectors (half the vector to the diagonal lattice point), we have a diagonal glide plane, denoted by the symbol n. An example for a/2 + b/2 is in Figure 1.11. When the shift is half of the F- or I-centering vector, we have a diamond glide plane, symbol d. This shift can be decomposed into components along lattice vectors (a /4) + (b /4) or (a /4) + (c /4) or (b /4) + (c /4) for the F-centered orthorhombic and cubic lattices, and into (a/4) + (b/4) +(c/4) for the I-centered tetragonal and cubic lattices. 9

As noted above (Section 1.1.5), the direction of a plane is the direction of the plane’s normal.

1.1

Symmetry

11

Figure 1.11 An orthorhombic diagonal glide n[001] in the xy plane, with its graphical symbol on top left (see also Appendix B). It creates a mirror image shifted by a/2 and b/2. The subsequent operation of the same diagonal glide then recreates the original point in the next unit cell.

1.1.7 Space-Group Symbols Shorthand symbols are used to name space groups. These consist of one of the Bravais-lattice symbols, P, F, I, R, A, B, C, followed by the symbol of the crystallographic point group, in which screw axes and glide planes can replace ordinary rotation axes and mirror planes when appropriate, for example Pnma. Non-symmorphic space groups are thus recognizable by the presence of symbols such as a, b, c, e, n, d, 21, 32, 42, etc., which indicate the fractional lattice translations. For quick understanding, it is helpful to know the orientation of the rotationalsymmetry elements listed in the standard10 space-group symbols (Table 1.3). Consider I 4/m c m (with individual posts separated for clarity) as an example. The presence of a fourfold axis, combined with the absence of threefold axes, tells us that this is a tetragonal space group (the I speciﬁes that the Bravais lattice is body-centered). The ﬁrst post 4/m means that both the fourfold axis and the mirror m are in the direction of c, hence 4 is perpendicular to m. The second post tells us that there are glide planes c in the directions of both edges of the square face (edges a and b) of the unit cell. The third post tells us that there are mirror planes in the direction of the diagonal of this square face. The triclinic crystal system has a P lattice and is compatible with only two symmetry elements; identity and inversion (Table 1.1). There are therefore only two triclinic space groups, those with symbols P1 and P1. As listed in Table 1.1, the monoclinic crystal system allows three types of rotational symmetry; the 2, m, and 2/m crystallographic point groups. There are two Bravais lattices (Figure 1.7) available; primitive, P, and base-centered, C. This results in six symmorphic space groups; P2, Pm, P2/m, C2, Cm, C2/m. Ten non-symmorphic monoclinic groups would be obtained by replacing 2 with screw axes 21 and m with glide planes c; P21, Pc, P21/m, P2/c, P21/c, C21, Cc, C21/m, C2/c, C21/c. However, not all of these 10 space groups are unique. This is because the combination of C-centering and the rotation axis 2 generates its “own” 21 (Figure 1.12). In the standard setting, they appear parallel to b at x = ¼ and ¾. For this reason, C21 ≡ C2, C21/m ≡ C2/m, C21/c ≡ C2/c, and there are not 16 10

Standard orientations are those with unit-cell axes a, b, c chosen by an agreed set of rules, as listed in the International Tables for Crystallography, Volume A. Permutations are possible but non-standard.

12

Structures of Crystalline Materials

Table 1.3 Directions of the three posts in standard space-group symbols. Trigonal directions refer to hexagonal unit cell. Crystal system

Post 1

Post 2

Post 3

Monoclinic Orthorhombic Tetragonal Trigonal Hexagonal Cubic

Perpendicular to the plane of the monoclinic angle (standard, || b) Edge a Edge b Edge c 4(4) || c Square edges Square diagonals 3(3) || c Rhombus edges Rhombus diagonal, longer 6(6) || c Edges 3(3) in body diagonals Face diagonals

Figure 1.12 Operation of a twofold axis 2[010] combined with monoclinic centering C (lattice points are marked with ×) makes a pattern of points related by screw axes 21[010] at x = ¼ and ¾ (marked with halfarrow heads).

but only 13 unique monoclinic space groups possible. Similar arguments can be developed for all crystal systems leading to a total of 230 unique 3D space groups. Symmetry information for all space groups is given in the International Tables for Crystallography, Volume A (for more details, see Appendix B of this book). The tables list, inter alia, the positions of all symmetry elements and how an atom at an initial point x,y, z is reproduced in the unit cell by the symmetry elements present.

1.1.8 Description of a Crystal Structure A crystal structure is deﬁned by its space-group symmetry, unit-cell parameters, and by the coordinates of the atoms in its asymmetric unit. The asymmetric unit contains only the atomic coordinates in the unit cell that are crystallographically unique, all other atomic positions are created by the symmetry-element operations. Atoms whose coordinates lie on symmetry elements are said to be on special positions, those which don’t, are on a general position (x,y,z, Appendix B). Different positions are often referred to using Wyckoff site labels. The Wyckoff site is labeled with a number and a letter (e.g. 8a). The number is the multiplicity of a site; it gives the number of equivalent points (atoms) generated by the available symmetry operations of that site from any one of them (the “original point”). The letter labels the sites for a given space group. The highest-symmetry site is listed as a and

1.2

Databases

13

Figure 1.13 Data needed to describe the crystal structure of nickel arsenide.

the lower-symmetry sites as b, c, d. . . (each with its own set of coordinates for symmetry equivalent points) in the International Tables for Crystallography, Volume A. For easy drawing, some ﬁgures will show auxiliary information that deﬁnes the crystal structure; its space group, unit-cell parameters, and fractional coordinates of atoms in the asymmetric unit. For example, in Figure 1.13, a nickel atom is listed in the site 2a at 0 0 0 and an arsenic atom in 2c at ⅓ ⅔ ¼. Application of symmetry operations in a structure-drawing software (or a look at pages of the space group number 194 in the International Tables, Volume A) yields an additional Ni at 0 0 ½ and an additional As at ⅔ ⅓ ¾, making a total of two formula units of NiAs per unit cell (Z = 2).

1.2

Databases In this chapter, we’ll introduce just a few of many structure types behind millions of individual crystal structures. Crystallography information comes in databases. The two with the longest tradition are the Inorganic Crystal Structure Database (ICSD) at the Fachinformationszentrum Karlsruhe in Germany and the Cambridge Structural Database (CSD), curated by the Cambridge Crystallographic Data Center. As of October 2020, the ICSD contained 232012 entries, the CSD 1094733. In addition, National Institute of Standards and Technology (NIST) has developed a wider Inorganic Structure database (NIST ICSD) that combines full structure data (mostly from ICSD) with the unit-cell identiﬁcation data set curated there as NIST Crystal Data since 1963. Databases provide powerful software tools for searching known structures, exploring similarities between materials, and for “data mining” to identify important chemical and structural trends. The structural information is exported in a standardized form of the crystallographic information ﬁle (cif) that is used as input for various crystallographic software packages. Some databases provide calculation of diffraction patterns, useful to identify materials. While the full databases require a license, there are several open-access resources online. Try a search on “icsd demo” or “database of zeolite structures” or “mineralogy database” or the “Crystallography Open Database”. Useful demo-version utilities for plotting crystal structures from cif ﬁles are searchable as well.

14

Structures of Crystalline Materials

1.3

Composition With the essential ideas of symmetry and crystallographic concepts in place, we’ll spend the rest of this chapter describing principles that rationalize structures as composites of different elements and entities. Materials adopt what at ﬁrst appears to be a bewildering variety of different atomic arrangements in 3D space. However, many of these arrangements can be readily understood by considering relatively simple structural rules that concern stoichiometry and connectivity patterns in compounds. For those purposes, it will be convenient to introduce the crystal-chemical formula [2] that summarizes structural information. These formulas list each crystallographically nonequivalent atom11 in the structure separately and contain information about its coordination to other atoms in superscripted square brackets. The coordination numbers in the brackets follow the same array as the atoms in the formula, and are separated by a comma, while any bonding to atoms of the same element comes after a semicolon. In addition to the coordination number, the bond geometry may be indicated by a lower-case letter (l = line, n = not in a line or plane, t = tetrahedron, o = octahedron, y = pyramid, p = prism, c = cube, co = cuboctahedron, etc.). To keep the formula as simple as possible, it’s common to include only connectivities of direct chemical bonds. These simpler formulas will generally be used in this chapter. The nomenclature is best illustrated with examples, such as those given in Table 1.4.

Table 1.4 Examples of crystal-chemical formulas for compounds; full = full* neighborhood, simpler = direct neighborhood (bonding). Full crystal-chemical formula Simpler crystal-chemical formula

Brief description of bonding

SiO2

Si[4t;]O2[2;] Si[4t]O2[2]

Si tetrahedrally coordinated by 4O while O is coordinated by 2Si

SrTiO3

Sr[8,12co;]Ti[8,6o;]O3[4,2;] Sr[12co]Ti[6o]O3[4,2]

Sr in cuboctahedron of 12 O and Ti in octahedron of 6O

FeS2

Fe[6o;]S2[3;1] Fe[6o]S2[3;1]

Fe in octahedron of 6S; (S–S)2− units present

MgAl2O4

Mg[12,4t;]Al2[6,6o;]O4[(1,3)t;] Mg[4t]Al2[6o]O4[1,3]

Mg in tetrahedral and Al in octahedral coordination

Y3Fe5O12

Y3[4,6,8c;]Fe2[6,6,6o;]Fe3[6,4,4t;]O12[(2,1,1)t;] Y3[8c]Fe2[6o]Fe3[4t]O12[2,1,1]

Y in a cube of 8O; two Fe sites, one octahedral, one tetrahedral

Formula

* Coordination numbers refer to the array of the other atoms in the formula, such as Sr 8-coordinated with Ti and 12-coordinated with a cuboctahedron of O in SrTiO3. Possible bonds to atoms of the same kind follow after the semicolon, such as 1 in FeS2.

11

Apart from chemical identity, crystallographically identical atoms have identical environments.

1.3

Composition

15

1.3.1 Coordination, Stoichiometry, and Connectivity If ionic charges are included, the crystal-chemical formula of a binary compound will incorporate three important balances: The electroneutrality balance, the connectivity balance, and the bond-valence balance (Figure 1.14). Let’s assume a binary compound CmAn of two non-identical elements, each at one unique site; one assigned as a “cation” C of charge number c, the other as an “anion” A of charge number a. The crystal-chemical formula is cþ ½N; a ½M; Cm An , where N and M are the coordination numbers of C and A, respectively. The electroneutrality balance requires that m × c = n × a. The connectivity balance requires that m × N = n × M because there must be an equal number of CA and AC connections. Lastly, c/N = a/M is the bond-valence balance [3].12 Understanding these balances allows us to make simple structural predictions from the chemical formula.13 Consider SiO2 as an example. We know from inorganic chemistry that silicon favors tetrahedral coordination, so the connectivity balance 1 × 4 = 2 × M gives M = 2 for the coordination number of oxygen (Table 1.4). For compounds having more than two sites, balances analogous to those for the two-site formula in Figure 1.14 can be set up. As an example, the mineral hausmannite, Mn3O4 (a spinel, Section 1.5.1), has Mn2+ in tetrahedral and Mn3+ in octahedral coordination. There is one oxygen site. Using this information, we write the formula Mn2+[4t]Mn3+2[6o]O4[x,y] with the coordination numbers around oxygen as unknowns. Two connectivity balances can be written, 1 × 4 = 4 × x for Mn2+ and 2 × 6 = 4 × y for Mn3+, and we see that each oxygen is coordinated by one Mn2+ and three Mn3+. For extended structures14 of ternary and higher-component phases, a bond graph is informative as it shows the connectivity visually, see Figure 1.15. The symbolism of a bond graph differs from symbolism of formulas used by molecular chemists, so let’s again illustrate it with the simple case of SiO2. One starts with the crystal-chemical formula (Table 1.4) and writes down one Si symbol surrounded by two O symbols. Then a line is drawn for each bonding connection between two atoms. The lines tell us that each oxygen is coordinated by two silicon atoms and each silicon is coordinated by four oxygens (the two lines between Si and O thus do not mean a double bond). A quick examination of the bond

Figure 1.14 Three balances in the crystal-chemical formula of a two-site compound. 12 13 14

Termed “the electrostatic valence principle” in ref. [3]. More on bond valences is in Section 5.4. Such estimates can be useful, see Box 1.1. Crystal structures with bond networks that extend over the entire volume.

16

Structures of Crystalline Materials

graphs of TiO2 and CaF2 shows that as the cation coordination number increases from 4 to 6 to 8, the anion coordination number increases from 2 to 3 to 4, consistent with the connectivity balance.

Figure 1.15 Examples of bond graphs. In V2O5, ﬁve oxygens occupy three crystallographically different sites of differing coordinations to V.

Box 1.1 Synthetic Methods: Preparation of Na3N Most binary ionic compounds were discovered long ago. A number of these compounds, such as NaCl and KCl, have played pivotal roles in the development and advancement of civilizations. In principle, such compounds form easily; one brings the two elements together and initiates the reaction. It is surprising to ﬁnd that, despite repeated attempts, at the end of the twentieth century no one had been able to prepare sodium nitride, Na3N. This changed in 2002 when Fischer and Jansen reported the ﬁrst successful synthesis [4]. Like many binary compounds, it was prepared from the elements. However, the preparation conditions were hardly typical. Atomic beams of the two components were generated separately in a microwave plasma and passed into a vacuum chamber where they condensed onto a sapphire substrate cooled to 77 K. At such a low temperature, the elements don’t react when deposited onto the substrate, but upon heating to 200 K they begin to form crystalline Na3N. This compound adopts the cubic ReO3 structure (see Table 1.9), with the cation and anion positions reversed. As might be expected for such an elusive compound, Na3N is not very stable, it decomposes above 360 K. Why is sodium nitride so difﬁcult to prepare and why is it unstable even after it forms? An important clue comes from the crystal-chemical formula, Na3[2l]N[6o]. Despite its large size, sodium is coordinated by only two nitride ions in a linear geometry. Compare this with stable transition metal nitrides such as ScN, ZrN, and CrN, where the NaCl-type structure gives a cation coordination number of six. The reason for the abnormally low cation coordination number in Na3N is a simple but unavoidable topological consequence of the stoichiometry. The C3A stoichiometry means that if the nitride ion is 6-coordinated (larger coordination numbers are rare for N3−) the sodium ion can only be 2-coordinated. This simple link between stoichiometry and coordination number [5] is the fundamental reason why the synthesis of Na3N has proved so difﬁcult. Typical coordination numbers for Na+ range from 6 to 12; the coordination number of two is an extreme outlier. Let’s also note that the densest-packing principle (Section 1.4.2) supports C3A of only the smallest cations C occupying voids among the largest anions A, such as Na3As or Li3N.

1.3

Composition

17

1.3.2 The Generalized 8−N Rule Atoms bond in patterns that yield stable electron conﬁgurations. For an electronegative sp atom of N valence electrons, the 8−N rule is valid: Valence electrons short of 8 are obtained in bonds. Carbon of 4 valence electrons obtains the missing 4 electrons by forming 4 bonds; phosphorus obtains the missing 3 electrons by forming 3 bonds, etc., as illustrated in Figure 1.16. In a binary compound, the more electronegative sp element, the one that attracts and holds electrons more, will maintain the 8−N rule in order to achieve a stable conﬁguration of the noble gas. Most electropositive sp elements will tend to lose their valence electrons to also achieve a noble-gas conﬁguration. The ionic approximation is therefore a convenient way of recognizing the stable conﬁgurations in a compound. Consider our binary solid CmAn (Section 1.3.1) of sp atoms. The valence-electron count per anion A, VECA, is calculated from the stoichiometry and from valence-electron numbers eC and eA: VECA ¼ ðm eC þ n eA Þ=n:

(1.1)

When VECA = 8, both atoms achieve the noble-gas conﬁguration as noted above. When VECA > 8, the excess electrons remain with the cation forming cation–cation bonds or cation-localized electron pairs. When VECA < 8, the atom A obtains the missing electrons by forming A–A bonds so that each A has an octet. The formal expression of this generalized 8−N rule [6, 7] for CmAn is: VECA ¼ 8 þ CC

m AA; n

(1.2)

where the variable CC is the number of electrons per “cation” C that form C–C bonds or are localized at the cation as lone pairs, and AA is the number of electrons per “anion” A that form A–A bonds. The generalized 8−N rule is useful for analysis of structures of nonmetallic sp phases. Let’s illustrate this using GaSe and SnCl2 with VECA > 8 and CdSb and CaC2 with VECA < 8. In GaSe, gallium has three valence electrons, selenium six, VECA = 9. The excess electron will remain with the Ga cation (CC = 1, Equation (1.2) and form single-bonded (Ga–Ga)4+ pairs. In

Figure 1.16 Structures of selected p elements drawn to equal scale.

18

Structures of Crystalline Materials

GaSe

SnCl2

Figure 1.17 Examples of structures with VECA > 8, in which the excess electrons per anion A are localized at the cation (smaller spheres) as bonds or as lone pairs. CdSb

CaC2

Figure 1.18 Examples of structures with VECA < 8, when “electrons missing to 8” at the anion A are obtained by sharing in bonds between A atoms.

SnCl2, tin has four valence electrons, chlorine seven, VECA = 9; one electron in excess. Given two Cl per Sn, two electrons remain at Sn (CC = 2) forming the lone electron pair of Sn2+. The structures of GaSe and SnCl2 are shown in Figure 1.17. In CdSb, the cadmium atom has two valence electrons,15 antimony ﬁve, and VECA = 7. The missing electron is obtained by sharing between two Sb atoms that form Sb24− singlebonded dumbbells (AA = 1) isoelectronic with I2 (Figure 1.18, left). In CaC2, calcium has two valence electrons, carbon four, and VECA = 5. The three missing electrons are obtained by sharing in three two-electron bonds (AA = 3), and triple-bonded C22− pairs isoelectronic with N2 are present in the crystal structure of CaC2 (Figure 1.18, right).

1.4

Structural Principles In this section, we’ll see that the principles of arranging atoms, ions, or molecules vary according to the type of forces that hold them together. In some structures, the building units are packed as efﬁciently as possible, in others directional covalent bonding gives rise to networks. In yet other structures it is the local chemical bonding environment of a central atom that dictates everything else about the structure. Appropriate visualization and understanding of such structures, as well as rationalizing their physical and chemical properties, depends on identifying the underlying principles upon which they were built. 15

4d orbitals in Cd are sufﬁciently low in energy that they can be considered part of the core.

1.4

Structural Principles

19

1.4.1 Packing of Spheres The structures of many materials can be understood by exploring how hard spheres pack. If we start in 2D, Figure 1.19 shows two symmetric ways of packing circles and their corresponding unit cells; it’s clear that the packing of Figure 1.19b is more space-efﬁcient. The packing efﬁciency, calculated as the area fraction ﬁlled by circles, is 0.785 and 0.907 for the two arrangements. The densest16 3D packing of spheres is based on stacking 2D layers of the type in Figure 1.19b. A second layer of spheres nestles in the dimples of the ﬁrst layer and is therefore laterally shifted relative to it (Figure 1.20). For the third layer, there are two choices for positioning the spheres. One choice reverses the shift direction so that the spheres in the third layer lie directly above those in the ﬁrst; the other choice continues shifting in the same direction, in which case the third layer does not lie directly above the ﬁrst layer. When we view the layers side on (Figure 1.21) the repeat unit is either AB or ABC. The former arrangement is called hexagonal closest packing (hcp), and the latter cubic closest packing (ccp). Both sequences ﬁll space equally efﬁciently (74.0% of space is occupied; 26.0% is voids between spheres) and would be energetically equivalent for hard spheres. For elements that adopt these arrangements, such as the solid noble gases and many metals, orbital symmetries make one or the other arrangement slightly more stable. Speciﬁc combinations of cubic and hexagonal stacking sequences can be stabilized in some structures; rare-earth metals are typical examples. Figure 1.22 shows how to analyze the sphere packing occurring in α-La. The ﬁrst step is to orient the unit cell so that we have an on-top view of the densely packed layers (against c in hexagonal structures) and the direction of subsequent shifts is horizontal; as shown in Figure 1.22 bottom. The structure is then rotated 90° so that the normals of the layers point up. We can then identify the closest-packed sphere layers as being A, B, C, mark the subsequent shifts as arrows, and assign letter c to a layer that has local cubic environment and h that has local hexagonal environment according to those shifts. The repetitive sequence of these letters is the basis of the Jagodzinski–Wyckoff notation of stacking sequences. The Ramsdell symbol gives the number of closest-packed sphere layers per unit cell of a Bravais lattice and a letter to signify the Bravais lattice (H for hexagonal, R for rhombohedral, C for cubic). As an example, the Ramsdell symbol for α-La is 4H. Figure 1.19 Two high-symmetry packings of circles. After Kepler [8].

16

Although these arrangements have long been suggested to be the densest form of packing of equal spheres (J. Kepler’s conjecture in ref. [8], apparently responding to the English Admiralty task to determine the most efﬁcient packing of cannonballs on ships), a widely accepted proof was only published in 1998 by Thomas Hales. A panel of referees was 99% certain the proof was correct.

20

Structures of Crystalline Materials

Figure 1.20 Two choices for placement of the third layer of densely packed spheres. One line of the subsequent layer shifts is used to analyze a densest packing.

Figure 1.21 Cubic (ccp) and hexagonal (hcp) closest packing of equal spheres. Edges of 8-unit cells are drawn for ccp, with body diagonals perpendicular to the layers. The two unit cells are below; facecentered cubic and primitive hexagonal.

1.4

Structural Principles

21

Figure 1.22 How to analyze sphere packing in hexagonal structures (α-La shown).

Figure 1.23 Spheres in contact in unit cells of primitive and body-centered cubic structures of metals.

In addition to the densest-packed arrangements, two other simple high-symmetry packings are found in metals and are shown in Figure 1.23; the primitive cubic arrangement on the left (adopted by α-Po) and the body-centered cubic (bcc) arrangement on the right. Note that in ccp (Figure 1.21), the spheres are in contact along the face diagonal of the unit cell, in bcc along the body diagonal, and in the primitive cubic packing along the cell edge. The preferred structures for metallic elements are given in Figure 1.24. Although the densest packing adopted by most elemental metals suggests non-directional bonds, this is true only as a ﬁrst approximation. It has been shown [9] that bonding electrons may concentrate in certain directions; in aluminum, they prevail in voids formed by every four mutually touching atoms of the cubic closest packing.

22

Structures of Crystalline Materials

Figure 1.24 Structure types commonly adopted by metallic elements.

Box 1.2 Nanoscale Concepts: Structure changes! At constant temperature and pressure, lattice parameters are constant. Except when the crystal enters the nano-size range. Then the lattice parameter contracts, depending of course on the crystal’s shape. The culprit is the surface of the nanocrystal. At a surface, only a portion of the atoms’ bonding ability is utilized, the remaining bonds are open-ended, so-called “dangling bonds”. The surface layer is therefore at a substantially higher energy level than the bulk. A system tends to minimize its energy either by increasing the entropy of itself, or of its surroundings by the bond-formation heat. The surface area is therefore minimized to keep the amount of dangling bonds to a minimum. The force to minimize the area is proportional to the excess energy of the surface over the bulk. If high enough, it will compress the entire crystal. The interplay of the surface and bulk has consequences even for the crystal structure adopted. While tungsten metal is bcc (like Fe in Figure 1.23), its nanoclusters are ccp, with a face-centered cubic (fcc) unit cell, when they have fewer than 7000 atoms [10]. Why? Whereas the bcc packing of spheres ﬁlls ~68% of space, fcc ﬁlls ~74%. The space volume per atom is then smaller for fcc by a factor of 68/74. The same atoms would pack a smaller pﬃﬃﬃ fcc sphere, of surface smaller than bcc by a factor of about (68/74)2/3 = 0.945; exactly ð3=4Þ 3 2. As the proportion of the surface and of its higher energy content increases with decreasing size of our originally bcc nanoparticle, the energy that can be released by minimizing the surface eventually exceeds the energy needed to form the normally less favored but denser fcc tungsten packing in the bulk, hence the transition.

1.4.2 Filling Holes As suggested in the previous section, voids are left between spheres of the atomic densest packing. There are two types of voids in hcp and ccp arrangements; tetrahedral holes and octahedral holes (Figure 1.25). Four spheres surround a tetrahedral hole; three from one layer touching, one from the next. Six spheres surround an octahedral hole; three from one layer and three from the next. One octahedral and two tetrahedral holes are present per each sphere.

1.4

Structural Principles

23

Table 1.5 Binary-compound structure types derived by full or fractional ﬁlling of octahedral and tetrahedral holes in planes between closest-packed layers of A. Filling in total of holes

General formula

Structure type hcp of anions

Structure type ccp of anions

The plane-ﬁlling sequence

All octahedral ½ octahedral ½ octahedral ⅓ octahedral ⅓ octahedral ⅔ octahedral ⅔ octahedral All tetrahedral ½ tetrahedral All

CA CA2 CA2 CA3 CA3 C2A3 C2A3 C2A CA C3A

NiAs CdI2 CaCl2 BiI3 RuBr3

NaCl CdCl2

All full Empty and full All ½ full Empty and ⅔ full All ⅓ full Empty, full, full * All ⅔ full All full All ½ full All full

YCl3 La2O3

Al2O3 ** ZnS wurtzite Na3As

Li2O ZnS sphalerite

*Lanthanum ﬁlls the octahedral holes in a strongly off-center manner that provides bonding across the empty hole plane with one of the oxygen atoms, by which La achieves coordination number 7. **Repulsion of cations in the two face-sharing tetrahedra prevents this type of hole ﬁlling.

Figure 1.25 Tetrahedral and octahedral holes between layers of ccp and hcp spheres. Note that the label C of the subsequent ccp shifts is partly obscured.

Structures of many simple compounds can be described in terms of smaller atoms (usually cations) occupying the octahedral and/or tetrahedral holes in closest-packed arrangements of larger atoms (usually anions).17 Table 1.5 summarizes several structure types that can be described in this way. They are discussed in the following paragraphs. Let’s start a more detailed account by analyzing ﬁlling of octahedral holes in densest packed arrays. The two-step structure-orientation process is shown in Figure 1.26 for the respective prototypes, NiAs and NaCl. In both, the cation-occupied octahedral holes are 17

The closest-packed spheres (atoms) begin to touch once the radius of the atom in the octahedral holes becomes less than √2 − 1 ≈ 0.414 of the sphere radius. For tetrahedral holes this occurs when the radius of the smaller atom becomes less than (√3/√2) − 1 ≈ 0.225 of the closest-packed sphere radius. Hence these radius ratios are the minima for the given coordination to occur, at least in the hard-sphere approximation.

24

Structures of Crystalline Materials

Figure 1.26 The hcp and ccp prototypes NiAs (left) and NaCl (right). Identiﬁcation of octahedral holes (black) by reorienting the structure from a general view to the top-on view (below) and ﬁnally to the sideon view (above) of the closest-packed layers.

Figure 1.27 Coordination of octahedral holes in NiAs and NaCl structures.

located in the intermediate planes between the closest-packed layers of anion spheres, and the sphere stacking sequence is immediately recognizable. In NiAs, the closest-packed As atoms have six nearest Ni neighbors forming a trigonal prism (Ni[6o]As[6p]). In NaCl, both cation and anion arrays have the same arrangement in space and both are octahedrally coordinated; Na[6o]Cl[6o]. Either of them can therefore be considered closest packed, though this description better suits the larger Cl− anion. Figure 1.27 illustrates how the Ni coordination octahedra in NiAs share opposite faces (in addition to sharing all edges), whereas the octahedra in NaCl do not (only edges are shared). In strongly ionic compounds, the NaCl-type structure is therefore preferred over NiAs in order to avoid the added electrostatic repulsion across the shared octahedral face.

1.4

Structural Principles

25

Figure 1.28 Composition CA2 via ﬁlling octahedral holes in hcp: CdI2 (fully ﬁlling every second plane of holes) and CaCl2 (half ﬁlling every plane).

Composition CA2 with “cations” C in half the octahedral holes is achieved in two ways; either by alternating one empty and one ﬁlled plane of octahedral holes, or by half ﬁlling each plane (Table 1.5). Figure 1.28 compares these two arrangements in the hcp array; the alternately ﬁlled arrangement is called the CdI2 structure type18 and the homogeneously halfﬁlled one is the CaCl2 structure type.19 Note that the symmetry of the CaCl2 structure is reduced to orthorhombic by the rectangular pattern of holes. The alternating empty and ﬁlled octahedral planes create a layered structure because the anions face each other across each empty plane of octahedral holes.20 The polyhedral representation in Figure 1.29 top shows two types of such isolated layers; a CA2 layer that has all octahedral holes ﬁlled and a CA3 layer with two-thirds of the holes ﬁlled. Surprisingly, these two octahedral layers give rise to four structural arrangements. This is because each can stack in either an hcp or ccp array. The two-thirds ﬁlling of every plane of octahedral holes in hcp also occurs in the structure of corundum, Al2[6o]O3[4t], an important refractory material. Figure 1.30 shows this twothirds ﬁlling and how it subdivides the NiAs-type inﬁnite columns of octahedra into pairs. The two octahedra share one face and their central Al3+ cations repel each other due to the proximity of their ionic charges. Let’s now focus on ﬁlling tetrahedral holes. A complete ﬁlling of all the tetrahedral holes in a ccp array leads to the composition C2A of materials such as Li2O. However, the traditional

18 19

20

Perversely, CdI2 tends to adopt numerous stacking sequences rather than this simple hcp structure. The structure of rutile, TiO2, is related, but with anions distorted such that they no longer lie in perfect layers. TiO2 is then better understood in terms of corner- and edge-sharing octahedra (see Figure 1.45). The layers are held together by weak electrostatic forces of electric dipoles generated by random ﬂuctuation of the electronic charge in one object, such as the anionic layer, generating a corresponding inverse-charge ﬂuctuation in the other such object (van der Waals forces, see Section 5.1.3).

26

Structures of Crystalline Materials

Figure 1.29 Top: Polyhedral representation of a single layer of octahedral holes, fully occupied (left) and two-thirds occupied (right). Bottom: Structure types formed when these layers are packed such that their anions form a ccp or hcp array.

Figure 1.30 Sequence of octahedral-hole ﬁlling in hcp oxygens in corundum. The hole plane is two-thirds ﬁlled (left; every third hole is empty). All hole sequences in a straight line along c are full, full, empty (sideon view on right). The formed Al2[6]O3[4] has pairs of octahedra sharing faces, with repulsion of their central Al3+ ions.

1.4

Structural Principles

27

Figure 1.31 CaF2: Identiﬁcation of tetrahedral holes (black) in the side-on view of the ccp layer stacking of Ca atoms (gray large spheres). Notice a tetrahedral hole both above and below each densest-packed Ca atom, hence CaF2.

Figure 1.32 Identiﬁcation of tetrahedral-hole planes (black dots) in the side-on view of the hcp (left) and ccp (right) stacking of two ZnS modiﬁcations.

prototype structure used is CaF2,21 and has a cation ccp array with the ﬂuoride anions in all of the tetrahedral holes. Figure 1.31 illustrates its pattern of densest packing and hole ﬁlling. There are no known structures based on an hcp array with all the tetrahedral holes ﬁlled. This can be understood with reference to Figure 1.25 where the face sharing of tetrahedra would have the cations unreasonably close (closer than the cation–anion distance). The prototype structures based on ﬁlling half of the tetrahedral holes in hcp and ccp are the wurtzite and sphalerite (zinc blende) polymorphs of ZnS. Identiﬁcation of their sphere packing and hole ﬁlling is illustrated in Figure 1.32. Polyhedral coordination of the ﬁlled tetrahedral holes in unit cells of the prototype ccp and hcp structures is compared in Figure 1.33. More about building up structures from polyhedra is given in Section 1.4.4. Structures of some ordered metal alloys can be described as densest-packed arrays with ﬁlled holes. An example is the family of Heusler alloys that has a variety of important 21

Consequently, Li2O is considered an anti-ﬂuorite type.

28

Structures of Crystalline Materials

ZnS sphalerite

CaF2

ZnS

wurtzite

S Ca

S

Figure 1.33 Coordination of tetrahedral holes in CaF2, sphalerite, and wurtzite.

Figure 1.34 Unit cells of the XYZ and X2YZ Heusler alloys.

magnetic and electronic properties. Two closely related types form, XYZ and X2YZ, the former called half-Heusler alloys. Figure 1.34 shows that both are derived from a ccp of X atoms in which Y and Z occupy tetrahedral holes in an ordered manner, giving the XYZ structure. In the structure of X2YZ, the added X ﬁlls all octahedral holes.

1.4.3 Network Structures For many materials, the directional character of the chemical bonding around each atom in the structure is of prime importance. The most natural way to view such structures is to consider them as networks. This often helps to reveal the relationships and similarities among many simple structures. In more complex materials, the ﬁeld of coordination polymers (Chapter 14) has driven developments in the nomenclature [11, 12], taxonomy [13], and classiﬁcation [14] of networks. Here, we’ll consider only the most elementary terms. Networks with a single type of vertex are uninodal networks; all vertices are N-connected. An example of a 3-connected uninodal network is graphene (the single sheet of graphite, Figure 1.35), in which carbon forms three sigma bonds and the fourth valence electron is delocalized. Networks with low coordination numbers may be characterized by a vertex symbol [11]. The vertex symbol contains one post for each angle that occurs at the vertex. The post is

1.4

Structural Principles

29

Vertex symbol 616161 Three angles at the vertex, each angle is part of one 6-membered ring

Figure 1.35 A 3-connected uninodal network of graphene.

Figure 1.36 Two 3-connected networks of polysilicide anions in CaSi2 (puckered planar) and SrSi2 (3D). One 10-membered ring is highlighted with a dashed line.

a number with a subscript. The number gives the size of the smallest ring that a particular angle at the vertex is part of. The subscript identiﬁes how many rings are joined at this particular angle. As an example, the vertex symbol for graphene has three posts because there are three angles at the vertex. Each angle forms part of only one smallest, 6-membered, ring so the vertex symbol is 616161.22 Let’s consider the silicide anions in CaSi2 and SrSi2 as other examples of 3-connected networks. Using the generalized 8−N rule (Section 1.3.2), both compounds have VECA = 5, and the three missing electrons are obtained by forming three Si–Si single bonds at each Si. The net representing the silicide-anion network on the left of Figure 1.36 has the same vertex symbol 616161 as graphene, but differs in that it is puckered due to accommodation of one nonbonding electron pair at each Si. The standalone crystal-chemical formula for this anion 22

Following Wells, a symbol (6,3) is sometimes used for this honeycomb of 6-membered rings and 3-connected vertices. Do not confuse these Wells symbols with the N,M-connected binodal nets!

30

Structures of Crystalline Materials

Figure 1.37 Two 4-connected uninodal nets—cubic and hexagonal diamond.

would be 2∞ Si−, where the subscript and superscript to the left denote its inﬁnite 2D nature. The network in SrSi2 on the right of Figure 1.36 has vertex symbol 105105105. There are three angles at the vertex, and each angle is a part of ﬁve 10-membered rings in this 3∞ Si− 3D network.23 Examples of 4-connected nets are shown in Figure 1.37. Both concern elemental carbon forming uninodal nets of the vertex symbol 626262626262. The symbol has six posts because there are six angles at each tetrahedral vertex, where each angle is part of two 6-membered rings. For uninodal networks with higher connectivity, we have already encountered in Figure 1.23 the primitive cubic structure of polonium, which is a 6-connected network, and body-centered cubic α-Fe that can be considered as an 8-connected network. A binodal network has two different types of vertices. When characterized using the ½N; a ½M; An , two different vertices are seen, crystal-chemical formula for a binary phase, Ccþ m an N-connected vertex C and an M-connected vertex A. We say that a binodal network has an N,M-connected net. The relationship between uninodal and binodal nets is instructive for understanding similarities among structures. One type of network-based similarity is site ordering.24 In its simplest case, identical vertices of a uninodal network become occupied by two different atoms in an ordered manner, forming a binodal network. Three examples of this relationship are shown in Figure 1.38. Site ordering removes the equivalence of sites that were symmetry related, 23 24

The only 3-connected 3D network that has all three bonds and angles around the vertex equal. One of the homeotypical relationships between two structures deﬁned in ref. [2]. Another such homeotypism is the formation of distortion variants upon decrease in the space-group symmetry.

1.4

Structural Principles

31

Figure 1.38 Examples of site ordering of uninodal networks (top) to create binodal networks (bottom).

which means that the ordered structure, a superstructure, has a lower point symmetry (e.g. d3m to 43m; as in diamond to sphalerite in Figure 1.38), or translational symmetry (the unit cell is multiplied; as in Po to NaCl in Figure 1.38), or both. If the site ordering multiplies the original cell, the new cell is called a supercell. A second important relationship is network expansion where a linker is placed between a pair of vertices [11]. For example, we can take the diamond-type net of elemental silicon and put an oxygen atom mid-way between each node, obtaining the high-temperature structure of cristobalite, SiO2. This and other examples are shown in Figure 1.39 on the same set of uninodal nets as in Figure 1.38. The linker does not have to be a single atom; the primitive cubic 6-connected net expanded with a −C≡N− linker is the generic ingredient of the Prussian-blue-type structures. A ﬁnal relationship worth mentioning is vertex decoration—replacing a vertex with a group of vertices. When this group is a cluster, it is common to describe this as network augmenting [11]. An example is the relationship between CaTe and CaB6 in Figure 1.40. CaTe itself is an example of a material with the CsCl-type structure, which in turn can be considered as a site ordering of the α-Fe bcc array of Figure 1.23. Vertex decoration and network expansion may occur simultaneously. This is a good approach for visualizing open metal–organic frameworks (MOFs). The example in Figure 1.41 starts with oxygen atoms in a cubic Po-type network, which are “decorated” by zinc to [Zn4O]6+ and then linked with the terephthalate anion [O2CC6H4CO2]2−. This forms a ReO3type network of these cations and anions.

32

Structures of Crystalline Materials

Figure 1.39 Examples of network expansion from uninodal to binodal networks.

Figure 1.40 Decoration (augmenting) of anion sites in the CsCl-type structure.

In some cases, two interpenetrating nets run throughout a structure without ever crossing each other. Cu2O is one such example. In the right-hand side of Figure 1.42, we see two 2,4-connected nets of cristobalite type which never intersect. In each net, CuI adopts its preferred coordination number, 2, and oxygen is tetrahedrally coordinated, Cu2[2l]O[4t].

1.4.4 Polyhedral Structures In previous sections, we have seen various approaches that help visualize extended structures. In functional materials, however, the local chemistry is often the key to desired properties. Coordination polyhedra are an efﬁcient way to illustrate these local bonding environments, and, often, to visualize the entire structure. We’ll ﬁnd in Chapter 6 that focusing on coordination polyhedra is also a convenient start for developing electronic band-

1.4

Structural Principles

33

Figure 1.41 Combined site decoration and network expansion in a Zn4O(O2CC6H4CO2)3 MOF.

Cu O Cu2O

Cu

Å Wyck. 2a 4b

x 0

y 0

z 0

Figure 1.42 Two interpenetrated nets (one solid, one dashed) in cuprite, Cu2O.

structure ideas and understanding certain properties. In Section 1.5.4 and in Chapter 14, we’ll discuss how SiO4 tetrahedra are the essential building block of many silicate structures. Building from the ideas in Section 1.4.3, Table 1.6 contains examples of common coordcþ ½N; a ½M; ination polyhedra for the “cation” and “anion” in the Cm An compounds of binodal N,M-connected nets. Many of the structures that were earlier described as based on ﬁlling octahedral or tetrahedral holes are also found in this table. Given the chemical preference to form a certain coordination polyhedron, can we make any generalizations how such equal polyhedra connect into networks? Let’s take SiO2 as an

34

Structures of Crystalline Materials

Table 1.6 Common coordinations in some binodal N,M-connected nets.25 N,M

Cation coordination

Anion coordination

Example

4,2 4,3 4,3 4,4 4,4 4,4 6,2 6,3 6,4 6,6 6,6 8,4 8,8

Tetrahedron Tetrahedron Square Tetrahedron Square Square Octahedron Octahedron Octahedron Octahedron Octahedron Cube Cube

Linear (bent) Triangle Triangle Tetrahedron Tetrahedron Square Linear Triangle Tetrahedron Octahedron Trigonal prism Tetrahedron Cube

SiO2 (in quartz, cristobalite, tridymite) Si3N4 Pt3O4 ZnS (in zinc blende, wurtzite) PtS NbO ReO3 TiO2 (in rutile, anatase, brookite) Al2O3 (in corundum) NaCl NiAs CaF2 CsCl

example and assume tetrahedral coordination of Si. If both oxygens are equivalent, the coordination number of O will be 2 (see the connectivity-balance argument in Section 1.3.1), and the composition of this polyhedral network can be conveniently described as SiO4/2. This is an example of a Niggli formula, in which every polyhedral vertex is listed by its connectivity. Accordingly, SiO4/2 is a silicon dioxide with four 2-connected O vertices of the polyhedron around Si, meaning that each of the four oxygen vertices is shared with another tetrahedron to form a network of corner-sharing tetrahedra. When the vertices do not have the same connectivity, the subscript in the Niggli formula is written as a sum of fractions. Various connectivities can therefore be combined to give the same composition. SiO4/2, SiO3/3+1/1, and SiO2/4+1/2+1/1 all refer to SiO2 built of tetrahedra, but of different connectivities at the vertices.26 Yet, looking at known CA2 phases, we do not ﬁnd the latter two structures. Why? Sharing three or four tetrahedra at a common vertex is not prohibitive; we do ﬁnd 3-connected tetrahedra in Si3N4 (Niggli formula SiN4/3) or 4-connected tetrahedra in SiC (Niggli formula SiC4/4). Empirically, we can conclude that it is favorable for the oxygen vertices in SiO2 to have the same bonding environments. When an identical environment is not possible, atoms of the same element usually prefer their environments to be as similar as possible. This preference was postulated by Linus Pauling [3] as the rule of parsimony: “The number of essentially different kinds of constituents in a crystal tends to be small.” While this rule aids estimates of polyhedral connectivity in many compounds, does it predict the structure type? In general it does not; several possible spatial arrangements 25

26

Note that geometries may depart slightly from ideal depending on local site symmetry. Examples do not necessarily represent the only networks that can occur for a given N,M-connected net. SiO4/2 means four 2-connected vertices, SiO3/3+1/1 three 3-connected and one 1-connected vertex, and SiO2/4+1/2+1/1 two 4-connected, one 2-connected, and one 1-connected vertex in the tetrahedron.

1.4

Structural Principles

35

Figure 1.43 Structures made of 2-connected tetrahedral vertices.

usually exist. We can see this by considering just a few of the structural variants for the 4,2-connected binodal network of CA2 materials. Both the quartz and cristobalite structures contain corner-sharing tetrahedra but have different 3D arrangements. The OCu2 structure (Figure 1.43) is related to cristobalite, but more complex due to the interpenetration of two networks shown in Figure 1.42. The HgI2 structure also has vertices shared by two tetrahedra but is layered (Figure 1.43). Let’s consider next the structural possibilities for CA6 octahedra sharing vertices, common in functional materials. Starting with the highest n/m composition ratio for CmAn, CA6 in octahedral coordination represents an isolated octahedron. CA5 can be written as CA2/2+4/1 where there are two 2-connected and four 1-connected vertices.27 Such structures contain variously oriented inﬁnite corner-connected octahedral chains. CA4 requires four octahedral vertices shared (CA4/2+2/1), and various clustered chains, layers, or networks are possible, as illustrated in Figure 1.44. With all six vertices shared, we have formula CA3 (CA6/2) and the octahedral network found in ReO3 and ccp perovskites (Section 1.5.3). Other connectivity patterns are possible if we allow octahedra to share edges instead of just vertices. We’ve already encountered this in the YCl3/BiI3 structures of Figure 1.29, which contain octahedra that share three edges of six vertices shared by two octahedra each, giving again the Niggli formula CA6/2. As the n/m ratio decreases below three, the average anion coordination number must continue to increase, and shared edges become a necessity. There are several paths to composition CA2. The octahedra must share at least two edges, and the simplest way to do this yields the rutile structure of TiO2 that contains inﬁnite chains of octahedra sharing two opposite edges with the two remaining corners linking the chains together (Figure 1.45). The brookite and anatase polymorphs of TiO2 are other possibilities. In general, edge and face sharing is more frequent for octahedra than for tetrahedra. This is because shared edges between CA4 tetrahedra lead to very short distances between cations. Face-sharing tetrahedra are not known (we have already encountered the rule that only half 27

Two of six octahedral vertices are shared between two octahedra. Or, stated in the language of coordination chemistry, there are two bridging and four terminal ligand atoms.

36

Structures of Crystalline Materials

Figure 1.44 Examples of structures with identical octahedra sharing four vertices.

Figure 1.45 Edge- and corner-sharing octahedra in TiO2 modiﬁcations. Two unit cells are drawn for rutile and anatase.

1.4

Structural Principles

37

Box 1.3 Nanoscale Concepts: Polymorphism of TiO2 nanocrystals As the proportion of the crystal’s surface atoms versus bulk atoms increases towards the ultimate unity for the absolutely smallest cluster, the proportion of the surface’s higher energy content also increases. Consider TiO2 (Figure 1.45). The surface and bulk energies of its three modiﬁcations are as follows [15]: TiO2

Surface energy (J/m2)

Relative bulk energy (kJ/mol)

Anatase Brookite Rutile

0.4 1.0 2.2

2.6 0.7 0

Rutile has the most stable bulk, yet its surface has the highest energy (sharing fewest octahedral edges in its bulk yields the most dangling bonds at the surface). Below particle sizes of about 35 nm [16], the increasing surface-energy proportion destabilizes the normally stable rutile in favor of brookite. Below 11 nm [16], TiO2 adopts the anatase structure that shares all octahedral edges and has the fewest dangling bonds at the surface. In the opposite direction, this affects the crystallization of TiO2, as detailed below. Since crystals grow from their smallest seed (called the nucleus), TiO2 obtained by precipitation from an acidic TiCl4 solution is anatase (instantaneous formation, smallest crystallites). This complies with Ostwald’s step rule—the least stable polymorph often crystallizes ﬁrst [17]. The metastable anatase will turn into the stable rutile only after prolonged aging that allows the crystallites to join and recrystallize. The size and structure of nanoparticles synthesized from solutions depends on the extent of this aggregative growth, called Ostwald ripening, in which the tiniest crystals dissolve and regrow on the surface of larger crystals, ultimately minimizing the surface-energy proportion of the system.

of tetrahedral holes in an hcp can be ﬁlled). In contrast, face-sharing octahedra are found in NiAs (Figure 1.26), corundum (Figure 1.30), the hexagonal perovskites (Figure 1.54), and other structures. At least one coordination polyhedron exists for every coordination number. As the coordination number increases, several polyhedra become possible; such as the cube, square antiprism, and dodecadeltahedron for coordination number 8, or cuboctahedron, anticuboctahedron, and icosahedron for 12. However, upon further increase, the number of known structural examples quickly decreases. One of the highest coordination numbers occurs in the SmCo5-type structure of superferromagnets. Each Sm in this alloy is surrounded by 18 Co atoms that form a 6-capped hexagonal prism. The six capping Co atoms are 3-coordinated, and the twelve prismatic Co atoms are 4-coordinated, giving a Niggli formula SmCo6/3+12/4 (Figure 1.46).

38

Structures of Crystalline Materials

Figure 1.46 Polyhedral representation of the crystal structure of SmCo5.

1.5

Structures of Selected Materials

1.5.1 The Spinel Structure The mineral spinel, MgAl2O4, gives its name to a structure type in which two metals of similar atomic sizes are accommodated in tetrahedral and octahedral sites in a ccp array of anions. A simple formula to remember is [tetrahedron]1[octahedron]2O4. A detailed analysis reveals that one-eighth of the tetrahedral and a half of the octahedral ccp holes are occupied in a non-trivial stacking sequence. Table 1.7 illustrates the ubiquity of spinels. Two limiting types of site occupation occur. The ﬁrst is MgAl2O4 with each ion at its respective site, [Mg2+][4t][Al3+Al3+][6o]O4, termed a normal spinel. In the inverse spinel, half the octahedral ions are exchanged with the tetrahedron, as in magnetite [Fe3+][4t][Fe2+Fe3+][6o]O4. Magnetite forms an inverse spinel due to the ligand-ﬁeld stabilization energy (LFSE) of the high-spin d 6 Fe2+ being larger at octahedral than at tetrahedral sites, while high-spin d 5 Fe3+ has no LFSE. LFSE of d 8 Ni2+ makes [Ga3+][4t][Ni2+Ga3+][6o]O4 an inverse spinel, and LFSE of d 4 Mn3+ stabilizes normal spinel [Mn2+][4t][Mn3+Mn3+][6o]O4 with no LFSE from d 5 Mn2+. A spinel of similar ions of no LFSE may show an intersite disorder, such as [Mn2+1−xFe3+x][4t][Fe3+2−xMn2+x][6o]O4, depending in general on several size- and bonding-related factors. The connectivity of the cation coordination polyhedra in the spinel structure is hard to visualize, but one key feature is the network of edge-sharing octahedra (Figure 1.47, left). The visualization in Figure 1.47 right is useful for rationalizing the magnetic and electronic properties of spinels that are discussed in more detail in Chapters 9 and 11. Table 1.7 Oxidation-state combinations for spinels. Tetrahedron

Octahedron

Chemical formula of an example

1 2 2 3 4 5 6

3 3 4 2 2 1 1

LiMn2O4 (a = 8.245 Å) ZnFe2O4 (a = 8.442 Å) Fe2TiO4 (a = 8.521 Å) Fe3O4 (a = 8.394 Å) Ni2SiO4 (a = 8.045 Å) LiZnNbO4 (a = 6.082, c = 8.403 Å) Na2WO4 (a = 9.108 Å)

4 3 2 3 2 2 1

1.5

Structures of Selected Materials

39

Figure 1.47 Left: Coordination polyhedra of cations within the unit cell of spinel. Right: The unit-cell content in its simplest representation (the cubes are empty).

1.5.2 The Garnet Structure The garnet structure type is found in many important magnetic, optical, and magnetooptical materials. Many solid state lasers use yttrium aluminum garnet (YAG) doped with ~1% Nd as the active laser medium. Garnet is a complex, high-symmetry structure, and the simplest formula to remember is [cube]3[octahedron]2[tetrahedron]3O12. Table 1.8 shows that a variety of metal atoms can be accommodated at these sites. Intersite disorder is again common, particularly for garnet minerals like pyrope, Mg3Al2Si3O12, almandine, Fe3Al2Si3O12, and others. The crystal structure of garnet is not easy to visualize. The crystal-chemical formula together with a polyhedral illustration (Figure 1.48) provides some idea about coordinations and connectivities. The tetrahedra connect to octahedra by corner sharing, whereas three tetrahedral and all six octahedral edges are shared with the rather deformed cubes. As in spinel, all oxygens have a distorted tetrahedral coordination.

Table 1.8 Oxidation states in garnets [cube]3[octahedron]2[tetrahedron]3O12. Cube

Octahedron

Tetrahedron

Examples

2 3 2 1

6 3 3 3

2 3 4 5

Ca3Te2Zn3O12 a = 10.930 Å Y3Fe2Fe3O12 a = 12.376 Å Mg3Al2Si3O12 a = 11.459 Å Na3Sc2V3O12 a = 10.913 Å

40

Structures of Crystalline Materials

Figure 1.48 Coordination polyhedra in one-eighth of the garnet unit cell, which corresponds to a single formula unit.

1.5.3 Perovskite Structures The mineral perovskite, CaTiO3, lends its name to a vast family of structures where adjoined MX6/2 octahedra form 12-coordinated voids that can be ﬁlled by larger atoms A so that the composition becomes AMX3. Perovskites can also be viewed in terms of closest-packed AX3 layers in which M occupy one-quarter of the octahedral holes—those that are formed solely by X. Although ccp is most common, perovskites with hcp of AX3 layers are also known. Figure 1.49 illustrates the ccp case on an ideal cubic perovskite where M ﬁts the octahedral holes exactly.

Figure 1.49 Octahedral network in an ideal cubic perovskite (origin at A is chosen).

The ccp array will be more stable than hcp until the increasing size of A prevents the MX6/2 octahedra from linking at corners. On the other hand, much smaller A atoms than this maximum can be accommodated while keeping the corners linked. This can be evaluated with the Goldschmidt tolerance factor [18] (Figure 1.50) in terms of the ionic radii of A, M, and X. In particular, the Shannon radii [19] for 6-coordinated M, 12-coordinated A, and 2-coordinated O are consistent with Goldschmidt’s size considerations: Cubic perovskites, of ideal ratio of the AX and MX bond lengths AX/(MX√2) = 1 as in Figure 1.50, top left, are

1.5

Structures of Selected Materials

41

Figure 1.50 Tolerance factor t and two ways it can become smaller than unity.

stabilized over the t range ~1.04 to ~0.98 [20] by minor bonding compromises. When t ≳ 1.04, the hcp stacking is often observed. In the t range between ~0.99 and ~0.83, perovskites are stabilized by structural distortions as discussed below. Figure 1.50 illustrates two scenarios for t < 1: either it is due to M being too large and expanding the MX6 octahedron, or due to A being too small so that A and X are no longer in contact. The drawing shows that both cases effectively mean that the A atom is smaller than one that would ﬁt exactly. The structure responds to this size mismatch by a coupled rotation of the corner-linked MX6/2 octahedra, which expands them in a ﬁxed frame of constant unit cell, accommodating the large M and bringing X closer to A. This octahedral tilting can profoundly inﬂuence the magnetic and electronic properties of perovskites. While symmetry analysis [21, 22] is the most rigorous approach to describe the various types of tilting, a simple combinatorics of these coupled rotations is the basis for the Glazer tilt classiﬁcation [23]. It considers a model of linked octahedra and evaluates all combinations of rotations along the three 4-fold axes of the octahedron in Figure 1.51. In the network, twisting the central octahedron anticlockwise mechanically requires its in-plane neighbors to twist clockwise in a cooperative manner. The plane of octahedra below the one under consideration, however, is free to rotate in either the same or the opposite sense. Let’s start with the simplest case of no rotation at all. It is given a three-letter symbol a0a0a0 because equal rotations about different axes of the octahedron are symbolized by use of the same letters. A uniaxial rotation is then denoted with “c” as the last letter (a0a0c+ and a0a0c− in Figure 1.51) where superscripts + or − specify whether the octahedra in adjacent layers rotate in the same direction (+, in phase) or in opposite direction (−, out of phase). For biaxial rotation of the octahedron, the letter “b” is added with a superscript sign, such as in

42

Structures of Crystalline Materials

a⁰ a⁰ c+

a⁰ a⁰ c–

Figure 1.51 Octahedron can rotate about each of its fourfold axes (center). Uniaxial rotations: In-phase between successive planes (left), out-of-phase (right).

a0b+c+ (two unequal rotations in phase), for triaxial rotation all three letters have superscript signs, such as in a+b+c+ (three unequal rotations in phase). Since for equal rotations about different axes the same letter is used, we may have a0b+b+ (two equal rotations in phase) or a−a−b+ (two equal rotations out of phase) or a+a+a+ (three equal rotations in phase). In total, this combinatorics yields 23 Glazer tilt systems in ref. [23]. Symmetry analysis [21] shows that there are 15 unique Glazer tilts28 (some tilts also do not form), but three are particularly frequent [24]. One of them is a0a0a0 for the cubic perovskite of Pm3m symmetry. SrTiO3 is one of many examples. Another frequent tilt is a−a−a−, which lowers the symmetry to rhombohedral, R3c. This tilt is equivalent to a single rotation of an octahedron around its threefold axis. Figure 1.52 shows this rotation for LaNiO3 and views of the structure along all three 4-fold axes of the octahedron. These three projections illustrate that all three tilts are equal and out of phase. The high symmetry extends to the coordination polyhedra, fulﬁlling Pauling’s parsimony rule and providing the most favorable ionic bonding of all tilted perovskites. This becomes important as the charge number of the A cation increases. The effect this tilt has on the A-atom coordination is to bring three of the twelve X atoms closer to A while moving three others away, hence approaching the coordination number 9. As the progressing rotation contracts only three of these nine A–X bonds, the range is limited, and the a−a−a− tilting is rare when t < 0.97. The most common tilt is a+b−b− that lowers the symmetry to orthorhombic Pnma. It again accommodates the smaller-than-optimal atom A by bringing some of the twelve X neighbors closer to increase their bond strength more than the rest of them lose it (Section 5.4). An example in Figure 1.53 is LaFeO3, where La has eight close O neighbors and the remaining four at a longer distance. Unlike a−a−a−, this tilt allows A to deviate from the center of its coordination polyhedron and is therefore prevalent among perovskites with t < 0.97. 28

The reduction from 23 to 15 tilts can be understood by careful consideration of the relationship between symmetry elements and the magnitude of the tilts imposed by Glazer’s notation. The number of unique tilts drops from 23 to 17 upon realizing that symmetry cannot restrain tilts of a different sense (in-phase versus out-of-phase) to be of the same magnitude. As an example, a+a−a− has the same symmetry as a+b−b−, and the latter thus covers both cases. Even if you forced the in-phase tilt to be of equal magnitude to the out-of-phase tilts, there would be no symmetry element that constrained it to be equal, hence, in a real crystal, it would never be more than approximately equal. For a full explanation of how symmetry reduces the number of allowed tilt systems, see ref. [21].

1.5

Structures of Selected Materials

43

Figure 1.52 Rotation of Glazer’s tilt a−a−a−. The actual physical rotation of eight corner-linked octahedra as viewed looking down the threefold axis (top right) and as separated into rotations around the three tilt axes of the octahedron (bottom).

Figure 1.53 Glazer’s tilt a+b−b−. The octahedron rotates around all three of its axes, in phase around one axis and out of phase around the remaining two.

44

Structures of Crystalline Materials

Figure 1.54 Left: Comparison of ccp perovskite with a polytype of (hc)2 stacking sequence. Right: The 4H BaMnO3 phase as an example of the latter.

Perovskites with hcp packing of AX3 layers are less common, because the ABAB layer repetition means that the MX6/2 octahedra share faces, forming columns. In between these columns there is a lot of space to accommodate large soft A atoms such as barium. These socalled hexagonal perovskites are therefore formed when the Goldschmidt tolerance factor t increases signiﬁcantly over 1, that is, when the A cation is too large for its site. Initially, ordered intergrowths of ccp with hcp occur. Figure 1.54 gives an example of 4H BaMnO3 (t = 1.11) that alternates ccp and hcp sequences. A completely hexagonal stacking is found for BaNiO3, with t of 1.13, the structure of which contains inﬁnite columns of face-sharing octahedra. The compositional variety of perovskites is extremely rich. Table 1.9 shows examples of cubic AMX3 perovskite-type structures for diverse oxidation-state combinations. At the bottom of the table, the anti-perovskites even contain a large cation at the X site. Several perovskites have the A site vacant; ReO3 (our cover star) is cubic while the related WO3 has its WO6/2 octahedra tilted and distorted.

1.5.4 Silicates Silicates are multicomponent oxides based on silicon–oxygen frameworks made up of predominantly corner-sharing tetrahedra. Silicon in these tetrahedra may in part be replaced

1.5

Structures of Selected Materials

45

Table 1.9 Oxidation-state combinations for AMX3 perovskites. A

M

X

Examples (cubic or nearly cubic chosen)

+4 +3 +2 +1

+5 +3 +4 +5 +6 +1 +2 +3 −2 −3 −2

−3 −2 −2 −2 −2 −1 −1 −1 +1 +2 +2

ThTaN3 a = 4.02 Å LaAlO3 a = 3.82 Å SrTiO3 a = 3.90 Å CsIO3 a = 4.67 Å □ReO3 a = 3.73 Å BaLiF3 a = 4.00 Å, BaLiH3 a = 4.02 Å KMgF3 a = 3.97 Å, (CH3NH3)PbBr3 a = 5.93 Å □ScF3 a = 4.00 Å AuORb3 a = 5.50 Å, ISAg3 a = 4.90 Å SbNCa3 a = 4.85 Å, AuNCa3 a = 4.82 Å GeOCa3 a = 4.73 Å

+2 +1 −1 −3 −4

by a neighboring element, typically aluminum. Very few silicates contain Si in octahedral coordination,29 very few feature edge-sharing tetrahedra, and the oxygen vertices are generally 2-coordinated. Silicates are the most common minerals in the Earth’s crust and represent about one-third of known inorganic crystal structure types. Although some crystalline silicates, in particular zeolites, have use as functional materials, silicate materials ﬁnd applications predominantly due to their mechanical properties. The oldest examples of artiﬁcial composite materials are silicates such as porcelain, the exquisite properties of which are caused by a texture of ﬁbrous crystals embedded in a glassy matrix. It’s impossible to cover the vast array of silicate structures here; instead we’ll focus on simple ideas and nomenclature in common use. We’ve already seen one way of understanding silicate structures in Section 1.4.3, where we described how the cristobalite modiﬁcation of SiO2 is derived via expanding the cubic-diamond network of Si and the how the tridymite modiﬁcation of SiO2 is derived from lonsdaleite. Along this line of thinking, replacement of every second Si in cristobalite with Al and compensation of the thus-formed negative charge by placing Na+ into the cavities in the tetrahedral network leads to carnegieite NaAlSiO4. In a similar way, tridymite can be expanded to the structure of nepheline (Figure 1.55). Such homeotypism occurs also between the quartz modiﬁcation of SiO2 and β-eucryptite, LiAlSiO4, which is a low-expansion material commonly used as a catalyst support in car exhausts. The coarsest chemical categorization of silicate anions is based on the network dimensionality. Silicates are classiﬁed as oligo- and cyclo- for ﬁnite polyanions, catena- for chains, phyllo- for layered anions, and the general name of tectosilicates is used for 3D networks.30 Examples of 1D and 2D networks are in Figure 1.56. Their chemical compositions can be determined from 29 30

Common only at high pressure in phases such as MgSiO3. From Greek, “olígos” few, “phýllo” leaf, “tekton” builder; and Latin, “catena” chain.

46

Structures of Crystalline Materials

Figure 1.55 Homeotypism between tridymite and nepheline.

Figure 1.56 Examples of cyclo silicate, catena silicate, and phyllosilicate anions.

the vertex connectivities with Niggli formulas. As an example, all the anions in the top row of Figure 1.56 have the same elemental composition. All have silicon coordination tetrahedra with two terminal and two shared oxygens, (SiO2+2/2)2–. It is clear that, for inﬁnite polyanions, neither the chemical formula nor the chemical name is very informative of the structural arrangement. A more detailed and informative nomenclature is given in Appendix C.

1.5.5 Zeolites From the discussion above, it should be clear that the connected tetrahedra in silicates may form an almost inﬁnite number of shapes. One technologically important subgroup of tectosilicates is the zeolites. Zeolites contain interconnected cages made of SiO4/2 and AlO4/2 tetrahedra, with pores in between them where guest ions, atoms, or molecules can be accommodated. Materials with pores of 2.5–20 Å in diameter are referred to as microporous, those with sizes 20–500 Å, mesoporous. Owing to the ease with which non-framework chemical species can be exchanged on the large inner surface area, zeolite properties can be

1.5

Structures of Selected Materials

47

Figure 1.57 Graphical representations of the alumosilicate cages in sodalite.

tuned to ﬁt many technological applications (discussed in Chapter 14). One common zeolite cage is the sodalite cage, built from 24 tetrahedra as shown in Figure 1.57. The visualization of the interconnected zeolite cages is greatly simpliﬁed by omitting the tetrahedra and connecting only their central atoms with a straight line (removing O atoms, the inverse of network expansion). The connectivity of the cages is accomplished by sharing (Figure 1.57) or by connecting their equivalent faces. When all square faces of the sodalite cage are shared at the Si atom with other sodalite cages, the sodalite structure is formed and contains small pores that do not qualify as micropores. However, when all square faces of sodalite cages are connected via Si–O–Si bonds, forming a neck between the cages, the so-called zeolite A is obtained. When four of the eight hexagonal faces of the sodalite cage are connected to other sodalite cages, zeolite X/Y (faujasite) is formed (Figure 14.2). Owing to important industrial applications, a zeolite nomenclature [25] has been adopted by the International Union of Pure and Applied Chemistry (IUPAC).

1.5.6 Zintl Phases Zintl phases are compounds of two elements one would consider as metals or semimetals (typically an alkali or alkaline-earth metal and a post-transition metal). Unlike conventional alloys and intermetallics, Zintl phases have ﬁxed stoichiometry and physical properties that are atypical for a metal. They are diamagnetic, brittle, and exhibit low electrical conductivity. Their composition follows the Zintl–Klemm concept of the more electropositive metal behaving as a cation that provides electrons for the more electronegative metal to form polyanions in which electrons are shared to complete the octet [26]. The composition can thus be treated by the generalized 8−N rule of Section 1.3.2. As an example, although we normally think of thallium as an electropositive metal, it forms a Zintl phase NaTl with the even more electropositive Na. Because VECA = 4, four electrons per Tl must be shared,

48

Structures of Crystalline Materials

Figure 1.58 The Zintl phases NaTl and SrGa2 with VECA = 4 and AA = 4 form anion networks that are electronically and structurally related to diamond and graphite.

Figure 1.59 Zintl phases KGe and CaSi with anions isoelectronic to elemental nonmetals.

forming four two-electron Tl–Tl bonds at each Tl. Indeed, the crystal structure in Figure 1.58 has a polyanion network 3∞ Tl− analogous to diamond. Similarly, for SrGa2 (Figure 1.58), VECA = 4 and four electrons per Ga are shared—three in single bonds, one via conjugation as in graphite. The crystal-chemical formula of the anion is 2∞ Ga−. In KGe, VECA = 5, and three two-electron bonds per Ge are formed (Figure 1.59). In the crystal structure of KGe, germanium occurs in Ge44− cages isoelectronic with molecules of white phosphorus. Another example is CaSi, where VECA = 6, suggesting two two-electron bonds per Si (Figure 1.59). In the crystal structure of CaSi, silicon forms polyanion chains 1∞ Si2−, isoelectronic with the ﬁbrous modiﬁcation of elemental sulfur, and similar to the structure of tellurium shown in Figure 1.16.

1.6

Problems (Note that some require a structure-drawing program.) 1.1 Write down the ⟨111⟩ set of symmetry-equivalent directions in a cubic lattice.

1.6

Problems

49

1.2 By analogy with Table 1.1, determine the number and type of 2D crystal systems via considering their possible minimum symmetry elements and sketching their Bravais lattices. 1.3 Write down indices for the following sets of equidistant planes:

c

c

b a

c

b a

c

b a

b a

1.4 Sketch a set of equidistant 113 planes in a cubic unit cell. 1.5 Sketch a set of equidistant 113 planes in a cubic unit cell. 1.6 State the Bravais lattice and write down the crystallographic point-group symbol for a structure of space-group symbol: (a) C2/m, (b) Fmm2, (c) I4/mmm, (d) P312, (e) R3m, (f) P6m2, (g) F23, (h) P213, (i) Ia3d. 1.7 Is it possible for a c glide plane to have the direction of: (a) a axis, (b) b axis, (c) c axis? If not, why is this not allowed? 1.8 Write down crystal-chemical formulas for two-site binary compounds CrN, Cr2O3, and CrO2 with octahedrally coordinated chromium. 1.9 Write down the three balances expressed in the crystal-chemical formulas of the phases in the previous problem. 1.10 Draw the bond graph for the mineral spinel MgAl2O4 (Figure 1.47). 1.11 Convert the bond graphs in Figure 1.15 into crystal-chemical formulas. 1.12 Describe or sketch a structure for layered V2O5 that is consistent with the bond-graph representation in Figure 1.15. 1.13 Use the generalized 8−N rule to identify whether anion–anion or cation–cation bonds are present for the following compounds (assume no cation-localized nonbonding electron pairs): (a) Na2Tl, (b) SrSb2, (c) BaTe2, (d) InSe. 1.14 Suggest the anion bonding that might occur in MgB2 and MgC2. 1.15 Calculate the percentage of available space that’s taken up by touching spheres in primitive and body-centered cubic arrangements. 1.16 Imagine a coordination polyhedron with a cation at the center. Now treat the ions as hard spheres and reduce the size of the cation until the anions just touch. What is the radius r of the cation for anions of unit radius in the following coordinations: (a) cube, (b) octahedron, and (c) tetrahedron. Hint: Body diagonal is √3 and face diagonal √2 times the cube edge. 1.17 From unit-cell parameters in ﬁgures in this chapter, calculate the following shortest distances: (a) Na–Cl and Na–Na in NaCl, (b) Ni–Ni in NiAs, (c) Ca–F in CaF2,

50

Structures of Crystalline Materials

1.18

1.19 1.20

1.21

1.22 1.23

1.24

1.25 1.26 1.27 1.28

1.29 1.30

(d) C–C in diamond, (e) Ti–Ti in TiO2 (rutile), and (f) Ti–O, Sr–O, and O–O in the cubic perovskite SrTiO3 (a = 3.90 Å). With a structure-drawing program, determine the stacking sequence in Tb (data for plotting, see Section 1.1.8: P63/mmc, a = 3.068, c = 14.87 Å, Tb in 2b at 0 0 ¼ and 4f at ⅓ ⅔ 0.083). Suggest the Ramsdell symbol and the Jagodzinski–Wyckoff notation. Determine the stacking sequence of Br in trigonal CdBr2 (R3m in hexagonal setting; a = 3.965, c = 18.70 Å, Cd in 3a at 0 0 0, Br in 6c at 0 0 0.25). In the low-temperature form of CrCl3, every second plane of octahedral holes is occupied. What is the ﬁlling fraction of the occupied planes? Check the result by a sideon view of the closest-packed layers perpendicular to their subsequent shifts (R3 in hexagonal setting; a = 5.94, c = 17.3 Å, Cr in 6c at 0 0 ⅓, Cl in 18f at ⅔ 0 0.0757). What is the type of densest packing? La in solid LaBr3 has a tricapped trigonal-prismatic coordination. What is the coordination number of Br? Is it possible that the tricapped trigonal prisms share only corners, or would you expect sharing of edges and/or faces? Check the result by viewing the structure and constructing polyhedra around La (P63/m, a = 7.971, c = 4.522 Å. La in 2c at ⅓ ⅔ ¼, Br in 6h at 0.3849 0.2988 ¼). Write the Niggli formula and the simple crystal-chemical formula for the CrO3 structure that contains chains of corner-sharing chromium-centered tetrahedra. Construct a bond graph or Niggli formula to determine if it is possible for all anions to be equivalent in a structure of tetrahedrally coordinated cations and stoichiometry of C2A3? Which alternative Niggli formula complies best with the rule of parsimony? Using the Niggli formula and the rule of parsimony, determine the stoichiometry that results from sharing (a) all corners, (b) all edges, and (c) all faces of a cation-centered cube of anions. Note the structure prototype where you recognize it. Write the Niggli formula for C3N4 made of identical CN4 tetrahedra. How many different types of nitrogen vertices are there? What is the coordination number of each? In β-Li3N, nitrogen is 11-coordinated. Write down the Niggli formula of the NLi3 polyhedron. ReO3 has a 3D network of octahedrally coordinated rhenium. Determine the N, M-connectivity for this binodal network Identify the type of derivative network relationship between: (a) CaO (Fm3m, a = 4.778 Å, O in 4a at 0 0 0, Ca in 4b at ½ ½ ½) and CaO2 (I4/mmm, a = 3.56 Å, c = 5.95 Å, Ca in 2a at 0 0 0, O in 4e at 0 0 0.394), (b) SrMoO3 (Pm3m, a = 3.965 Å, Sr in 1b at ½ ½ ½, Mo in 1a at 0 0 0, O in 3d at ½ 0 0) and the high-temperature Sr2FeMoO6 phase (Fm3m, a = 7.93 Å, Sr in 8c at ¼ ¼ ¼, Mo in 4b at ½ ½ ½, Fe in 4a at 0 0 0, O in 24e at 0.253 0 0). Which type of similarity do you see between the Laves phase MgCu2 (Fd3m, a = 7.034 Å, Mg in 8a at 0 0 0, Cu in 16d at ⅝ ⅝ ⅝) and the spinel in Figure 1.47? Rewrite the chemical formulas in Table 1.7 into simpliﬁed crystal-chemical formulas of spinel.

1.8

References

51

1.31 Analyze hole ﬁlling in the spinel structure of ccp oxygens. (a) Given the general formula [tetrahedron]1[octahedron]2O4, calculate the total fractions of tetrahedral and octahedral holes ﬁlled. (b) Use a structure-drawing program to orient the structure and identify the type of ﬁlled holes between layers of densely packed oxygen atoms. (c) Determine the sequence and the fraction of each hole ﬁlling. 1.32 With a structure-drawing program, determine which of the three most common tilts the perovskite prototype CaTiO3 (ICSD 62149) adopts. 1.33 Give the Niggli formula for a cyclosilicate anion containing 3 Si. 1.34 What is the formula of the inﬁnite alumosilicate anion in sodalite? 1.35 Use VECA modiﬁed for the stable 18-electron conﬁguration of Kr to justify the network of Cu tetrahedra in MgCu2. 1.36 Suggest the bonding present in the Zintl phase LiAs. 1.37 Suggest the bonding present in the Zintl phase KIn. 1.38 Suggest the bonding present in the Zintl phase CaIn2. Verify your suggestions with the ICSD and a structure-drawing program.

1.7

Further Reading A.F. Wells, “Structural Inorganic Chemistry” (1984) Oxford University Press. B.G. Hyde, S. Andersson, “Inorganic Crystal Structures” (1989) Wiley. F.A. Cotton, “Chemical Applications of Group Theory” (1990) Wiley. G. Burns, A.M. Glazer, “Space Groups for Solid State Scientists” 2nd edition (1990) Academic Press. M. O’Keeffe, B.G. Hyde, “Crystal Structures I: Patterns and Symmetry” (1996) Mineralogical Society of America. A. Vincent, “Molecular Symmetry and Group Theory” (2001) Wiley. R. Tilley, “Crystals and Crystal Structures” (2006) Wiley. U. Müller, “Inorganic Structural Chemistry” 2nd edition (2007) Wiley. M. de Graef, M.E. McHenry, “Structure of Materials: An Introduction to Crystallography, Diffraction and Symmetry” (2007) Cambridge University Press. C. Giacovazzo, H.L. Monaco, G. Artioli, D. Viterbo, M. Milaneso, G. Ferraris, G. Gilli, P. Gilli, G. Zanotti, M. Catti, “Fundamentals of Crystallography” 3rd edition (2011) IUCr/Oxford University Press. U. Müller, “Symmetry Relationships between Crystal Structures” (2013) IUCr/Oxford University Press.

1.8

References [1] J. Foadi, G. Evans, “On the allowed values for the triclinic unit-cell angles” Acta Crystallogr. Sect. A 67 (2011), 93–95.

52

Structures of Crystalline Materials

[2] J. Lima de Faria, E. Hellner, F. Liebau, E. Makovický, E. Parthé, “Nomenclature of inorganic structure types” Acta Crystallogr. Sect. A 46 (1990), 1–11. [3] L. Pauling, “The principles determining the structure of complex ionic crystals” J. Am. Chem. Soc. 51 (1929), 1010–1026. [4] D. Fisher, M. Jansen, “Synthesis and structure of Na3N” Angew. Chem. Int. Ed. Engl. 41 (2002), 1755–1756. [5] M. O’Keeffe, B.G. Hyde, “Stoichiometry and the structure and stability of inorganic solids” Nature 309 (1984), 411–414. [6] A. Kjekshus, “The general (8-N) rule and its relationship to the octet rule” Acta Chem. Scand. 18 (1964), 2379–2384, and references therein. [7] E. Parthé, “Valence-electron concentration rules and diagrams for diamagnetic, nonmetallic ion covalent compounds with tetrahedrally coordinated anions” Acta Crystallogr. 29 (1973), 2808–2815. [8] J. Kepler, “Strena seu de nive sexangula” Godfried Tambach, Frankfurt am Main (1611). [9] P.N.H. Nakashima, A.E. Smith, J. Etheridge, B.C. Muddle, “The bonding electron density in aluminum” Science 331 (2011), 1583–1586. [10] H.K. Kim, S.H. Huh, J.W. Park, J.W. Jeong, G.H. Lee, “The cluster size dependence of thermal stabilities of both molybdenum and tungsten nanoclusters” Chem. Phys. Lett. 354 (2002), 165–172. [11] M. O’Keeffe, M. Eddaoudi, H. Li, T. Reineke, O.M. Yaghi, “Frameworks for extended solids: geometrical design principles” J. Solid State Chem. 152 (2000), 3–20. [12] V.A. Blatov, M. O’Keeffe, D.M. Proserpio, “Vertex-, face-, Schläﬂi-, and Delaney symbols in nets, polyhedra and tilings: recommended terminology” CrystEngComm 12 (2010), 44–48. [13] O. Delgado-Friedrichs, M. O’Keeffe, O.M. Yaghi, “Taxonomy of periodic nets and the design of materials” Phys. Chem. Chem. Phys. 9 (2007), 1035–1043. [14] O. Delgado-Friedrichs, M.D. Foster, M. O’Keeffe, D.M. Proserpio, M.M.J. Treacy, O.M. Yaghi, “What do we know about three-periodic nets?” J. Solid State Chem. 178 (2005), 2533–2554. [15] M.R. Ranade, A. Nawrotsky, H.Z. Zhang, J.F. Banﬁeld, S.H. Elder, A. Zaban, P.H. Borse, S.K. Kulkarni, G.S. Doran, H.J. Whitﬁeld, “Energetics of nanocrystalline TiO2” Proc. Natl. Acad. Sci. USA 99 (2002), 6476–6481. [16] H. Zhang, J.F. Banﬁeld, “Understanding polymorphic phase transformation behavior during growth of nanocrystalline aggregates: insights from TiO2” J. Phys. Chem. B 104 (2000), 3481–3487. [17] W. Ostwald, “Studien über die Bildung und Umwandlung fester Körper. 1. Abhandlung: Übersättigung und Überkaltung” Z. Physik. Chem. 22 (1897), 289–330. [18] V.M. Goldschmidt, “Laws of crystal chemistry” Naturvissenschaften 14 (1926), 477–485. [19] R.D. Shannon, “Revised effective ionic radii and systematic studies of interatomic distances in halides and chalcogenides” Acta Crystallogr. Sect. A 32 (1976), 751–767. [20] M.W. Lufaso, P.M. Woodward, “Predictions of the crystal structures of perovskites using the software program SPuDS” Acta Crystallogr. Sect. B 57 (2001), 725–738. [21] C.J. Howard, H.T. Stokes, “Group theoretical analysis of octahedral tilting in perovskites” Acta Crystallogr. Sect. B 54 (1998), 782–789. [22] D. Wang, R.J. Angel, “Octahedral tilts, symmetry-adapted displacive modes and polyhedral volume ratios in perovskite structures” Acta Crystallogr. Sect. B 67 (2011), 302–314.

1.8

References

53

[23] A.M. Glazer, “Classiﬁcation of tilted octahedra in perovskites” Acta Crystallogr. Sect. B 28 (1972), 3384–3392. [24] P.M. Woodward, “Octahedral tilting in perovskites. II. Structure stabilizing forces” Acta Crystallogr. Sect. B 53 (1997), 44–66. [25] L.B. McCusker, F. Liebau, G. Engelhardt, “Nomenclature of structural and compositional characteristics of ordered microporous and mesoporous materials with inorganic hosts” Pure Appl. Chem. 73 (2001), 381–394. [26] E. Zintl, “Intermetallische Verbindungen” Angew. Chem. 52 (1939), 1–6.

2

Defects and More Complex Structures

We have seen in Chapter 1 that the solid state world is dominated by long-range order and beauty. Crystalline materials contain highly symmetric arrangements of atoms that are regularly repeated over millions of unit cells. In this chapter, we will question how realistic this picture is. In reality, there are a number of ways in which crystalline materials deviate from perfect long-range order and contain imperfections or disorder. This can occur via “mistakes” in the atomic arrangement of a pure material or via the introduction of impurity atoms giving rise to chemical disorder. These defects can occur locally or extend over lines, planes, or 3D volumes of materials. Such effects, even when they occur at very low levels, are vitally important to the chemical and physical properties of materials. They turn low-value minerals into precious gemstones; soft iron into strong and corrosion-resistant stainless steel; and they control the semiconducting properties of silicon in the transistors powering modern electronics. This chapter also introduces a variety of ways in which materials can deviate from having simple stoichiometric formulae. This can occur either via the presence of defects or chemical substitutions in a material or can have a variety of more complex structural origins. In later chapters, we will see how these various effects inﬂuence many of the important properties of functional materials.

2.1

Point Defects in Crystalline Elemental Solids We have seen that the structures of many elements can be described in terms of regular arrays of spherical atoms. At the local level, this order can be perturbed by three different types of point defects; vacancies, interstitials, and substitutional disorder. These are shown schematically in Figure 2.1. A vacancy occurs when an atom is missing from a site in the structure as shown in Figure 2.1, left. An interstitial defect occurs when an extra atom sits in a site that would not normally be occupied. An interstitial site can be occupied either by an atom of the same type that

54

2.2

vacancy

Intrinsic Point Defects in Compounds

interstitial

55

substitution

Figure 2.1 Different types of point defects.

makes up the structure, or by an impurity atom. It is common, for example, for small nonmetallic elements such as C, N, O, and H to occupy a fraction of interstitial positions in the structures of transition metals. Such materials can be of great technological importance: C interstitials in iron greatly increase its mechanical strength; and Pd can store around 0.6% by mass of H interstitials, which is of interest for hydrogen storage (see Box 2.1). The third common type of defect is substitutional disorder where a foreign atom adopts a site in the structure of a pure element. At low levels, foreign aliovalent1 atoms are frequently referred to as dopants and can signiﬁcantly alter chemical (Chapter 3), electronic (Chapters 6 and 10), and optical (Chapter 7) properties of a material. Doping silicon with low levels of Al or P, for example, leads to the formation of p- or n-type semiconductors, respectively. At higher levels of doping, one typically refers to solid-solution or alloy formation. This process can again be used to tailor a material’s properties. Real materials exist with any one of these basic types of defects or with various combinations of them.

2.2

Intrinsic Point Defects in Compounds Similar defects to those depicted in Figure 2.1 for elements can occur in ionic compounds,2 though with the additional constraint that one must maintain overall electrical neutrality in the crystal. If, for example, one simply removed an Na+ ion from a compound such as NaCl to create a defect, the crystal would end up with a negative charge. Defects in ionic compounds can only occur in ways that avoid such charge build-up. Defects that can occur in pure compounds are called intrinsic defects. A Schottky defect is a cation vacancy compensated by an appropriate number of anion vacancies (Figure 2.2), i.e. it is a missing formula unit. For a binary phase MX, the number of vacancies on cation and anion sites will be equal; for MX2, two X− anion vacancies would be needed for every M2+ vacancy. In terms of ionic charges, removing M+ 1 2

Of different valence or oxidation state to the atom it replaces; isovalent means of the same valence. Our discussion in this chapter will largely be in terms of formal ionic charges in materials. This need not, of course, imply that ionic bonding is actually dominant.

56

Defects and More Complex Structures

Box 2.1 Materials Spotlight: Hydrogen-storage materials Efﬁcient energy production, storage, and use is one of the major challenges facing the modern world. Both developed and developing economies are heavily reliant on fossil fuels in all areas of energy use. Fossil fuels are limited in supply and polluting when burnt. One alternative fuel under consideration for automotive applications is hydrogen, which produces benign H2O. Safe and efﬁcient storage of H2 is a major issue [1, 2]. H2 is gaseous at temperatures above 20.3 K and while its heat of combustion per unit mass is high compared to other fuels (H2 120 MJ/kg, gasoline 44.5 MJ/kg) the value per unit volume is low: at standard conditions, hydrogen gas has ΔHcomb = 9.6 kJ/L and even as a liquid ΔHcomb = 8.4 MJ/L compared to 31.2 MJ/L for gasoline. For automotive use, the US Department of Energy state speciﬁc targets of a gravimetric energy density of 7.9 MJ/kg (2.2 kW h), corresponding to 6.6 wt% H2, and a volumetric energy density of 6.1 MJ/L at the time of writing. In addition, the fuel storage in a car needs to be reversible (~1000 times) and allow refueling in 3 minutes—signiﬁcant challenges! One possibility is to store H2 as a high-pressure gas or as a liquid at 20 K. It costs about 15% of the energy content to pressurize H2 to 700 bar or about 20% to liquefy it (plus around 2% per day to keep it cold). For these and other technological reasons, high-pressure seems the more viable storage solution. Chemical solutions to the H2 storage problem can be divided into two main categories— those that rely on chemisorption and formation of chemical bonds, and those that rely on physisorption of H2. In the chemisorption case, the stability of the compounds formed means that a key challenge is to provide materials that decompose to release H2 at a low enough temperature (below approximately 90 °C) to be compatible with, for example, polymer electrolyte membranes in fuel cells. For physisorption, the challenge is the opposite: to provide systems that still hold H2 at room temperature and ambient pressure. The adsorption of H2 by carbon nanotubes, graphene, polymeric materials, and the metal–organic frameworks of Chapter 14 has received signiﬁcant attention [3]. Currently, no materials come close to targets under ambient conditions and any adsorption-based storage systems will rely on liquid-N2 temperatures and the use of several tens of bar pressures. The alloy LaNi5 is one potential storage material as the number of H atoms that can be stored in interstitial sites (forming LaNi5H6) per unit volume is around double that of H2 liquid at its boiling point. The reversibility of H2 uptake is good, and the H2 pressure at room temperature is around 2 bar. Unfortunately, the mass content of hydrogen is too low at ~1.4 wt%, and La is expensive. Similar problems face CoNi5H4 (1.1 wt%) and PdH0.6 (0.6 wt%). The latter decomposes close to room temperature and shows excellent reversibility, but suffers from the high cost of Pd metal. The only way to achieve a higher mass content of hydrogen in a storage compound is to focus on hydrides from the top rows of the periodic table. MgH2 is one material of interest and can practically store around 7.6 wt% H2, though its decomposition temperature is rather high (~330 °C) and reversibility is poor. Other materials under investigation include complex hydrides such as NaAlH4. When small amounts of Ti or other metals are included as a catalyst, this material can reversibly produce H2 by two processes:

2.2

Intrinsic Point Defects in Compounds

57

Box 2.1 (cont.) NaAlH4 → 1/3Na3AlH6 + 2/3Al + H2 (3.7 wt% H2, > 33 °C) Na3AlH6 → 3NaH + Al + 3/2H2 (1.8 wt% H2, > 110 °C) Although NaAlH4 could theoretically release 5.5 wt% H2, in practice only around 4% can be stored reversibly. In addition, the kinetics are slow. An interesting strategy for reducing the decomposition temperature of a hydrogen-storage material is to either destabilize the hydrogenated form or stabilize the dehydrogenated form. For example, LiBH4 releases ~13.6 wt% H2 in an endothermic reaction, LiBH4 = LiH + B + 3/2H2 (ΔH = 67 kJ/mol H2). If one mixes it with MgH2, the mass hydrogen content is reduced to 11.4 % but the exothermic formation of MgB2 in the reaction, LiBH4 + ½MgH2 → LiH + ½MgB2 + 2H2, makes the total reaction less endothermic (ΔH = 25 kJ mol/H2), and the release temperature lower. Other materials under investigation include the lithium amide–imide–nitride system (LiNH2–Li2 NH–Li3N, which stores 10.4 wt% H2 and in which nonstoichiometric materials are believed to play a key role [4]), ammonia borane (BH3NH3, ~14 wt% release from 100–180 ºC) and related lithium/ sodium amidoboranes (LiNH2BH3/NaNH2BH3, ~11/~7.5 wt% at ~90 °C), though reversibility of all these systems remains an issue. Even if the chemical challenges can be met, there are still signiﬁcant engineering challenges for practical H2-fueled cars. For example, there is signiﬁcant heat produced when either the endothermic chemical processes described above are reversed on refueling, or the heat of adsorption for cryo-adsorption systems is released. Heavy heat exchangers capable of handling hundreds of kilowatts would be required for chemical systems capable of acceptable refueling rates, reducing the gravimetric storage capacity of the system. More information on hydrogenstorage materials can be found via www.doe.gov.

Schottky

Frenkel

Figure 2.2 Schottky and Frenkel defects. Black and white circles represent cations and anions.

from its structural site will perturb the local electroneutrality—the negative charge on surrounding X− ions is no longer cancelled by the charge of the cation. The uncompensated 1− charge is therefore formally assigned to the cation vacancy. The anion vacancy created elsewhere in the crystal at the same time will carry an analogous 1+ charge. These

58

Defects and More Complex Structures

ideas are formalized in the Kröger–Vink notation outlined in Section 2.6. In a Schottky defect, the negative and positive charges will attract each other, which can lead to vacancy clustering in the structure (see Section 2.9). One might also expect that on creation of a defect, the surrounding structure may relax or distort. This is indeed the case but may be difﬁcult to detect using conventional structural characterization techniques (which tend to probe average structures rather than local structures), particularly at low defect concentrations. In Section 2.9, we will see how substantial long-range structural changes can occur at larger defect concentrations. A Frenkel defect consists of a vacancy and a corresponding interstitial ion (of the same charge) to maintain charge balance. Frenkel defects can occur for cations or for anions. AgI commonly shows cation-Frenkel defects, CaF2 anion-Frenkel defects. The number of Frenkel defects increases with the temperature, and materials with a high concentration of Frenkel defects can have signiﬁcant ionic mobility at high temperatures. We’ll see in Chapter 13 that this defect type gives rise to cationic conductivity in AgI and anionic conductivity in CaF2-type materials. We’ll mention other types of disorder/defects possible in compounds only brieﬂy. For many materials, intersite disorder is possible, for example the (Mn2+1−xFe3+x)(Fe3+1−x/2Mn2+x/2)2O4 spinels we discussed in Section 1.5.1, or disordered alloys such as FePt (see Section 4.4.2). In Chapter 13, we’ll also encounter ions that are rotationally disordered in the solid state. The ﬁnal intrinsic point defect we’ll discuss is a color center. It can be described as electrons trapped on vacant anion sites by the positive charge of the vacancy. Isolated trapped electrons are known as F centers. More complex color centers consisting of pairs (M centers) or triplets (R centers) of electrons or trapped holes are also known. The shape of the potential holding the electron in an F center is complex but it can give rise to a localized s-like state as well as a more extended p-like shape. Excitation from one state to the other frequently leads to light absorption in the visible region giving rise to characteristic colors. F centers can be generated in a variety of ways including by exposing alkali halides to excess alkali-metal vapor or by X-ray irradiation. In nature, they give rise to blue forms of calcite and feldspar as well as green diamonds.

2.3

Thermodynamics of Vacancy Formation What factors determine how many defects will be present in a material? Let’s consider an ideal crystal in two dimensions, formed by a single type of atom, such as the one drawn in Figure 2.3. There are N0 atomic sites in the entire crystal. We can consider the formation of a vacancy as the process of moving one atom from its regular site to a new site on the surface of the crystal. The number of sites becomes N0 + 1. What is the Gibbs energy of creating n such isolated, non-interacting, vacancies? The main driving force behind vacancy creation is the increase in conﬁgurational entropy: there are many possible ways to position the vacancy. The conﬁgurational entropy

2.3

Thermodynamics of Vacancy Formation

59

Figure 2.3 Formation of a vacancy in an ideal crystal.

Figure 2.4 Gibbs energy of formation of n vacancies in an ideal crystal with N0 sites.

contribution to ΔG is −kT∙lnΩ per n vacancies formed. In this expression, Ω is the number of ways n vacancies can be arranged over the N0 + n sites, which is given by Ω = (N0 + n)!/(N0!n!) and k is the Boltzmann constant.3 Note that −kT∙lnΩ (Figure 2.4) is not a linear function of the number of vacancies. There is also a smaller vibrational contribution to the entropy, ΔSvib, which arises on vacancy formation. The overall favorable increase in entropy is counteracted by the positive enthalpy of vacancy formation. The enthalpy term is positive as the chemical bonds broken on vacancy formation are only partially compensated by the formation of new bonds at the surface site. At low vacancy concentrations, the ΔH and ΔSvib terms depend simply on the number of vacancies n. Since ΔG = ΔH − TΔS, we can express the total change in Gibbs energy for formation of n vacancies as ΔG = n(ΔH − TΔSvib) − kT∙lnΩ. This expression is plotted as a function of n in Figure 2.4. The nonlinear nature of the conﬁgurational-entropy term means that the minimum in ΔG always occurs at a non-zero value of n; that is, a small equilibrium number of vacancies, neq, will always be formed. The value of neq can be calculated by ﬁnding the minimum in ΔG by differentiation: d ðN0 þ nÞ! nDH nTDSvib kT ln ¼0 (2.1) dn N0 !n!

3

Boltzmann constant k = 1.380649×10−23 J/K.

60

Defects and More Complex Structures

The factorial term can be treated by applying Stirling’s formula, ln(x!) ≈ xlnx − x for large x, which on differentiation leads to: N0 þ neq ¼0 (2.2) DH TDSvib kT ln neq Note that the term in brackets involving neq is simply the inverse of the fractional concentration of vacancies formed, xv. Rearrangement shows that the fractional concentration of vacancies depends solely on temperature and the two parameters, ΔH and ΔSvib: neq DSvib DH ¼ exp xv ¼ exp (2.3) N0 þ neq k kT The form of this equation suggests that the concentration of non-interacting point defects at equilibrium4 follows the mass-action law. We’ll investigate the use of such equilibria in Chapter 3. We can approximate the absolute number of defects by assuming N0 >> neq, which gives: DSvib DH neq ≈ N0 exp exp (2.4) k kT A similar expression would hold for the formation of isolated interstitials. We can see from this expression that either a low ΔH or high T will favor the formation of defects. For Schottky defects in an ionic material, one must consider the number of ways of arranging both cation and anion vacancies. The conﬁgurational entropy term will be −2kT∙ln Ω. A similar derivation gives the equilibrium number of Schottky defect pairs as: DSvib DHS exp (2.5) neq;Schottky ≈ N0 exp 2k 2kT where ΔHS is the formation enthalpy of a Schottky defect pair. For Frenkel defects, one generates n vacancies on the N0 sites and places them on n interstitial sites out of a possible number of NI. There will be a conﬁgurational entropy term of the form N0/I!/(N0/I –n)!n! for both vacancies and interstitials. One can then show that: DSvib DHF ½ neq;Frenkel ≈ ðN0 N1 Þ exp exp (2.6) 2k 2kT Table 2.1 gives molar enthalpies and entropies of defect formation for various compounds from which the number of defects can be readily estimated.5 In Cu metal at 1000 °C, for example, 4

5

Reaching such equilibrium in solids usually requires high temperatures, it’s easy to “trap” non-equilibrium numbers of defects on cooling. Note the need to convert between the Boltzmann constant k, with units J/K, and the molar gas constant R, with units J/(K mol), when using molar quantities; NAk = R.

2.4

Extrinsic Defects

61

Table 2.1 ΔHf and ΔSf for defect formation from ref. [5]. Schottky values concern two vacancies such that the energy per vacancy is similar for all three categories. Defect type

Material

ΔHf, kJ/mol

ΔSf, J/(K mol)

Vacancies

Cu Ag Au Al NaCl NaI KCl KI AgCl AgBr

123 105 91 72 235 193 245 244 140–150 109–124

21 12 8.3 18 81 63 75 86 45–101 55–101

Schottky

Frenkel

one would estimate xv as around 10−4. If one considers that a 1 cm3 block of Cu contains around 8.5×1022 atoms, the total number of defects (~1019) is considerable. It’s worth emphasizing that thermodynamics gives the equilibrium number of defects ignoring kinetics—if a real sample has been rapidly cooled from high temperatures, the actual defect concentration might be much higher than the equilibrium value calculated at the temperature of the cooled sample. Defect concentration calculations are illustrated and expanded in the end-of-chapter problems.

2.4

Extrinsic Defects Defects involving new chemical species are called extrinsic defects. For elemental solids, we’ve seen that foreign atoms can be substituted6 for atoms of the host material to produce what can be described as doped systems at low levels of incorporation or alloys at higher levels. This is called substitutional disorder. Substitutional disorder is also common, and often deliberately targeted, in ionic compounds. As with intrinsic defects, it is important to consider charge balance. In an ionic oxide MO, one can envisage replacing M2+ with another 2+ metal to give a solid solution M1−xM 0 xO (so-called isovalent substitution); a typical example might be Co1−xMnxO that is known to form a solid solution for all values of x. A common and technologically important group of materials based on isovalent cation substitution are luminescent phosphors that rely on doping optically active rare-earth atoms such as Nd and Eu into optically inactive hosts such as La2O2S. More examples of this phenomenon are given in Chapter 7. 6

Loose language by soccer commentators means that there’s often confusion about usage of the verb to substitute; indeed Fowler [Modern English Usage (1964) Oxford] amusingly describes the verb as a “treacherously double edged sword”! The correct usage is that if we “substitute A for B”, B is removed and A is put in its place. “Beckham is substituted for Rooney”, means Rooney leaves the pitch. If in doubt use the verb “replace”.

62

Defects and More Complex Structures

In an aliovalent substitution, an atom is replaced by one with a different oxidation state. An example might be the substitution of Ca2+ for Zr4+ in ZrO2. The introduction of a lower-valent ion means that the substituted site has a formal negative charge that must be compensated (Ca2+ has insufﬁcient charge to compensate the negative charge of O2− ions surrounding the former Zr4+ site). In this case, charge balance is predominantly achieved through the introduction of vacancies on the anion lattice. For every Zr4+ that is replaced by Ca2+ (charge difference of 2 units), a corresponding O2− vacancy is required giving rise to a material with formula Zr1−xCaxO2−x. If one substituted Y3+ for Zr4+ (charge difference of 1), one oxide-ion vacancy for every two Y3+ ions would be required; Zr1−xYxO2−x/2. There is a variety of possible charge compensations involving substitution, vacancies, or interstitials; these are summarized in Table 2.2. In semiconducting materials such as Si, dopants with either more or fewer valence electrons can be introduced: a phosphorus atom is able to donate an electron to the conduction band and is said to be a donor; an aluminum atom accepts electrons from the valence band (or equivalently adds holes to the valence band) and is said to be an acceptor. We’ll explore the case of Li+ acceptor and Al3+ donor doping in NiO in detail in Chapter 3. In cases where the elements present have chemically accessible lower or higher oxidation states, it is possible to achieve charge balance via redox compensation without the introduction of vacancies. If we take the example of La2CuO4, which contains Cu in the +2 oxidation state, it is possible to replace 7.5% of the available La3+ sites with Sr2+ to produce La1.85Sr0.15CuO4. We can understand the charge balance in this material in terms of copper changing its oxidation state from +2 to +2.15 on average. A similar Cu oxidation can also be achieved by incorporating extra oxygen in interstitial sites of La2CuO4, which produces La2CuO4.075. Again, we can understand the charge balance by considering oxidation of Cu from +2 to +2.15 manifested as a mixture of 0.85Cu2+ and 0.15Cu3+ on the Cu site. Both processes convert insulating antiferromagnetic La2 CuO4 into a superconductor at low temperatures (see Chapter 12). The range of different types of cation substitutions, combined with the range of different ways in which charge can be compensated, leads to the development of remarkably complex materials from chemically simple starting points. Even for a binary oxide such as NiO, where oxidation/reduction can lead to a nonstoichiometric formula, there are many possibilities. On oxidation, one can incorporate excess oxygen or create Ni vacancies; on reduction, create Table 2.2 Charge compensation mechanisms in cation-doped materials with ﬁxed integer oxidation states. Symbol ⃞ represents a vacant site. Dopant charge Higher positive Higher positive Lower positive Lower positive Any

Compensated by Cation vacancy Anion addition Cation addition Anion vacancy Double substitution

Host NaCl CaF2 SiO2 ZrO2 CaAl2Si2O8

Dopant 2+

Ca Y3+ Al3+ Ca2+ Na+

Substituted material Na1−2xCax⃞ xCl Ca1−xYxF2+x LixSi1−xAlxO2 Zr1−xCaxO2−x⃞ x (Ca1−xNax)(Al2−xSi2+x)O8

2.5

Solid Solutions and Vegard’s Law

63

Table 2.3 Redox compensations in materials (oxidation states can change). Redox-active metal

Defect or dopant

Examples

Importance

Oxidized

Cation vacancy

Fe1−xO LiCoO2→Li1−xCoO2

Vacancy clustering Battery material

Reduced

Cation interstitial

TiS2→LixTiS2 WO3→NaxWO3

Battery material Electrochromic

Oxidized

Anion interstitial

La2CuO4→La2CuO4+x UO2→UO2+x

Superconductor Structural evolution

Reduced

Anion vacancy

YBa2Cu3O7→YBa2Cu3O7−x WO3→WO3−x

Superconductor Crystallographic shear

Oxidized

Lower-valent cation

La2CuO4→La2−xSrxCuO4 LaMnO3→La1−xCaxMnO3

Superconductor Magnetoresistance

Reduced

Higher-valent cation

Nd2CuO4→Nd2−xCexCuO4 CaMnO3→Ca1−xLaxMnO3

Superconductor Magnetoresistance

oxygen vacancies or incorporate excess Ni. The ways how to treat these possibilities in combination are explored quantitatively in Chapter 3.1. Table 2.3 summarizes some of the possible substitutional mechanisms and gives examples of materials in each category that will be discussed in later chapters. Just as for cations, substitutions for anions are possible, and there is a similar range of charge-compensation mechanisms. Solid solutions based on anion substitution are generally less common than those based on cation substitution. This is principally because the range of anions of similar size/charge is smaller than the range of metals. However, in later chapters we will meet important materials that can be understood in terms of substitution of O2− for F−, N3−, or S2− ions.

2.5

Solid Solutions and Vegard’s Law At low levels of substitution and for certain element combinations, substitutions will occur randomly throughout a crystal structure leading to a solid solution. In many cases, the properties of solid solutions evolve smoothly as one changes the degree of substitution. This enables ﬁne tuning of important parameters. As an example, the unit-cell parameters and volume of a material often vary smoothly from that of the host (e.g. AY) towards those of the substitutent (BY), as the degree of substitution x in A1−xBxY is increased. Such a material is said to follow Vegard’s law (Figure 2.5); for the unit-cell parameter a as an example: aðxÞ ¼ xaBY þ ð1 xÞaAY

(2.7)

64

Defects and More Complex Structures

5.664

3.86

pseudo-cubic cell parameter (Å)

(a)

cell parameter (Å)

5.662 5.660 5.658 5.656 5.654 5.652

(b) 3.84 3.82 3.80 3.78 3.76 3.74

3.72 0

0.5 x in Alx Ga1–x As

1

0

0.5 x in CaRu1–x Mnx O3

1

Figure 2.5 (a) Unit-cell parameter of the AlxGa1−xAs thin ﬁlms [6] and (b) pseudo-cubic cell parameter of CaMnxRu1−xO3 [7]. Dotted lines show the Vegard’s-law prediction.

One can then estimate the degree of substitution directly by determining the cell parameters and rearranging this expression to give x ¼ ½aðxÞ aAY =ðaBY aAY Þ. Control of cell parameters via Vegard’s law can be particularly important when trying to grow an epitaxial (lattice matching) layer of a material on top of a substrate. For example, a semiconductor laser emitting between 1.2 and 1.65 μm (i.e. within the transparency window of optic ﬁbers) can be prepared by sandwiching In1−xGaxP1−yAsy between n- and p-type InP. By adjusting x and y, it’s possible to exactly match the cell parameter of the sandwich layer to that of InP. In addition, the band gaps of many semiconductors can also show a Vegard’s-law dependence. While maintaining the same cell parameter, different combinations of x and y may have different band gaps allowing control over the device’s properties. For a system such as this, our simple form of Vegard’s law must take account of each component present and becomes: aðx; yÞ ¼ xy aGaAs þ xð1 yÞ aGaP þ ð1 xÞy aInAs þ ð1 xÞð1 yÞ aInP

(2.8)

If one introduces appropriate cell parameters (aGaAs = 5.65 Å, aGaP = 5.45 Å, aInAs = 6.06 Å, aInP = 5.87 Å), the relationship between x and y to achieve lattice matching simpliﬁes to: x¼

y 2:21 0:053y

(2.9)

In practice, Vegard’s law is not always followed precisely. For some systems, intermediate members of a solid solution have smaller unit cells than predicted—a negative deviation from Vegard’s law. Others have larger unit cells than predicted and show a positive deviation. This departure is due to the fact that atoms/ions can only be approximately treated as hard

2.5

Solid Solutions and Vegard’s Law

65

Table 2.4 Examples of Kröger–Vink notation of point defects. Symbol vNa 0 CaNa• Fi 0 vO••

Example +

Na vacancy in Na1−2xCaxCl Ca2+ on a Na+ site in Na1−2xCaxCl F− interstitial in Ca1−xYxF2+x O2− vacancy in Zr1−xCaxO2−x

Charge number (effective charge) −1 +1 −1 +2

spheres and speciﬁc bonding interactions cause small deviations in volume. Even for AlxGa1−xAs, the high-precision data of Figure 2.5a show a small but signiﬁcant positive deviation from Vegard’s law; the departure is such that a Vegard’s-law derived Al content would be ~3% in error at x = 0.5. The data for CaMnxRu1−xO3 in Figure 2.5b show a much more marked deviation. The authors have interpreted this as being due to the presence of Mn3+/Ru5+ (as opposed to the expected isovalent Mn4+/Ru4+ substitution) at intermediate compositions.7 Departure from Vegard’s law can therefore give a useful indication of a change in relevant properties of a material under investigation (see also the unit-cell parameter discontinuity in YBa2Cu3O7−x upon entering the superconducting regime in Chapter 12). Many materials also show a maximum range of solid solution, beyond which it is impossible to perform further substitution, a solid-solubility limit. Departure from Vegard’s law can reveal when this limit is reached. Finally, as we will again see in Chapters 3 and 4, the ease of forming solid solutions is often temperature-dependent, and, as a material is cooled, a solid solution may separate (phase segregate) into its component phases. This can lead to islands of one phase surrounded by a matrix of the second.

2.6

Kröger–Vink Notation When discussing defects in crystals it is often useful to adopt a shorthand notation for the various types of defects encountered. The most common is the Kröger–Vink notation in which a symbol of the form ACB is used. Position A is the chemical symbol of the atom concerned or v for vacancy. Superscript B indicates the effective charge of the defect (remember that a cation vacancy leaves a local excess of negative charge at the defect site; an anion vacancy an excess of positive charge). A dot is used for a positively charged defect (i.e. AC•) and a prime for a negatively charged defect (i.e. AC0 ). Finally, the subscript C identiﬁes the site in the crystal on which the defect occurs via the symbol of the host atom or a symbol i if the site is interstitial.8 Typical examples are given in Table 2.4 using materials introduced in Table 2.2. 7

8

Note that the y-axis scales on Figures 2.5a/b are very different: the overall percentage change in cell parameter is ~ 0.1% in (a) and ~3% in (b). In (b) we plot (volume/4)1/3 to give a pseudo-cubic-cell parameter related to the simple perovskite cell. One may also use an s for a surface site (it is often convenient to think of the atoms that are missing in, e.g. a Schottky defect as having migrated to the surface of the crystal).

66

Defects and More Complex Structures

2.7

Line Defects in Metals The defects considered up to now have all been randomly distributed, isolated point defects where the probability of ﬁnding a defect at a given point in a structure is largely independent of whether nearby sites contain a defect. Energetically favorable defect clustering means, however, that it is common to ﬁnd aggregated and extended defects in materials. It is this type of defect, which, for example, gives metals their characteristic properties of malleability and ductility and allows them to be worked into useful forms. We’ll consider two basic types of line defects in metals; edge dislocations and screw dislocations.

2.7.1 Edge Dislocations An edge dislocation can be envisaged as shown in Figure 2.6a illustrating a 2D slice through a crystal structure. An extra plane of atoms (running perpendicular to the plane of the paper) has been inserted into the top half of the crystal. This gives rise to a dislocation line (again perpendicular to the plane of the paper) shown by a star. This defect is similar to the interstitial defect of Figure 2.1b but extends over a 2D plane of the structure. The existence of edge dislocations helps explain why metals can be relatively easily deformed without cracking or failure. If one applies a force perpendicular to the top half of the crystal of Figure 2.6, then the “extra” plane of atoms can move to alleviate the imposed stress. This can occur in a series of steps in which a single line of bonds breaks and then reforms in the crystal such that the dislocation line moves across the crystal by one lattice spacing at a time. The plane along which the dislocation line moves is called the slip plane (shown as a dashed line). In each step only a small number of chemical bonds need to be broken, which helps rationalize the ease with which metals can be deformed. Alternative models of deformation would require the simultaneous breakage of entire planes of metal– metal bonds and would be prohibitively costly in terms of energy. The importance of dislocation motion also helps explain why minor impurities can have a large inﬂuence on the mechanical properties of metals. Impurities can trap dislocations at speciﬁc locations in a sample and prevent their motion. This process is known as pinning. The description of deformations of materials via the slippage of atomic planes also rationalizes why ceramic materials are usually harder, more brittle, and more prone to cleavage than metals. The delocalized, isotropic nature of metallic bonding allows easy slip-plane formation and slippage as opposed to covalent solids; in an ionic solid slippage of planes by one atomic unit is unfavorable due to the repulsive interactions between ions of like charge.

2.7.2 Screw Dislocations The second common type of line defect in metals is a so-called screw dislocation. One can imagine this as a “spiral staircase” or “corkscrew” arrangement formed by slicing a crystal to

2.8

Planar Defects in Materials

67

slip plane

(a)

(c)

(b)

(d)

Figure 2.6 An edge dislocation due to an extra plane of atoms (a). Application of a shear stress moves the edge dislocation through the crystal (b, c) eventually forming a step on the crystal surface (d). Such processes occur as metals are worked.

its center and sliding adjacent layers of atoms by one atomic plane as shown schematically in Figure 2.7. As subsequent atoms attach to the growing crystal surface, they will form a spiral arrangement as shown in the experimental image of SiC on the right of the ﬁgure. This is a line defect, and the line of the dislocation runs up the center of the spiral. Screw dislocations can move through a crystal under applied stress in a similar manner to edge dislocations. In practice, the dislocations in metals may appear more complex than simple edge or screw dislocations. However, most common dislocations can be described as a combination of these two basic types.

2.8

Planar Defects in Materials Many defects in materials involve planes of atoms as opposed to the point and line defects described above. Three categories of planar defects found in technologically important materials are stacking faults, twins, and antiphase boundaries.

2.8.1 Stacking Faults Many materials can be described in terms of layers of atoms or groups of atoms that stack along a certain direction in the structure. These range from metals, which are essentially 3D in their properties, to materials such as graphite, layered transition-metal sulﬁdes, and

68

Defects and More Complex Structures

Figure 2.7 Left: A schematic picture showing the start of a screw dislocation in a crystal. Right: An image of a screw dislocation in a crystal of SiC; the width of the inner terraces is ~10 μm. Image courtesy of Dietmar Siche.

silicate clays which are far more 2D. Section 1.4.1 describes, for example, how the structure of many metals is based on either hexagonal or cubic closest packing of spheres that repeat in the layer-stacking sequence ABABAB and ABCABCABC, respectively. Both ﬁll the same percentage (74.05%) of available space and are close in energy. In fact, some materials switch from one sequence to another under different conditions (for example Co from AB to ABC upon heating above 690 K, or Al from ABC to AB under very high pressures). Such materials may also be prone to faults in the stacking sequence. Stacking faults also occur easily in layered materials such as those related to the CdCl2 or CdI2 structure types (Figure 1.28). In some cases, the forces holding together adjacent layers can be so weak or non-speciﬁc that although materials are highly ordered in two dimensions, adjacent layers along the stacking direction rapidly lose registry. This type of disorder, turbostratic disorder, is commonly found in graphite, layered clays, and molecular intercalates (Chapter 13). While stacking faults occur at random in some materials, in others they give rise to ordered structures. Ordered variants differing by their stacking sequences are referred to as polytypes, and a schematic example is shown in Figure 2.8. Polytypism (formation of several polytypes) is commonly observed in the layered halides, structurally related transition-metal dichalcogenides, SiC, and many other systems. It is a subset of the more general phenomenon of polymorphism: the existence of more than one structural form of a given material.

2.8.2 Twinning Crystallographic twinning is an extended defect that is important in areas as diverse as the mechanical properties of metals, the optical properties of crystals, and the performance of piezoelectrics and ferroelectrics (Chapter 8). A twinned crystal is deﬁned as an intergrowth of two or more individual crystals of the same species, in which the different portions are related by a symmetry operation that doesn’t belong to the point group of the crystal. Each individual is called a twin component or a twin domain and the symmetry operation relating them a twin

2.8

a A

C

A

A

A A

69

b

A B

Planar Defects in Materials

A

A

A

C A

C

A

B

A

A

A

A

B

c A a

A

A

A

b

Figure 2.8 Polytypism of an element. Left: ccp, layer sequence ABC. Right: ABAC.

law. The interface between domains is called a twin boundary or domain boundary, and these can be several atomic layers thick if there is signiﬁcant structural rearrangement required across the boundary. Figure 2.9 contains some examples. Twinning can be detected in a number of ways. Sometimes it leads to crystals with re-entrant9 angles between faces. In translucent crystals, it can be seen using cross polarizers in a polarization microscope as different domains show light extinction at different angles. It is also apparent in singlecrystal diffraction experiments, since each domain will give rise to its own diffraction pattern; hkl reﬂections from different domains may or may not overlap in reciprocal space depending on the twin law. Twinning can be an unwanted complication in these experiments and is one of the reasons why powder-diffraction methods are often used for structural work. There are three twin categories; growth twins, deformation (glide) twins, and transformation twins. Growth twins can arise during the formation of a crystal if it grows from multiple crystallization nuclei. In Figure 2.9a, we can imagine that two domains have grown from different nucleation sites at the twin boundary. Deformation twins occur when a shear stress is applied to a crystal and causes each plane of atoms to move by a fraction of a unit cell relative to the layer below it. Major changes in the crystal’s macroscopic shape arise from small individual atomic displacements, and the process can occur very rapidly (Figure 2.9b). This type of twinning is important in steel-production, mineralogy, and in the superelastic and shape-memory alloys discussed in Box 2.2. In functional materials, twinning is most commonly encountered when the shape of the unit cell has a higher point symmetry than the atomic contents.10 If one imagines producing a crystal by stacking together such unit cells (like building a wall out of parallelepiped bricks), it is easy to make a mistake and start placing bricks upside down without disrupting the overall stacking. 9

10

A re-entrant angle in an irregular polyhedron is an angle inside that polyhedron, which is greater than 180°, such as on the right-hand side of the crystallite shown in Figure 2.9b. Or close to higher symmetry. For example, a monoclinic cell with a β = 90.05° approximates an orthorhombic cell.

70

Defects and More Complex Structures

twin boundary

twin Brick

Brick boundary

Brick

Brick

Brick

Brick

(a)

twin boundary

(b)

(c)

Figure 2.9 (a) A twinned crystal where a growth fault leads to domains related by a mirror plane. (b) A deformation twin where atoms in the top domain of the crystal have been displaced by a shear stress. (c) A high-temperature square lattice (a = b) that distorts into rectangles (a ≈ b) at low temperature will form a twin-domain structure in which the longer edge (emphasized by an arrow) can be aligned in different directions, two of which are shown; domains are related by a fourfold rotation of the square lattice.

Figure 2.9a shows a 2D example where the unit cell is a rectangle and thus has two mirror planes (mm symmetry) while the cell contents (here the word “Brick”) have lower symmetry (here no symmetry). When a “mistake” is made, a new twin component is formed, related to the ﬁrst by one of these mirror planes. This process is only likely to occur if the energy penalty for placing the unit cell in an alternative orientation is low. One situation where this happens is when a structure undergoes a phase transition from a high-symmetry to a related low-symmetry form.11 If only minor structural changes occur, the “lost” symmetry element is likely to act as a twin law giving rise to a transformation twin.12 A common example is when a material is cubic (a = b = c) at high temperature but distorts to a lower symmetry tetragonal (a = b ≲ c) structure on cooling. In this process, it is likely that different regions of the crystal will have their longer c unit-cell axis pointed in different directions in 3D space, giving rise to different domains (a 2D simpliﬁcation is shown in Figure 2.9c where the long cell direction is indicated by an arrow). In fact, doing this will lower the strain across the entire crystal, such that multidomain crystals usually form on cooling. In a transformation twin, the domains are formally related by a rotational symmetry element that is present in the high-symmetry phase but absent in the low-symmetry phase. They are therefore associated with translationengleiche transitions (see Appendix B) in which the translational symmetry is retained (all lattice points are kept) but a portion of the rotational symmetry is lost. The number of twin variants (different twin-domain orientations that will form) can be predicted from the ratio of the number of rotational symmetry operations13 per lattice point in the two space groups in question. The ratio is called the index 11 12

13

There are numerous examples discussed in Chapter 4 and throughout this book. The spatial arrangement of atoms originally related by symmetry is regenerated across the twin boundary when the symmetry operation becomes a twin law. These symmetry operations are in a numbered list for each space-group entry under the heading “Symmetry operations” in the International Tables for Crystallography, Volume A (see Appendix B), one for each point of the general position. In centered space groups, there is a set associated with each of the centering translations (i.e. with each lattice point per cell). The number of individual domains can be much higher than the number of variants obtained from the symmetry-operations ratio per lattice point.

2.8

Planar Defects in Materials

Box 2.2 Materials Spotlight: Shape-memory alloys Shape-memory alloys are a remarkable family of structural materials that can be mechanically deformed at low temperature but will regain their original shape on gentle heating. They thus retain a “memory” of their initial shape. What’s the origin of this memory effect? On cooling, some materials undergo diffusionless transitions (each atom only moves a small distance relative to its neighbors) which lead to twinning of the type shown in Figure 2.9b. These are commonly called martensitic transformations after the well-known example that occurs when austenite (fcc) transforms irreversibly to lower-symmetry martensite (body-centered tetragonal) during the quenching of steel. Shape-memory alloys undergo reversible martensitic transitions in which the details of the low-temperature domain structure control the shape of the crystal. This is shown in the ﬁgure below. If a shape-memory alloy is cooled through the phase transition while restricted to a certain physical shape (step 1 in the ﬁgure), a twin structure with domains of optimal size and arrangement to ﬁt this particular shape will develop. When this cooled form is mechanically deformed (step 2), the twin-domain boundaries will move into a new interlocked metastable position. In it, the twin domain that best compensates the applied stress has grown at the expense of the others, facilitating the deformation. When that form is heated (step 3) above the temperature of the low- to high-symmetry phase transition, the domain structure, and hence the mechanically deformed shape, will be lost. On subsequent cooling (step 4) the original twin structure “stored” in the sample during its initial manufacture, and hence its shape, is reformed.

1 cool

2 deform

3 heat

4 cool

The best-known shape-memory alloy is a 1:1 alloy of Ni and Ti, commonly known as nitinol (nickel titanium Naval Ordnance Laboratory); other commercial materials are based on Curich CuZnAl and CuNiAl alloys. NiTi is cubic at high temperature but on cooling undergoes a phase transition to a structure with a small monoclinic distortion. This martensitic transformation starts at around 60 °C on cooling and 71 °C on warming, but slight changes in composition allow the transition temperature to be controlled between −50 °C and 100 °C. For Cu-based systems, transition temperatures from −180 °C to 200 °C can be achieved. Annealing temperatures of 500–800 °C are typically used to “store” a speciﬁc shape in a sample. Shape-memory alloys have a range of potential applications. Biomedical implants can be prepared, which are inserted into the body in a compressed, deformed state and unfold as they warm to body temperature. Shape-memory ﬁttings to join piping together are available commercially; these are made as tubes, slightly smaller than the pipes, and then deformed at

71

72

Defects and More Complex Structures

Box 2.2 (cont.) low temperature to ﬁt over the two pipes to be joined. On gentle heating, they regain their original dimensions thus forming a tight seal. So-called two-way shape-memory alloys that “remember” the shape of both the low- and high-temperature form can also be prepared. This is achieved by using defects, which create local stresses in a material, to control the places where individual twin domains form. Typing “shape memory movie” into a search engine will provide links to a number of on-line movies that give dramatic illustrations of this effect. A second property of these alloys—their high pseudoelasticity or superelasticity—is exploited in eyeglass frames that can withstand distortions without damage. Here, one operates just above the transformation temperature of the material so that the martensitic transition occurs on application of stress, allowing signiﬁcant mechanical distortion. When the stress is removed, the material reverts to the austenite form and the original shape is regained.

of the translationengleiche subgroup (Appendix B) of the two groups. For example, if a cubic material with space group Pm3m (#221) undergoes a phase transition to a tetragonal structure with space group P4/mmm (#123), the former has 48 symmetry operations (or general points), the latter 16. We therefore expect 48/16 = 3 variants. This result can also be obtained straightforwardly by considering the point-group order alone, which again changes from 48 for m3m (Oh in Schönﬂiess notation) to 16 for 4/mmm (D4h).14

2.8.3 Antiphase Boundaries A third type of planar fault that can occur in crystals is an antiphase boundary. These are frequently associated with site ordering in materials. Consider the situation shown in Figure 2.10, which could represent a square array of oxide ions with metal ions of two different charges (e.g. 1+ and 3+) sitting in the four-coordinate sites. At high temperature, the two types of metal ions are disordered over their common crystallographic site in the structure. On cooling, it may become thermodynamically favorable for them to order in, say, a checkerboard pattern as in the bottom left of Figure 2.10, where cations of low charge are surrounded by high charge and vice versa. Such an arrangement minimizes electrostatic repulsions as it maximizes the separation between the 3+ ions. The second column of Figure 2.10 represents a situation where an antiphase boundary was formed by two ordered regions meeting out of phase as the crystal cools from its surface. The 14

The point group contains only rotational symmetry operations that leave at least one point unchanged. The order is the number of operations it contains. We include the Schönﬂies notation of the point groups (Appendix A) as it’s familiar to most chemists and most inorganic texts will contain point-group character tables that state the group order.

2.8

Planar Defects in Materials

73

cooling

cooling

cooling

no antiphase boundary

antiphase boundary

Figure 2.10 Formation of antiphase boundaries. A hypothetical array of oxide anions (small circles) contains an equimolar mixture of 1+ and 3+ metal cations that are disordered at high temperature (gray circles) and order (white/black circles) on cooling from two hypothetical seeds at the opposite crystal surfaces; 50% meet in phase (on the left), 50% out of phase (on the right). The ordered structure here has a quadrupled unit cell reﬂecting a loss of translational symmetry.

two components are related by a symmetry element present in the high-symmetry structure but missing in the low-symmetry structure. In contrast to twinning, antiphase boundaries form when a subset of translational symmetry elements is lost rather than rotational elements. Antiphase boundaries are therefore associated with klassengleiche subgroups.15 Clearly, the domain-boundary structure on the bottom right is energetically unfavorable with respect to that in the bottom left, but considerable atomic rearrangement would be required to “heal” the fault. The presence and number of antiphase boundaries will depend strongly on the thermal history of a sample. Real examples where antiphase boundaries occur include M-site ordering in double perovskites such as A2MM 0 O6 (AM0.5M 0 0.5O3) that contain a mixture of differently charged M and M 0 ions (e.g. 2+/4+ or 1+/5+) on the octahedral site. Similar effects are found in metal alloys such as FePt that has a cubic structure at high temperature, with Fe and Pt disordered over all sites of an fcc lattice, but orders on cooling to a tetragonal structure with alternate layers of Fe and Pt. Faults occur when different ordered domains meet such that two layers of Fe or two layers of Pt are adjacent or the layers grow in different orientations. The ordered material is of interest in that it has high magnetocrystalline anisotropy making it potentially useful for magnetic data storage. 15

See Appendix B. Klassengleiche subgroups involve a partial loss of translational symmetry (for example, loss of some lattice points due to formation of a supercell or a loss of centering.). The point-group symmetry or crystal class is retained.

74

Defects and More Complex Structures

2.8.4 Crystallographic Shear Structures A ﬁnal family of planar defects that can give rise to nonstoichiometric formulae and structures that initially appear remarkably complex are found in the crystallographic shear structures. They are also frequently referred to as Magnéli phases after A. Magnéli who ﬁrst described Mo9O26 and W20O58. The key to understanding them in terms of extended planar defects was provided by Wadsley [8]. A good example is provided by the tungsten oxides. We have seen in Section 1.5.3 that the structure of WO3, a yellow semiconducting material, can be described in terms of distorted and tilted corner-sharing WO6 octahedra (a distorted variant of the ReO3 structure). When WO3 is heated under reducing atmospheres, or when it is reacted with additional W in the absence of oxygen, a series of compounds of general formula WO3−x (e.g. WO2.9) can be made. These are typically bright blue in color due to partial reduction of W(VI) to W(V). Although their compositions can be approximated as WO3−x, x is not a continuous variable but takes certain discrete values. Careful structural studies have shown that these materials are members of homologous series with general formulae such as WnO3n−1 and WnO3n−2; a material such as WO2.9 being better formulated as W20O58, the n = 20 member of the second series. The structural origin of these general formulae can be understood with respect to Figure 2.11. If one imagines that partial reduction of WO3 initially removes an entire plane of oxygen atoms, one would generate the structure in the middle of Figure 2.11, in which W atoms on either side of the missing plane are only ﬁve-coordinate. If each W in the right-hand ﬁve-coordinate plane is shifted by half a unit cell parallel to the two in-plane axes of the original unit-cell edge of pseudo-cubic WO3, the sixfold coordination of each W is regained. We see a double chain in Figure 2.11 of octahedra that share two edges in addition to sharing their remaining three corners. In the example of Figure 2.11, the octahedra translate solely in the plane of the ﬁgure, but we could also imagine octahedra moving out of the plane to share apical edges instead of the equatorial ones. In reality, many different crystallographic shear planes are possible for WO3. Figure 2.12 shows some of them. Figure 2.12b shows the (101) fault plane. This corresponds to a twin where all oxygens remain coordinated to two octahedral W atoms, and the formula remains WO3. As the plane of defects rotates clockwise in Figure 2.12 from (102) to (103) to (001) ≡ (10∞), the 2D projection shows a line of blocks of four edge-sharing octahedra in part (c), a line of blocks of six octahedra in part (d) and a continuous zig-zag belt of octahedra sharing two edges in (e), with a corresponding decrease in the oxygen content as the oxygen connectivity increases. Irregular (102) Wadsley defects have been observed for WO3−x with x = 0.002. By x = 0.05, these defect planes become ordered, giving a WnO3n−1 family of phases (n = 20 for x = 0.05) with the integer n decreasing as the defect planes get closer on lowering oxygen content (increasing x). Ordered structures of this type are known down to n ≈ 12 of W12O35 (WO2.92 or x = 0.08). Beyond x ≈ 0.08, the spacing of (102) defects becomes too close, and (103) defects are observed instead, leading to WnO3n−2 materials that are well characterized for at

2.9

Gross Nonstoichiometry and Defect Ordering

75

Figure 2.11 A section of the structure of WO3 showing a projection of corner-sharing octahedra. Removal of a plane of oxygen atoms followed by a displacement along the shear plane recreates octahedral coordination around each W. The pseudo-cubic unit cell of WO3 is shown as a dark box.

least n = 26–18 (WO2.92 to WO2.89). As might be expected, similar structures are also observed when a small amount of Nb5+ is substituted for W6+. Figure 2.12f shows an extreme case with regularly spaced defects corresponding to a formula of M2O5; the ideal16 structure of V2O5. The structure of the mixed-anion compound Nb3O7F can similarly be described in terms of crystallographic shear planes of the type shown in Figure 2.12e separated by a single plane of fully corner-shared octahedra. If one allows shear planes in two perpendicular directions, a large family of closely related structures results. An excellent description of the various possibilities is given in the text by Hyde and Andersson (see Further Reading). A similar phenomenon occurs in the rutile TiO2 structure leading to a variety of compositions between Ti3O5 (TiO1.67) and TiO2. The shear planes are harder to depict as there’s no convenient projection to draw, but the resulting structures contain inﬁnite 2D slabs of rutile separated by regions with a portion of face-sharing octahedra. Depending on the shear plane involved, materials with formula TinO2n−p result: TiO1.75 to TiO1.89 have 4 < n < 9 and p = 1; TiO1.89 to TiO1.93 have 9 < n/p < 16 and p > 1; TiO1.93 to TiO1.98 have 16 < n < 40 and p = 1. It’s also common (and unsurprising) to ﬁnd intergrowths of different slabs in electron microscopy images of samples rapidly cooled from high temperature.

2.9

Gross Nonstoichiometry and Defect Ordering In Section 2.3, we investigated the number of vacancies one might expect to ﬁnd in a simple ionic material with ﬁxed oxidation states. For compounds with variable metal oxidation states, defect 16

V2O5 is normally described as layers of edge- and corner-sharing VO5 square pyramids. However, an oxygen from an adjacent layer makes up the sixth coordination site of the V such that it can be described as a highly distorted octahedron.

76

Defects and More Complex Structures

a

c

(101)

(a)

(b)

(103)

(102)

(d)

(c)

(001)

(e)

(f)

Figure 2.12 Possible planar defects for an ideal WO3-type structure. (a) The WO3 structure viewed down the b axis; the unit cell is bold. (b) A twin boundary. (c–e) Crystallographic shear planes with loss of oxygen from the structure. (f) The idealized structure of V2O5.

levels can be sufﬁciently high that defect interactions and ordering become important—this can be remarkably complex. The different TiOx (0 ≤ x ≤ 2) phases that form when Ti is progressively oxidized give several examples [9]. Ti itself is an hcp metal. On oxidation, O2− ions initially adopt interstitial sites in the hcp structure at random before ordering at higher concentrations. At composition Ti6O, oxygen ﬁlls one-third of the octahedral holes in half of the hole planes, at Ti3O, two-thirds of them, and at Ti2O all of them, with anti-CdI2-type ordering adopted. The structure and composition probably evolve continuously over much of this range, and Vegard’s law is

2.9

Gross Nonstoichiometry and Defect Ordering

77

followed up to Ti3O. Early literature [10] suggested that, around TiO0.67–0.75, a structure related to ε-TaN forms but with high O deﬁciency; this can equally be described as O interstitials in the ω-Ti structure. This same structure type has more recently been reported [11] for a TiO composition synthesized in a Bi ﬂux so there is some doubt about the earlier work. Around x = 1, TiO more commonly forms with an NaCl-type structure and a signiﬁcant number of defects. On the O-deﬁcient side (TiO0.64), up to ~36% of oxygen sites are vacant; on the O-rich side (TiO1.26), ~23 % of Ti sites and some O sites are vacant. At the 1:1 composition, ~15 % of both sites are vacant such that we might write the formula as Ti0.85O0.85. Note that in a case like this, neither elemental analysis nor site occupancies reﬁned from diffraction data (which merely measure relative scattering from cation and anion sites) would reveal the presence of defects; density measurements of the type explored in the end-of-chapter problems are one way of detecting them. At low temperatures, vacancies in TiO order to give a monoclinic structure, in which a regular arrangement of one in six cation and anion sites of the NaCl-type structure is empty. Similarly, Ti4O5 (TiO1.2) orders at low temperature to a structure in which four out of ﬁve cation sites are occupied, and O sites are essentially fully occupied. At higher oxygen contents, one reaches Ti2O3 (with the corundum structure), Ti3O5 (several polymorphs)17, Ti4O7, and then the crystallographic shear-plane series TinO2n−1 (with n = 5, 6, . . .) discussed in Section 2.8.4. Iron monoxide (wüstite) provides an example where nonstoichiometry and clustering of defects add signiﬁcant complexity to its ideally NaCl-type structure. In fact, the homogeneity range of FeO does not include the stoichiometric (or integer-valence; see Chapter 3) phase. At 1350 °C, Fe1−xO with 0.06 ≤ x ≤ 0.16 can be prepared; at lower temperatures, the range of x is smaller. These materials are thermodynamically stable above ~570 °C (below this Fe and Fe3O4 are stable) and there has been considerable investigation into the defect structures of quenched samples. The principal defect present is a vacancy on the regular octahedral Fe2+ site (vFe 0 0 ; V for brevity in this FeO case), which is charge-compensated by a small number of interstitial Fe3+ at nearby tetrahedral holes (Fei••• or T) like those occupied by Zn in ZnS, sphalerite, Figure 1.32.18 Due to their effective charge, the vFe 0 0 and Fei••• defects attract each other such that locally the Fe3+ interstitial is surrounded by four Fe2+ vacancies—a V4T cluster (Figure 2.13). What’s more controversial is how these small vacancy clusters are arranged on a longer length scale to form larger clusters.19

17

18

19

The structural chemistry of Ti3O5 is complex, and several polymorphs (α–δ, λ) exist with different arrangements of corner-, edge-, or face-sharing TiO6 octahedra. The γ polymorph [S.-H. Hong, S. Asbrink, Acta Crystallogr. Sect. B 38 (1982), 2570; ICSD 35148] can be viewed as an n = 3 rutile shear structure. We shouldn’t be surprised by this as a similar site is occupied by Fe3+ in Fe3O4 (an inverse spinel structure, i.e. a ccp of O2− with Fe3+ in one-eighth of the tetrahedral holes and Fe2+/Fe3+ in half the octahedral holes). If the clusters order in three dimensions, one would see extra superstructure peaks in diffraction patterns due to the larger unit cell involved. Such peaks are indeed observed experimentally, though for some compositions a commensurate superstructure with asup = 2.5n·aFeO (n is an integer) is formed while at others the superstructure 00 0 is incommensurate (Section 2.11) with asup = (2.51−2.73)n·aFeO—so-called P and P ordering respectively.

78

Defects and More Complex Structures

(a)

(b)

(c)

(d)

Figure 2.13 Iron-vacancy clusters proposed for Fe1−xO: (a) V4T cluster, (b) V10T4, (c) V12T4, and (d) V13 T4. White squares represent Fe2+ vacancies and gray circles interstitial Fe3+ sites. The ccp O2− that lie on the unmarked vertices of each cube are omitted for clarity. Note that each cube here has the size of one octant of the NaCl unit cell shown in Figure 1.26.

In one of the early studies on the defect structure of FeO [12], Koch and Cohen proposed the V13T4 cluster shown in Figure 2.13. Other clusters have been suggested, including the V12 T4 cluster, which, when regularly spaced at a distance of 2.5aFeO (i.e. close to experimentally observed superstructures), would lead to a composition of Fe0.872O. Yet other workers have suggested the importance of V10T4 clusters. A single-crystal study [13] investigating both Bragg diffraction and diffuse scattering on a speciﬁc Fe0.943O sample suggests that V13T4 and V16T5 clusters are important. The experimental data were interpreted in terms of defect clusters lying on the vertices of a highly distorted cubic lattice with spacing ~2.7aFeO, with around 50% of these cells containing a defect and 50% being defect-free. The defect and defect-free regions are not homogeneously distributed through the structure. Interestingly, if one considers the size of a V13T4 cluster and the fact that for charge balance (its charge number is 14−), neighboring octahedral sites must contain a portion of Fe3+ ions, close packing of the overall units would require a cell of ~2.5aFeO. A mixture of larger V16T5 and V13T4 would require a cell of around 2.7aFeO. These values are consistent with experimental observations and explored in the end-of-chapter problems. The precise structural picture of samples quenched to low temperatures is clearly complex, though it’s clear that, at high temperature, isolated vacancies and smaller defect clusters become more important.

2.10 Incommensurate Structures A number of materials exist that appear to have full occupancy of atomic sites in the structure, yet still possess a nonstoichiometric formula. One case occurs in the so-called incommensurate structures, which can’t easily be described using the simple 3D concept of one unit cell and space group introduced in Chapter 1. An example is Sn1.17NbS3.17; one of a number of A1+xBX3+x compounds that were long thought to have a simple ABX3 composition. The origin of the structural complexity in this family is at its heart simple. The structure of Sn1.17NbS3.17 can be described as alternating layers of NaCl-like SnS and

2.10

SnS

a

79

S Nb S

NbS2

c

Incommensurate Structures

Sn,S Sn,S

c b

NbS2

S Nb S

a(NbS2) 12 a(NbS2) ~≈ 7 a(SnS) a(SnS)

Figure 2.14 The intergrowth structure of (SnS)1.17NbS2. The right-hand view shows that b cell parameters of SnS and NbS2 segments are identical such that the layers ﬁt together in a simple fashion; the left-hand view shows that the a cell parameters have no simple relationship.

NbS2 (Figure 2.14).20 The relative sizes of the ideal unit cells of the SnS and NbS2 portions of the structure are such that along b the cells ﬁt together but along a they don’t. In addition, there is no simple integer ratio of the a cell parameters such that, for example, three units of SnS would match up with two units of NbS2; the two periodicities do not match.21 It’s therefore not possible to use a simple multiplied unit cell. The situation is rather like tiling a bathroom with rows of tiles of two different lengths—if one starts in one corner of the room and works along the wall, the gaps between the two rows of tiles may never perfectly align. In fact, for Sn1.17NbS3.17, the cell parameters of the two portions (aSnS = 5.673 Å; aNbS2 = 3.321 Å) are such that the structure approximately matches up after seven SnS and twelve NbS2 unit cells. The formula of the material can therefore be approximated as (SnS)2×7 (NbS2)12 (2 × 7 as each SnS cell contains two formula units) or (SnS)1.17NbS2 (equivalent to Sn1.17NbS3.17) and could be approximately described on a supercell with a = 39.8 Å. This description is, however, rather inelegant, and incommensurately modulated structures such as this are better described using the language of superspace groups and modulation functions (structures that are incommensurate in 3D can be conveniently described in a superspace of (3 + n)D with n added modulation periodicities) [14], but this description is beyond the scope of this text. This approach may also be applied to commensurately modulated structures, those with periodicities that match a small multiple. The advantage is a low number of structural variables, as opposed to working with a large supercell of many atoms.

20 21

The NbS2 layers are similar to those found in CdI2, but with trigonal prismatic rather than octahedral coordination of Nb. In the original publication [Meetsma et al., Acta Crystallogr. Sect. A 45 (1989), 285–291] the SnS portion of the structure was described with a = 5.673 Å, b = 5.750 Å, c = 11.760 Å in space group C2mb with Sn at 0 0.25 0.1335 and S at 0.476 0.25 0.0954 and the NbS2 portion with a = 3.321 Å, b = 5.752 Å, c = 11.763 Å in space group Cm2m with Nb at 0 0 0 and S at 0 0.3335 0.1328. The sets of b and c cell parameters measured differ by less than the experimental uncertainty.

80

Defects and More Complex Structures

Sr Cu O

Figure 2.15 Structure of Sr0.73CuO2. The a axis runs horizontally in the plane of the paper.

Figure 2.15 shows a related phenomenon in the structure of Sr0.73CuO2 that has a Sr periodicity of 3.72 Å and Cu periodicity of around 2.73 Å along the a direction. The Sr:Cu ratio is thus 2.73/3.72 = 0.73. The Cu atom is always in a square-planar coordination environment, whereas the Sr coordination varies as you move along a. Many other materials display structural modulations. For example, the hexagonal perovskite Sr14/11CoO3 [15] has a misﬁt modulation where voids between face-sharing octahedral columns accommodate an excess of the relatively small Sr ions compensated by a partial reduction of Co4+ to Co3+; or metal alloys such as Zn22Li6 [16] show occupational modulation. Incommensurate structures have even been found for simple metals such as Ba and Bi under high pressure.

2.11 Inﬁnitely Adaptive Structures We’ll ﬁnish this chapter with a short discussion of other structures that use simple building principles to accommodate nonstoichiometric and continually variable formulae. In fact, we’ve seen examples of this behavior already in the shear structures of Section 2.8.4, where, as the shear plane or plane spacing changes, a variety of closely related structures with variable composition evolve. Systems where any small compositional change leads to a structure that is unique, even if closely related to those of neighboring compositions, are called inﬁnitely adaptive.22 Another example is the family of Y3+ materials of composition Y(O, F)2.13 to Y(O, F)2.20 that can be formed by the reaction of appropriate quantities of YOF and YF3. Within this composition range, the excess anions are accommodated in a practically inﬁnite series of very closely related structures, each ﬂuorite-related (as is YOF itself). We can understand the structures by considering the ﬂuorite MX2 structure (Figure 1.31) in terms of square grids of X, with a checkerboard arrangement of M above and below the square grid, forming a slab of edge-sharing XM 4/4 tetrahedra (Figure 2.16, left). Fluorite itself can be built up by alternating this MX slab with square grids of X along a stacking axis, giving MX + X = MX2 overall. In the Y3+O1−mF1+2m23 structures, alternate square grids of X are replaced by a layer of X anions with a triangular grid, which, for an ideal situation, is denser by a factor of 2/√3 = 1.155. The composition of this ideal situation 22

23

Using the language of Chapter 4, each composition is a single phase. The compositions are so dense that there are effectively no two-phase regions, just one solid-solution range. The MX2+δ composition can be expressed in various ways. The general formula can be expressed as YxOx−yFx+2y ≡ YO1−mF1+2m ≡ Y(O1−mFm)F1+m; the ﬁnal representation emphasizes that anion sites in the square grid are fully occupied.

2.12 Problems

81

anions

cation

CaF2-structured Y(O1–mFm) slab

hexagonal F layer

Y5O4F7 Y5(O4F)F6 (YO0.8F1.4 MX 2.2)

Figure 2.16 The structure of Y5O4F7 (right) can be built up from Y(O, F) layers of the ﬂuorite type alternating with hexagonal F anion layers with a denser packing than in the square grid. In the Y(O, F) slab, cation sites below the anion layer are shown in paler gray.

becomes MX + 1.155X = MX2.155. Through small adjustments in the size of the triangular anion nets, m in YO1−mF1+2m can be varied from 0.13 to 0.22 (YO0.87F1.26 to YO0.78F1.44). The way in which the square and triangular grids match up in the plane perpendicular to our imagined stacking direction can lead to large unit cells (analogous to the situation drawn in the lower part of Figure 2.14). In the m = 0.2 case of Y5O4F7 shown on the right of Figure 2.16, six triangles line up with ﬁve squares; in m = 0.167 Y6O5F8, seven triangles line up with six squares. These ideas are explored in Problem 2.27. In these phases, the Y sites have local coordination numbers varying between eight (like ﬂuorite) and six, and this type of behavior is therefore most likely in materials where cations have ﬂexible coordination environments. Similar features occur in a range of structures built from different slabs or columns. Traditionally, the structures have been described using large unit cells, but the continuous range of structures within a given system means that they are again often better described as incommensurately modulated structures [17]. While we’ve only touched on a couple of examples, the complexity and range of structures possible in real materials should be apparent.

2.12 Problems 2.1 Given that Cu adopts a ccp structure with a cubic cell parameter of 3.615 Å, conﬁrm that the equilibrium number of vacancies in a 1 cm3 sample at 1000 °C is around 1019. Note the need to convert between k, in J/K, and R, in J/(K mol), when using molar quantities: NAk = R.

82

Defects and More Complex Structures

2.2 Calculate the fractional number of vacancy sites in Cu at (a) 300 K, (b) 800 K, and (c) its melting point (1357 K). 2.3 Assuming a unit-cell parameter of 5.62 Å, estimate the equilibrium number of Schottky defects in a 1 mm3 grain of NaCl at 300 K and at 700 K. 2.4 Derive the equations given in the text for the number of defects at equilibrium, neq, for Schottky and Frenkel defects. You will ﬁnd the following expressions useful: for large x, d d ðc xÞlnðc xÞ ¼ lnðc xÞ 1, and xlnðxÞ ¼ lnðxÞ þ 1. lnðx!Þ≈ xlnðxÞ x, dx dx 2.5 A sample of nonstoichiometric nickel oxide (A) was found to contain 77.70% Ni by mass. (a) Calculate the empirical formula of A and state the two alternatives for the intrinsic defect that would on its own give rise to this formula. (b) A has the NaCl-type structure and an experimental density of 6526 kg/m3. Assuming a cell parameter of 4.180 Å, state which of the two defects is present. (c) State how the cell parameter of A could be determined experimentally and suggest how it would compare to that of stoichiometric NiO. 2.6 A brown sample of zinc oxide was found to have the hexagonal wurtzite structure with a = b = 3.2495 Å, c = 5.2069 Å (α = β = 90°; γ = 120°). Chemical analysis gave 80.765% Zn by mass. Density measurements gave 5810 kg/m3. Determine the formula of the material and state whether it contains oxygen vacancies or interstitial metal atoms. 2.7 Suggest oxidation states for the metal ions in each of the following materials: (a) FeO, Fe0.872O, Fe3O4, FeS2; (b) FeTe, Fe1.1Te; (c) LaOFeAs, LaO0.9F0.1FeAs; and (d) YBaFe2O5, NdBaFe2O5.5, and NdBaCo2O6. 2.8 Suggest oxidation states for the metal ions in each of the following materials: (a) TiS2, Li0.7TiS2; (b) LaMnO3, La0.8Sr0.2MnO3, La0.5Ca0.5MnO3; (c) La2CuO4, La1.85Ba0.15 CuO4, La2CuO4.075; and (d) BaPbO3, BaBiO3, Ba0.6K0.4BiO3. 2.9 TiO with a 1:1 ratio of Ti:O was synthesized and found to have a NaCl-related structure with a = 4.1831 Å and an experimental density of 4927 kg/m3. Comment on these values. 2.10 The table below gives cell parameters and densities for a range of TixOy materials. Determine the defects present in each. From a graph of your results, estimate x for a 1:1 stoichiometric sample TixOx. z in TiOz

Cell (Å)

Density (g/cm3)

1.32 1.12 0.69

4.1608 4.1755 4.2212

4.713 4.867 4.992

3

2.11 NbO has an NaCl-related structure, a cell parameter of 4.21 Å and a density of 7.27 g/cm .

Calculate the percentage of vacant sites in the material. Draw a sketch of how the vacancies can be arranged in an ordered way so as to give square-planar coordination of Nb. What is the O coordination?

2.12 Problems

83

2.12 GaAs1−xPx has a unit-cell parameter of 5.59 Å. Calculate x and estimate the band gap 2.13 2.14

2.15 2.16

2.17

2.18

2.19

(Eg) of the material, given aGaAs = 5.65 Å, Eg = 1.42 eV; aGaP = 5.45 Å, Eg = 2.24 eV. Using the cell parameters quoted in Section 2.5, conﬁrm the form of Equation (2.9). Using the cell-parameter information stated in Section 2.5, calculate the cell parameter expected for In0.76Ga0.24P0.47As0.53. Would this composition be lattice matched to any of the four possible end members: InP, GaP, InAs, or GaAs? State the Kröger–Vink notation for the predominant defects in each of the materials in Table 2.2. Suggest what type of twinning might occur in: (a) an orthorhombic structure with two cell edges approximately equal; (b) a structure with a monoclinc cell with β = 90.1°; (c) an orthorhombic structure with cell parameters a = 3.92 Å, b = 11.21 Å, c = 7.88 Å; and (d) a structure with a conventional primitive monoclinic unit cell with a ≈ c. At high temperatures, BaTiO3 has the cubic perovskite structure. On cooling, it undergoes a series of phase transitions in which the Ti atom moves away from the center of the TiO6 octahedron, and there are changes in the space group and unit-cell parameters causing the ferroelectric behavior discussed in Chapter 8. Determine the number of twindomain variants (orientations) that could form in the ﬁrst step when the cubic (a ≈ 4 Å, space group Pm3m) structure undergoes a phase transition to a tetragonal structure with space group P4mm and cell parameters a = b ≈ c ≈ 4 Å, α = β = γ = 90°. At high temperature, Cu3Au has a disordered fcc structure with space group Fm3m. On cooling, an ordering transition occurs (similar to that in Figure 4.14) and the low-temperature structure has space group Pm3m with Au at 0 0 0 (Wyckoff site 1a) and Cu at ½ ½ 0 (3c). (a) Sketch the low- and high-temperature structures. (b) Is this a translationengleiche or klassengleiche transition? (b) State the number of domain variants in the low-temperature structure and whether they will be related by twin or antiphase boundaries. Like tungsten oxides, molybdenum oxides show a variety of crystallographic shear structures. The unit cell for one of them is shown here:

The octahedra also share corners with octahedra in identical layers above and below the

84

Defects and More Complex Structures

2.20

2.21

2.22

2.23 2.24

2.25

2.26

2.27

plane of the paper. What is the composition of this compound? What is the oxidation state of Mo? A mixture of WO3 and MoO3 was heated with a small excess of W and Mo metals to give a blue single-phase product containing 25.09% O by mass and a 1:1 W:Mo ratio. Determine the empirical formula of the product and suggest its structure type. Assuming the presence of a V12T4 defect cluster of the type shown in Figure 2.13, it is possible to build an ordered superstructure for Fe1−xO using a 5a × 5a × 10a unit cell. This supercell would contain 16 vacancy clusters. Calculate the composition. Assuming that the unit-cell parameter of Fe1−xO is given by Vegard’s law as a = 4.3325 − 0.4103x Å, calculate the experimental density for (a) the hypothetical stoichiometric FeO and (b) an Fe-deﬁcient material with an Fe:O ratio of 1.075. A sample of Fe1−xO has a measured density of 5491 kg/m3 and cell parameter of 4.281 Å. Estimate the composition based on these two observations. Sketch a V4T cluster for the Fe1−xO structure showing both O and vacant Fe sites. Indicate the nearest shell of occupied octahedral Fe sites relative to the vacant site. State how many of these sites must on average be occupied by Fe3+ to achieve electroneutrality. Write down the Kröger–Vink notation of each defect present. Assume that the defect structure of a crystal of Fe1−xO can be described in terms of V13T4 clusters arranged such that they have a cubic cell with a = 2.7 × aFeO, and that on average 50% of these cells contain a defect cluster. Calculate the value of x. A layered material with approximate composition PbNbS3 was found to have a very similar X-ray-diffraction pattern to that of Sn1.17NbS3.17. Single-crystal studies revealed that the PbS portion could be described with cell parameters of a = 5.834 Å, b = 5.801 Å, c = 11.90 Å and the NbS2 part with cell parameters of a = 3.313 Å, b = 5.801 Å, c = 2 × 11.90 Å (ref. [18]). (a) Give a brief description of the likely structure of “PbNbS3”. (b) State how large the a axis would need to be to describe this structure using a conventional crystallographic unit cell. (c) From the cell parameters given, calculate the true composition of “PbNbS3”. (d) Suggest why the c axis of the NbS2 part of the structure is double that of the PbS part. (e) Suggest a likely structure for a material of composition Pb1.14Nb2S5.14. The structure of Y(O, F)2+δ materials can be described in terms of a YX slab based on a square grid of anions alternating with a hexagonal anion grid as shown in Figure 2.16. (a) Conﬁrm that the composition of a material with ideal anion arrays (all nearest anion– anion distances equal) would be MX2.155. (b) State whether you’d expect this MX2.155 material to be commensurate or incommensurate. (c) Assume that the triangles are compressed slightly in the b direction such that horizontal rows of anions align after ﬁve squares and six triangles as in Figure 2.16. Calculate the composition of this material. Repeat your calculation for a system in which anions align after six squares and after

2.14 References

85

seven triangles. (d) State the relationship you’d expect between the square and triangular anion grid in Y7O6F9.

2.13 Further Reading Defects: F.A. Kröger, “The Chemistry of Imperfect Crystals” (1964) North-Holland; K. Kosuge, “Chemistry of Nonstoichiometric Compounds” (1994) Oxford Science Publications; O. Toft Sorensen, “Nonstoichiometric Oxides” (1982) Materials Science Series, Academic Press; R.J. D. Tilley, “Principles and Applications of Chemical Defects” (1998) CRC Press. Twinning: A. Putnis, “Introduction to Mineral Sciences” (1992) Cambridge University Press; U. Müller “Symmetry Relationships between Crystal Structures” (2013) Oxford University Press. Crystallographic shear: B.G. Hyde, S. Andersson, “Inorganic Crystal Structures” (1989) Wiley. Modulated structures: S. van Smaalen, “Incommensurate Crystallography” (2007) Oxford University Press.

2.14 References [1] A.C. van den Berg, C.O. Aréan, “Materials for hydrogen storage: Current research trends and perspectives” Chem. Commun. (2008), 668–681. [2] U. Eberle, M. Felderhoff, F. Schüth, “Chemical and physical solutions for hydrogen storage” Angew. Chem. Int. Ed. Engl. 48 (2009), 6608–6630. [3] L.J. Murray, M. Dinca, J.R. Long, “Hydrogen storage in metal–organic frameworks” Chem. Soc. Rev. 38 (2009), 1294–1314. [4] W.I.F. David, M.O. Jones, D.H. Gregory, C.M. Jewell, S.R. Johnson, A. Walton, P.P. Edwards, “A mechanism for non-stoichiometry in the lithium amide/lithium imide hydrogen storage reaction” J. Am. Chem. Soc. 129 (2007), 1594–1601. [5] A.R. Allnatt, A.B. Lidiard, “Atomic Transport in Solids” (1993) Cambridge University Press. [6] S. Gehrsitz, H. Sigg, N. Herres, K. Bachem, K. Kohler, F.K. Reinhart, “Compositional dependence of the elastic constants and the lattice parameter of AlxGa1−xAs” Phys. Rev. B 60 (1999), 11601–11609. [7] T. Taniguchi, S. Mizusaki, N. Okada, Y. Nagata, S.H. Lai, M.D. Lan, N. Hiraoka, M. Itou, Y. Sakurai, T.C. Ozawa, Y. Noro, H. Samata, “Crystallographic and magnetic properties of the mixed valence oxides CaRu1−xMnxO3” Phys. Rev. B 77 (2008), 014406/1–7. [8] A.D. Wadsley, “Nonstoichiometric metal oxides” Advances in Chemistry Series 39 (1963), 23–36. [9] J.L. Murray, H.A. Wriedt, “The O–Ti (Oxygen–Titanium) system” Bull. Alloy Phase Diagrams 8 (1987), 148–165. [10] B.G. Hyde, S. Andersson, “Inorganic Crystal Structures” (1987) J. Wiley and Sons. [11] A. Shinsaku, D. Bogdanovski, H. Yamane, M. Terauchi, R. Dronskowski, “ε-TiO, a novel stable polymorph of titanium monoxide” Angew. Chem. Int. Ed. Engl. 55 (2016), 1652–1657.

86

Defects and More Complex Structures

[12] F. Koch, J.B. Cohen, “The defect structure of Fe1−xO” Acta Crystallogr. Sect. B 25 (1969), 275–287. [13] T.R. Welberry, A.G. Christy, “Defect distribution and the diffuse X-ray diffraction pattern of wustite Fe1−xO” Phys. Chem. Miner. 24 (1997), 24–28. [14] T. Wagner, A. Schönleber, “A non-mathematical introduction to the superspace description of modulated structures” Acta Crystallogr. Sect. B 65 (2009), 249–268. [15] O. Gourdon, V. Petricek, M. Dusek, P. Bezdicka, S. Durovic, D. Gyepesova, M. Evaina, “Determination of the modulated structure of Sr14/11CoO3 through a (3 + 1)-dimensional space description and using non-harmonic ADPs” Acta Crystallogr. Sect. B 55 (1999), 841–848. [16] V. Pavlyuk, I. Chumak, L. Akselrud, S.Lidin, H. Ehrenberg, “LiZn4−x (x = 0.825) as a (3 + 1)dimensional modulated derivative of hexagonal close packing” Acta Crystallogr. Sect. B 70 (2014), 212–217. [17] S. Schmid, “The yttrium oxide ﬂuoride solid solution described as a composite modulated structure” Acta Crystallogr. Sect. B 54 (1998), 391–398. [18] G.A. Wiegers, A. Meetsma, R.J. Haange, S. Van Smaalen, J.L. De Boer, A. Meerschaut, P. Rabu, J. Rouxel, “The incommensurate misﬁt layer structure of (PbS)1.14NbS2, ‘PbNbS3’, and (LaS)1.14NbS2, ‘LaNbS3’: An X-ray diffraction study” Acta Cryst. Sect. B 46 (1990), 324–332.

3

Defect Chemistry and Nonstoichiometry

One key aspect of materials chemistry is the ability to prepare materials with precisely controlled composition. We’ll see countless times in later chapters that ever minor changes in chemical composition can hugely inﬂuence a material’s properties. Defects of the type we’ve met in Chapter 2 play a key role in both synthesis and composition control. In the ﬁrst sections of this chapter, we’ll investigate how simple ideas of chemical equilibria can give us qualitative and quantitative insights into defect formation. In the second half of the chapter, we’ll look at the diffusion of different types of defects, which controls the reactivity of solids and the properties of some functional materials.

3.1

Narrow Nonstoichiometry in Oxides We learned in Chapter 2 that entropy favors a certain small number of defects in all extended solids. In a metal oxide, defects such as metal or oxygen vacancies and interstitials give rise to a narrow range of oxygen nonstoichiometry around the integer oxidation state of the metal.

3.1.1 Point Defects in a Pure Stoichiometric Oxide Let’s use NiO as an example. Formation of vacancies (Figure 2.4) is one of several possible ways for intrinsic ionic defects to occur in the NaCl-type structure of NiO. In Equations (2.3) to (2.6) we saw that the mass-action law applies to defect formation as if it were a chemical reaction. Using the Kröger–Vink notation (Section 2.6), we can write “chemical” equations for the formation of all possible intrinsic-defect pairs in stoichiometric (1:1) NiO. Table 3.1 shows there are four such pairs: The term “nil” denotes the value of 0 obtained after crossing out the regular structure sites on both sides of the equation. The ﬁrst four equations describe structural defects already introduced in Chapter 2. The last equation describes electronic defects. We symbolize them as electrons and holes, but in a redox-prone oxide such as NiO, the electron e0 would behave as Ni+ (an aliovalent 87

88

Defect Chemistry and Nonstoichiometry

Table 3.1 Formation equations for the four alternative intrinsic ionic-defect pairs in NiO and for intrinsic ionization. Process

Reaction

Schottky: Anti-Schottky: Cation-Frenkel: Anion-Frenkel: Intrinsic ionization:

nil = vNi 0 0 + vO•• NiNi˟ + OO˟ = Nii•• + Oi 0 0 NiNi˟ = vNi 0 0 + Nii•• OO˟ = vO•• + Oi 0 0 nil = e 0 + h• (2NiNi˟ = NiNi 0 + NiNi•)

defect NiNi 0 in the Kröger–Vink notation), whereas the hole h• would represent the oxidized state Ni3+ (NiNi•). The last reaction in Table 3.1 is in principle a disproportionation of divalent nickel into mono- and trivalent defects.1

3.1.2 Point Defects upon Oxidation/Reduction of the Stoichiometric Oxide The possible changes in the numbers of intrinsic defects on oxidation and reduction of the stoichiometric NiO are in Figure 3.1. When NiO is reduced within its homogeneity range,2 either an O deﬁcit appears at its regular structural sites or an excess of Ni at interstitial sites, yielding NiO1−δ or Ni1+δO, respectively. Upon oxidation, either an O excess or a Ni deﬁcit may occur as NiO1+δ or Ni1−δO. These alternative responses are based on the four possible intrinsic point-defect reactions in Table 3.1. Which of them actually dominates in a particular material can only be answered by a rather involved experimental study. One useful rule is that large closest-packed atoms form defects less readily than smaller atoms located in the holes. In nickel oxide and other 3d monoxides, oxidation (adding oxygen) creates metal vacancies vNi 0 0 rather than inserting bulky oxygen interstitials. Likewise, vCr 0 0 0 forms in Cr2O3 and other corundum-type 3d oxides. Reduction (oxygen removal) may form interstitials such as Zni•• in ZnO. However, if the size difference is less pronounced, this approximation fails: CdO with the NaCltype structure, for example, forms oxygen vacancies upon reduction. While the defect type follows from the structure, the propensity for a dominant oxidative or reductive nonstoichiometry depends on the chemistry. A signiﬁcant nonstoichiometry often develops towards another stable oxidation state of the metal. For example, FeO tends to be oxidized towards FeIII. 1

2

Chemically, 2Ni2+ = Ni+ + Ni3+. We will see in Chapter 10 that nil = e 0 + h• represents a thermal excitation of an electron from a valence band to a conduction band, which leaves a hole behind in the valence band. In a redox oxide such as NiO, the electron becomes trapped as Ni+ close to the conduction band, whereas the hole is trapped as Ni3+ close to the valence band. In Chapter 7, we’ll see that optical excitation also creates an electron–hole pair. By “reduction” or “oxidation” in the context of defects, we’ll mean a trace reduction or trace oxidation that creates nonstoichiometry but does not decompose the phase.

3.1

Narrow Nonstoichiometry in Oxides

anion-Frenkel cation-Frenkel

89

Figure 3.1 The four alternative pointdefect compensations for reduction and oxidation of stoichiometric (1:1) NiO are the four alternative intrinsic-defect pairs named on the right.

3.1.3 Equilibrium Equations for Oxidative and Reductive Nonstoichiometry Just as we did for intrinsic defects in Section 3.1.1, we can write equilibrium equations for the point-defect changes that occur on oxidation or reduction of an oxide. Let’s assume O2 to be the only gaseous reactant3 in the intrinsic redox reactions of NiO at high temperature.4 For clarity, we’ll proceed via an auxiliary equation of a small amount of oxygen, δO, reacting with NiO. As shown in the middle column of Table 3.2, oxidation forms holes compensated by the intrinsic negative defect vNi ″ or Oi ″ (Figure 3.1) in an equation balanced in terms of charges, sites (denoted in subscripts), and chemical elements. Analogously so for reduction and electrons in Table 3.3. Next, the auxiliary reactions are simpliﬁed into the defect-formation equation on the right of Table 3.2 and Table 3.3 by crossing out species occurring on both sides, changing to O2, and removing fractions.

Table 3.2 Two alternative compensations of oxidative nonstoichiometry in NiO. Auxiliary scheme vNi ″ Oi ″

3

4

Equation for oxidation •

NiO + δO → δvNi 0 0 + 2δh + δOO˟ + NiNi˟ + OO˟ NiO + δO → δOi 0 0 + 2δh• + NiNi˟ + OO˟

O2(g) ⇄ 2vNi 0 0 + 4h• + 2OO˟ O2(g) ⇄ 2Oi 0 0 + 4h•

An analogous set of equations would have to be set up for every other reacting gas species such as atomic oxygen, ozone, or nickel vapor. Temperature T provides the needed activation energy (for dissociation of O2 and diffusion of defects) in the form of thermal energy kT (k is the Boltzmann constant, 1.380649×10−23 J/K, see Appendix J).

90

Defect Chemistry and Nonstoichiometry

Table 3.3 Two alternative compensations of reductive nonstoichiometry in NiO. Auxiliary scheme Nii•• vO••

NiO − δO → NiO − δO →

Equation for reduction

δNii•• − δNiNi˟ + 2δe 0 − δOO˟ + NiNi˟ δvO•• + 2δe 0 − δOO˟ + NiNi˟ + OO˟

+ OO ˟

2OO˟ + 2NiNi˟ ⇄ 2Nii•• + 4e 0 + O2(g) 2OO˟ ⇄ 2vO•• + 4e 0 + O2(g)

3.1.4 Defect Equilibria for Schottky-Type Redox Compensation In this section, we’ll explore the redox defect chemistry and nonstoichiometry of NiO if Schottky intrinsic-defect pairs (cation and anion vacancies) dominate. We will therefore need to consider two intrinsic-defect pairs—the Schottky pair vO•• and vNi ″ is one, the other is e 0 and h•. There will be two intrinsic-pair formation reactions and two5 redoxdefect reactions, one for oxidation one for reduction; the equilibria 6 are summarized in Table 3.4: Table 3.4 Schottky-type* redox compensation in NiO. Process

Reaction equation

Reaction quotient

Schottky Ionization Oxidation

nil ⇄ vNi 0 0 + vO•• nil ⇄ e 0 + h• O2(g) ⇄ 2vNi 0 0 + 4h• + 2OO˟

KS = [vNi 0 0 ][vO••] Ki = [e 0 ][h•] Kox = [vNi 0 0 ]2[h•]4·pO2−1

Reduction

2OO˟ ⇄ 2vO•• + 4e 0 + O2(g)

Kred = [vO••]2[e 0 ]4·pO2

* Reaction quotients (but not the full reaction equations) for anti-Schottky, Frenkel, and anti-Frenkel intrinsic defect pairs are obtained upon appropriate substitution of defect symbols: Nii•• ≡ vO•• and Oi 0 0 ≡ vNi 0 0 .

Only three of the four reaction quotients (mass-action terms) are independent, as the equilibrium constants combine to KS 2 Ki 4 ¼ Kox Kred . We have four unknowns (the fraction of holes, electrons, nickel vacancies, and oxygen vacancies per NiO formula of regular sites), and we need one more equation. This comes from the electroneutrality condition requiring equal amounts of positive and negative charges: 2½vNi ″ þ ½e0 ¼ ½h• þ 2½vO ••

5

6

(3.1)

Both involve O2 gas. If nickel vapor were present as well, two additional redox equations would follow—one for oxidation of the vapor by holes into regular nickel sites, Ni(g) + vNi 0 0 + 2h• = NiNi˟, and one for reduction of NiNi˟ to nickel vapor, NiNi˟ + vO•• + 2e 0 = 2Ni(g). One of their two reaction quotients would be independent of all the others, which allows us to solve one more variable, the Ni vapor pressure. The unexpressed fractional concentrations of atoms at their regular sites are set to unity due to the low concentration of defects.

3.1

Narrow Nonstoichiometry in Oxides

91

The four independent equations can then be chosen and rearranged such that each of them expresses the fraction of only one type of defect as a function of the partial pressure of oxygen, pO2, having three equilibrium constants as parameters. The equations7 can be solved either analytically or numerically to give the fractions of defects. Once this is done, the oxygen nonstoichiometry [vNi 0 0 ] − [vO•• ] can be evaluated8 as a function of pO2. Figure 3.2 shows logarithmic plots of defect fractions versus pO2 for two limiting cases of dominating intrinsic-defect pair; ionic (left), electronic (right).9 The approximate oxygen nonstoichiometry is given in the upper plots. High oxygen pressures lead to excess oxygen in the oxide; low pressures to oxygen deﬁciency. The defect-concentrations in the lower plots illustrate what causes this simple composition change—changing fractions of electronic defects [e 0 ] and [h•], and of ionic defects [vNi 0 0 ] and [vO•• ]. High [vNi 0 0 ] and [h• ] emerge upon

Figure 3.2 Oxygen nonstoichiometry (top) and defect fractions per formula (bottom) in NiO with dominant ionic defects (left; KS = 10−6, Ki = 10−9, Kox = 10−9) and with dominant electronic defects (right; KS = 10−12, Ki = 10−6, Kox = 10−9).

7

2KS3/2Kox1/4 + KiKSpO2−1/4[vO•• ]1/2 − Kox1/2pO21/4[vO•• ]3/2 − 2Kox1/4KS1/2[vO••]2 = 0

−2KSKox1/4 − Kox1/2pO21/4[vNi 0 0 ]1/2 + KipO2−1/4[vNi 0 0 ]3/2 + 2Kox1/4[vNi 0 0 ]2 = 0 2KoxpO2 + Ki(Kox pO2)1/2[h•] − (Kox pO2)1/2[h• ]3 − 2KS[h• ]4 = 0

8

9

−2KSKi2 − Ki(Kox pO2)1/2[e 0 ] + (Kox pO2)1/2[e 0 ]3 + 2(Kox pO2/Ki2)[e 0 ]4 = 0. The unit of concentration is the same as in the equilibrium constants. The maximum error due to this simpliﬁcation of the precise δ = ([vNi 0 0 ] − [vO••])/(1 − [vNi 0 0 ]) in NiO1+δ is 1% of the nonstoichiometry value at the left edge of the graph in Figure 3.2. PbO is an example of predominant ionic and CuO of predominant electronic defects.

92

Defect Chemistry and Nonstoichiometry

oxidation in oxygen-rich atmospheres, high [vO••] and [e 0 ] upon reduction in oxygen-poor atmospheres.10 In between, there are two important points: Zero nonstoichiometry is associated with the point of integer structure where occupied metal and oxygen sites have the stoichiometric ratio 1:1 and the intrinsic structural defects compensate each other, [vNi 0 0 ] = [vO••]. The point where the electronic defects compensate each other, [e 0 ] = [h•], is the point of integer valence.11 For a pure binary oxide, these two points coincide on the pO2 scale. In several regions of Figure 3.2, the defect fractions have essentially linear variation on the log–log scale. This occurs in ranges where a pair of mutually compensating defects dominates. When Schottky vacancies dominate, the electroneutrality condition in Equation (3.1) simpliﬁes to [vNi 0 0 ] = [vO••] = constant. The mass-action equations for oxidation and reduction in the and [e 0 ] is proportional to last two rows in Table 3.4 then show that [h•] is proportional to pO1/4 2 −1/4 pO2 . This holds in the central part of the plot in Figure 3.2, left, where the slopes on the log–log plot are +¼ and −¼, respectively. In Figure 3.2, right, the central range is dominated by electronic defects, [e 0 ] = [h•] = constant, and analogous substitution gives [vNi 0 0 ] proportional and [vO••] proportional to pO−1/2 . In the most oxidized region, holes are compensated to pO1/2 2 2 by metal vacancies. The electroneutrality condition is 2[vNi 0 0 ] = [h•], and substitution for [h•] in the mass-action term in the “Oxidation” row of Table 3.4 shows that [vNi0 0 ] is proportional . In the most reduced region, electrons are compensated by oxygen vacancies. The to pO1/6 2 electroneutrality condition is [e 0 ] = 2[vO••]. Substitution for [e 0 ] in the mass-action term in the . The existence of linear “Reduction” row of Table 3.4 shows that [vO••] is proportional to pO−1/6 2 regions allows construction of approximate diagrams of defect fractions versus pO2 using straight lines with these slopes—Brouwer diagrams [1], Figure 3.3.

Figure 3.3 Brouwer-diagram sketches corresponding to the previous ﬁgure.

10

Recall that h• is equivalent to Ni3+, e 0 to Ni+.

11

Or of integer oxidation state.

3.1

Narrow Nonstoichiometry in Oxides

93

3.1.5 Acceptor-Doped Oxides How do things change when we replace a small portion of Ni2+ with a cation of a lower and ﬁxed oxidation state (such as Li+), which is called acceptor12 doping? All the mass-action equations from Table 3.4 remain the same. The only difference appears in the electroneutrality condition that now includes the additional defect LiNi 0 : 2½vNi 00 þ ½e0 þ ½LiNi 0 ¼ ½h• þ 2½vO ••

(3.2)

Expressing defect fractions as functions of pO2 can be done in the same way as the pure-oxide case, except that we now have four parameters that control the defect equilibria; the three equilibrium constants and the ﬁxed fraction of the acceptor defect, [LiNi 0 ]. Figure 3.4 shows how the defect concentrations of pure NiO in Figure 3.2 change when [LiNi 0 ] = 0.02. The Li+ acceptor moves the point of integer valence, [e 0 ] = [h•], to lower pO2 because Ni2+ is now more easily oxidized in order to keep the charges balanced. The point of integer structure, [vNi 0 0 ] = [vO••], moves towards higher pO2 because oxygen vacancies are

Figure 3.4 Defect fractions per formula in Li-doped NiO, [LiNi 0 ] = 0.02, for dominant ionic (left) and electronic (right) defects with equilibrium constants as in Figure 3.2. The square in the chemical formula in the top left stands for vacancies.

12

In electronics, an acceptor is a neutral atom with fewer valence electrons than the regular atom. In our context, it is an atom of a ﬁxed oxidation state lower than the matrix atom it replaces.

94

Defect Chemistry and Nonstoichiometry

more easily formed after LiO1/2 has dissolved in NiO and a higher O2 pressure is then needed to ﬁll them. Of the two readily formed defects h• and vO•• that compensate the LiNi 0 acceptor, holes h• dominate around the point of integer structure and vacancies vO•• around the point of integer valence. As before, some regions of Figure 3.4 have a practically linear dependence on log pO2. The reasons for linearity in the extreme oxidized and reduced regions are the same as for the undoped oxide. The integer-valence point and the integer-structure point split due to the doping, and we get approximately linear ranges around both. Because vacancies vO•• compensate the acceptor around the point of integer valence, the electroneutrality condition in Equation (3.2) simpliﬁes there to [LiNi 0 ] = 2[vO••] = constant. As this also keeps [vNi 0 0 ] constant, mass-action equations for oxidation and reduction in the last two rows in Table 3.4 and [e 0 ] proportional to pO−1/4 . Holes h• compensate the give [h•] proportional to pO1/4 2 2 acceptor around the point of integer structure, hence the electroneutrality condition in Equation (3.2) simpliﬁes to [LiNi 0 ] = [h•] = constant. Because this also keeps [e 0 ] constant, mass-action equations for oxidation and reduction in the last two rows in Table 3.4 give [vO••] and [vNi 0 0 ] proportional to pO1/2 . Brouwer diagrams are explored in the proportional to pO−1/2 2 2 end-of-chapter problems.

3.1.6 Donor-Doped Oxides Finally, let’s replace a small portion of Ni2+ in NiO with a higher-valent ion of ﬁxed oxidation state (for example Al3+)—donor13 doping. The mass-action equations from Table 3.4 remain the same, but the electroneutrality condition changes to: 2½vNi 00 þ ½e0 ¼ ½AlNi • þ ½h• þ 2½vO ••

(3.3)

Figure 3.5 shows that the defect fractions and oxygen nonstoichiometry as a function of the partial pressure of oxygen are the inverse of the acceptor case for the same level of doping [AlNi•]. Relative to the pure oxide, it is now easier to reduce Ni2+ and to create nickel vacancies. These [e 0 ] and [vNi ″ ] compensate [AlNi•].

3.1.7 Solid Solubility of Dopants In the previous two subsections on doping, we implicitly assumed that the doping level was always lower than the actual solid solubility of the dopant. In fact, the donor or acceptor solubility in oxides depends on the temperature and partial pressure of oxygen. Before we make some qualitative considerations on the effects of these two variables, let’s consider a simpler case of isovalent substitution. For isovalent substitutions, the effect of temperature on solubility is straightforward. A solution has higher entropy than the sum of its pure components, and increasing 13

In our context, a donor has a ﬁxed oxidation state higher than the matrix atom it replaces.

3.1

Narrow Nonstoichiometry in Oxides

95

Figure 3.5 Defect fractions per formula in Al-doped NiO, [AlNi•] = 0.02, for dominant ionic (left) and electronic (right) defects with equilibrium constants as in Figure 3.2.

temperature will increase the entropy term TΔS that drives the dissolution, thus increasing the solubility. We know empirically that chemically similar isostructural crystals of close enough14 atomic radii mix completely at high temperatures, but calculations [2] do show that they would eventually demix at low temperatures. For aliovalent defects, oxidation and reduction make the picture more complex. Let’s consider ﬁrst the effect of temperature. In an oxide15, increased temperature will favor loss of oxygen (chemical reduction) because the released gas has high entropy. Donor doping makes reduction easier because we can think of the donor oxide (like AlO3/2 dissolved in NiO) as bringing excess oxygen into the structure. Increased temperature will therefore favor dissolution of the donor also by promoting reduction (not only by increased TΔS of mixing). The situation is different for an acceptor. Since an acceptor introduces an oxygen deﬁcit into the structure, the further oxygen loss at high temperature will disfavor this dissolution, but the general entropic driving force of dissolution will still be present. The effect of increasing temperature on the solid solubility of an acceptor therefore can’t be predicted. The effect of the partial pressure of oxygen can be estimated from the Le Chatelier principle16. Dissolution of a donor oxide brings excess oxygen, thus a tendency for easy 14 15 16

Size differences less than 15% typically allow complete solubility at high temperatures. In particular of a redox-active element such as Ni. Equilibrium will adjust to minimize the effects of external changes.

96

Defect Chemistry and Nonstoichiometry

Table 3.5 Dissolution of Al donor in NiO around the point of integer structure. Dissolution reaction Al2O3(s) ⇄ 2e 0 +

2AlNi•

Mass-action term ˟

+ 2OO + ½O2(g)

Ksd = [AlNi•]2[e 0 ]2pO21/2

Table 3.6 Dissolution of Al donor in NiO around the point of integer valence. Dissolution reaction

Mass-action term

Al2O3(s) ⇄ vNi 0 0 + 2AlNi• + 3OO˟

Ksd = [AlNi•]2[vNi 0 0 ]

loss of O2, and this will be favored at low partial pressures of oxygen. Therefore, low pO2 will increase donor solubility, whereas high pO2 will suppress it. For an acceptor, the opposite holds. The dissolved acceptor oxide introduces an oxygen deﬁcit, implying a tendency for easy inclusion of the missing oxygen into the solid; high pO2 will promote this process and increase the solid solubility of the acceptor. The combination of these temperature- and pO2 effects is unambiguous only for dissolution of the donor oxide—high temperature and low pO2 will increase the donor’s solid solubility. To evaluate this quantitatively, we must include the dissolution reaction of the donor oxide in the set of equilibrium defect-reaction equations. Let’s consider the dissolution of the trivalent donor Al in the integer structure of NiO. The defect predominantly compensating the donor will be e 0 (see Figure 3.5 right), and the dissolution reaction will maintain the 1:1 ratio of the anion and cation sites as shown in Table 3.5. At equilibrium with excess Al2O3, [AlNi•] is the solid-solubility fraction x of the donor, and we see from the equilibrium equation that [AlNi•] = [e 0 ]. Substitution into the mass-action term in Table 3.5 gives x = Ksd¼pO2−⅛, and we observe that the solid solubility of the donor increases when pO2 decreases. Similarly, we can evaluate the donor solubility about the point of integer valence. The predominant defects compensating the donor will be vNi 0 0 (see Figure 3.5 left). Table 3.6 above shows that the donor solubility is independent of the partial pressure of oxygen when the defect that predominantly compensates the donor is a structural point defect.

3.1.8 Cautionary Note on Defect Models in Pure Oxides A pitfall of defect modeling in “pure” oxides is that they are never truly pure. In any oxide, there will be impurities inﬂuencing the defect equilibria at some level. Furthermore, some deceptively simple oxides, such as the NaCl-type wüstite of ideal composition FeO, are grossly nonstoichiometric and exhibit clustering of defects (Section 2.9). Real materials

3.1

Narrow Nonstoichiometry in Oxides

Box 3.1 Synthetic Methods: Oxygen-nonstoichiometry control in oxides A precise and homogeneous (non)stoichiometry is important for many functional oxide materials. All methods to achieve this start with equilibrium of the oxygen exchange between the point defects in the solid and the surrounding gas atmosphere. Two processes occur. The ﬁrst is the surface reaction where O2 splits to, or forms from, two oxide anions and four holes. This is a redox reaction since the holes represent the oxidized state of the metal. The subsequent process is a diffusion-driven homogenization, during which the surface-oxygen excess (or deﬁcit) homogenizes throughout the bulk. The oxygen nonstoichiometry can be controlled by the following parameters, depending on whether the system is closed or open: Control parameters

Redox reagent

System

pO2, T

Flowing gas of given pO2 pO2 buffer Oxygen getter or source

Open Closed Closed

T Mass

The open systems use hot ﬂowing reaction atmospheres with deﬁned partial pressures of oxygen. These can be mixtures of Ar and O2 down to pO2 = 10−4 bar; mixtures of Ar, H2, and H2O (via H2O ⇄ H2 + ½O2) below pO2 = 10−10 bar; and CO/CO2 (via CO2 ⇄ CO + ½O2) in the intermediate range. After isothermal equilibration, samples are quenched to low temperature because otherwise they would oxidize during the cool-down. The closed systems are usually set up in sealed ampoules. The pO2 buffer is a solid redox-couple mixture that maintains constant pO2 when it is in excess of the nonstoichiometric sample and not in contact with it. Like in the previous technique, the constant pO2 value is ﬁxed by the temperature. Gibbs phase rule (Chapter 4) states that F = C + 2 − P, where F is the degree of freedom, C is the number of components, and P is the number of phases in equilibrium. As long as the buffer, say, a homogeneous mixture of Ni and NiO, contains Ni and NiO1−δ at equilibrium, the pO2 above them remains constant at a given temperature: 2 components + 2 intensive variables (temperature + pressure) − 3 phases (Ni, NiO, O2) = 1 variable that can be varied independently in the current phase system without a phase disappearing. The temperature will therefore ﬁx the pO2. Almost any pO2 can be achieved by a good choice of the redox couple in equilibrium with O2, from low (Ni– NiO) to very high pO2 (Ag2O2–Ag2O in gold wraps in anvil cells). The oxygen-getter/oxygen-source technique is similar, but here it is the amount of the added substance that controls the oxygen taken up or released by the sample. Zirconium metal is a good getter that completely and rapidly oxidizes into ZrO2 but only if relatively high pO2 levels are generated by the sample. When very low pO2 is needed to reduce the oxide, Mg, Zn, or Fe can be used. A common oxygen source is Ag2O, which releases all O2 above 450 °C. A versatile modiﬁcation of the getter/source technique is solid state coulometry, where speciﬁc amounts of oxygen are dosed to or from an enclosed sample electrochemically, via a window made of cubic stabilized zirconia; an excellent conductor of oxide ions (Chapter 13) yet a poor electronic conductor. When appropriate electric charge is supplied from a Pt electrode, the corresponding amount of oxide anions moves through the zirconia window.

97

98

Defect Chemistry and Nonstoichiometry

range from nearly ideal oxides with randomly distributed dilute point defects, such as Cu2O, NiO, ZnO, and Cr2O3, to quasi-random distributions (CoO), to defect clustering (FeO), to formation of defect-ordered superstructures (CeO2, PrO2), or inﬁnitely adaptive defectordered structures (e.g. Magnéli phases). Simple clustering, such as dimerization or donor–vacancy association, is common for impurities (dopants) even in oxides that exhibit a random distribution of point defects. In general, we must take extreme caution. On the other hand, the next section shows that some complex oxides can have surprisingly simple defect equilibria.

3.2

Wide Nonstoichiometry in Oxides Wide nonstoichiometry ranges can occur between two oxidation states of an atom in two closely related integer structures. An example is the YBa2Cu3O7−δ high-Tc superconductor (0 < δ < 1; Figure 3.6), in which one entire oxygen atom per formula can be removed. In YBa2Cu3O6, one copper atom has a linear coordination typical of Cu+ and the other two are Cu2+. In YBa2Cu3O7, the linear coordination becomes square planar, consistent with Cu3+. This type of nonstoichiometry can also be treated with defect equilibria. We only have to decide which of the limiting structures (Figure 3.6) contains the integer valence that corresponds to the intrinsic situation [e 0 ] = [h• ], where, as Figure 3.2 suggests, properties related to the concentration of these charge carriers should achieve minimum values. Electrical conductivity and oxygen diffusivity decrease towards YBa2Cu3O6 (as discussed in ref. [3]), suggesting it is the integer-valence point. The other limit, YBa2Cu3O7, is then deﬁned as the integer-structure point by formally considering YBa2Cu3O7−δ as an acceptor-doped Y3Cu3O7 with 2BaY 0 per formula. YBa2Cu3O6

YBa2Cu3O7

Cu2+

Cu2+ Ba2+

Cu+

Cu3+ Ba2+

Cu2+

Cu2+ Y3+

Figure 3.6 Two limiting structures of YBa2Cu3O7−δ.

3.3

Point Defects and Diffusion

99

The intrinsic ionic defects in the YBa2Cu3O7 integer structure are of the anion-Frenkel type; oxygen vacancies and interstitials. We can then set up the redox compensations in analogy with Table 3.4 and solve the mass-action equations together with the electroneutrality condition. The Frenkel-process reaction is OO x ¼ vO •• þ Oi 00 , the oxidation reaction is ½O2ðgÞ ¼ 2h• þ Oi 00 , the reduction reaction is OO x ¼ 2e0 þ vO •• þ ½O2ðgÞ . A profound simpliﬁcation can be achieved by subtracting the Frenkel reaction from the oxidation, which yields the intuitive reaction of vacancy ﬁlling and oxidation: ½O2ðgÞ þ vO •• ¼ OO x þ 2h•

(3.4)

Equation (3.4) does not include the e 0 and Oi 0 0 defects important for reduction and oxidation beyond the YBa2Cu3O6 and YBa2Cu3O7 limits, respectively, but it is reasonably valid for YBa2Cu3O7−δ within this range. With vacancies counted from the point of integer structure of the acceptor-doped model, ½vO •• ≈ δ. With holes counted from the point of integer valence, ½h• ≈ 2ð1 δÞ. The mass-action term for Equation (3.4) is then: Kvox ¼ pO2½ 4ð1 δÞ2 =δ

(3.5)

Equation (3.5) has a solution for δ as a function of pO2: Kvox δ¼1 8

rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 16 pﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃ pO2 þ pO2 pO2 Kvox

(3.6)

which describes the entire nonstoichiometry range well for temperatures below 600 °C. As an example, Kvox = 55 bar−1/2 at 500 °C, and δ = 0.12 (YBa2Cu3O6.88) is calculated. That matches both experiment [4] and the full defect-model approach within their uncertainties. Above 600 °C, a progressive deviation from the experimental reality appears for the highest and lowest values of δ calculated by Equation (3.6). Further implications of the YBa2Cu3O7−δ nonstoichiometry are in the end-of-chapter problems and in Chapter 12. This example illustrates that in some cases a simple approximation works for wide nonstoichiometry.

3.3

Point Defects and Diffusion In Section 3.2, we discussed point defects taking part in the reaction of O2 with a crystalline solid. How can oxygen move inside a compact crystal? How long does it take? In fact, the oxygen speed in YBa2Cu3O7−δ is amazing; one day at 400 °C in O2 is enough to fully oxidize a pellet of 1 cm in diameter. We can understand this by realizing that point defects are mobile and disperse homogeneously in a material in order to maximize entropy. This is one of many examples of a process called diffusion. Solid state diffusion is behind major industrial processes, such as hardening of steel, fabrication of doped semiconductors, or “ﬁltering”

100

Defect Chemistry and Nonstoichiometry

oxygen or hydrogen via permeable membranes. It also underpins some important technology, such as the transport of Li+ in lithium batteries or of O2−/H+ in fuel cells. Equations describing diffusion are deceptively simple. Fick’s ﬁrst law states that dc J ¼ D (3.7) dy when limited to one17 direction, y. It tells us that the ﬂux J (the ﬂow density of the diffusing particle in the matrix or substrate18) is directly proportional to the negative gradient of the concentration c of the particle along the ﬂux direction.19 The minus sign is there because the ﬂow in positive direction occurs along a gradient of higher to lower concentrations, down a negative slope, so we have to turn this negative gradient into a positive number. The proportionality constant D is the diffusivity or diffusion coefﬁcient.20 The diffusivity D is characteristic for a particle–matrix pair at a given temperature and pressure; it is not a constant. When the diffusion concerns changes in chemical composition, D is called the chemical diffusion coefﬁcient and is denoted as DA formally implying diffusion of a neutral atom A. Since time does not appear in Equation (3.7), Fick’s ﬁrst law is valid for steady-state diffusion, in which the particle ﬂow into a system equals the ﬂow out. An example is permeation of CO2 (or heat) through a house wall into an open space. The CO2 (heat) ﬂux is constant in the steady state, and its concentration proﬁle across the wall is a straight line of negative slope. Non-steady-state diffusion concerns the spread of diffusing particles as a function of time. The time, τ, is introduced via a continuity consideration—the concentration increase per time equals the net incoming ﬂux per unit length (the negatively taken negative gradient of the particle ﬂux). At every instant, ∂c/∂τ in m−3/s equals −∂J/∂y in (s−1 m−2)/m. Plugging in J from Equation (3.7) leads to Fick’s second law: ∂c ∂ ∂c ¼ D (3.8) ∂τ ∂y ∂y If D is constant and independent of c, it comes before the differential, ∂c/∂τ = D(∂2c/∂y2). This equation states that the change of concentration with time is proportional to the curvature of 17

18 19

20

It can be changed to three dimensions by adding terms for x and z, and treating D as a tensor if the material is anisotropic. In our treatment, we will consider diffusion along one direction in an isotropic matrix of a 3D structure, for which D behaves as a scalar. In a broad sense, the substrate or matrix is everything except the particle whose diffusion we follow. The ﬂux is the number of atoms [J] = s−1 m−2, or moles, [J] = mol s−1 m−2, or kilograms, [J] = kg s−1 m−2 passing per unit time through a unit cross-sectional area perpendicular to the ﬂux. The respective concentrations are in m−3, or mol m−3, or kg m−3. A simple consideration for the units of D and, say, the mole ﬂux: Particles that ﬂow at a rate of 1 mol/s perpendicularly through a 1 m2 window under a concentration gradient of 1 (mol/m3)/m have diffusivity D = 1 m2/s. Substitute into Equation (3.7).

3.3

Point Defects and Diffusion

101

the concentration gradient. In a curved gradient, ﬂuxes at any two points are different, Equation (3.7), and will tend to equalize the concentration. When the diffusion proceeds into an enclosed space, the curvature of the gradient disappears once the concentration c becomes equal throughout the bulk. However, if the particle can leave the bulk, a steady state is eventually obtained. Let’s conclude by noting that both of Fick’s laws belong to a family of equivalent laws that include thermal and electrical conduction.21 In the following sections, we shall consider transport along a ﬁeld gradient in a crystal, termed lattice (bulk) diffusion.22 Uncharged species will move down the chemical-potential slope, whereas charged defects will also move down an electric-potential slope.

3.3.1 Point-Defect Movements Vacancies and interstitials are the transport vehicles in crystal structures. Atoms at regular sites jump into neighboring vacancies, whereas interstitial atoms jump between interstitial sites (Figure 3.7).23 Why do atoms jump? The free energy of an atom is at a minimum at its regular site. Jumps occur because the atom’s thermal vibration24 of frequency ν (in s−1) provides a chance of passing the Gibbsenergy barrier Δ‡Gm for moving to the neighboring vacant site (see Figure 3.9 later on). The likelihood that a vibration becomes a successful jump follows the Boltzmann probability distribution, pB ¼ expðD‡ Gm =kTÞ

(3.9)

where kT is the thermal energy. If pB is, say, 0.0002, on average there will be a jump into a new position every 5000 vibrations. Consider the 2D interstitial in Figure 3.7. It will jump with frequency pBν, but only one-quarter of these jumps will move it forward by the length

21

22

23 24

The thermal-conduction ﬂux is in J s−1 m−2, the electrical-conduction ﬂux in C s−1 m−2 (where J s−1 = W and C s−1 = A). The thermal diffusivity in units of J s−1 m−1 K−1 (under gradient of thermal potential in K per length of 1 m) is normally called thermal conductivity. The electrical diffusivity (under gradient of electric potential in V per length of 1 m, called electric ﬁeld) in units C s−1 m−1 V−1 (= S m−1, siemens per meter) is normally called electrical conductivity. The mass-, thermal- or electrical-conduction ﬂux is generally a vector (in contrast to electric- or magnetic-induction ﬂuxes treated later in the book, which are scalars, being an integral amount of a vector quantity over a ﬁnite area; a dot product of these two vectors, a scalar). This is in order to distinguish it from diffusion via extended defects and grain boundaries, which is usually faster than bulk diffusion. However, for high concentrations of point defects, as in many functional materials, bulk diffusion may dominate. There are also other, more complicated, mechanisms of atom movements. The vibration frequency ν is about 1013 s−1. In the Debye model of atomic oscillators connected by elastic springs of chemical bonds in a periodic solid, ħν = kΘD, where ħ = h/2π and h is the Planck constant (6.62607015×10−34 J s), k is the Boltzmann constant (1.380649×10−23 J/K) and ΘD is the Debye temperature of the solid, typically a few hundreds of kelvins. The kΘD term is the maximum energy (highest frequency) of a sound wave propagating in the solid. ΘD is proportional to the square root of the “spring constant” (the chemical bond strength).

102

Defect Chemistry and Nonstoichiometry

a

Figure 3.7 Self-diffusion of an atom via vacancy (left) or interstitial (gray, right).

a along the chosen direction of the diffusion marked with the arrow. The progression rate (in s−1) of that jump in 2D is rprogression = ¼ pBν. In general, the progression rate of a jump in the direction of the ﬂux is obtained by multiplying the jump frequency pBν with the probability pavail that there is a site to jump to, with the probability pdir that such a site moves the atom forwards by a certain distance along the direction of the ﬂux, and with a correlation factor fc (described below) between the atom that has jumped and the space it left behind: rprogression ¼ fc pdir p avail pB ν

(3.10)

All three factors, pavail, pdir, and fc, depend on the crystal structure and the diffusion mechanism. Let’s consider a body-centered cubic crystal (Nn = 8 nearest neighbors, Figure 1.23) of a metal M with very dilute25 vacancies as the sole defects. Self-diffusion of the atoms via vacancies will have pavail = 8[vM], which is a probability that a vacancy occurs around a selected metal atom when the fraction of vacant sites is [vM].26 The atom will then jump into this vacancy. The probability pdir that this particular vacancy will move the jumping atom along the positive direction of the unit-cell edge is ½. This is because 4 of the 8 nearestneighbor sites advance the atom along this direction (all by a/2). Thus, pavail pdir = 4[vM] in this example. Now, it is relatively unlikely that there will be another vacancy waiting for our atom to jump further. Why doesn’t it jump straight back into the vacancy it left behind? The reason is that it needs to overcome the same energy barrier to jump back. While it waits for this (for a time dictated by the probability), other atoms may ﬁll that vacancy. The probability of the Nn − 1 = 7 neighbors not jumping into the vacancy before our atom is just ½. If they don’t, our atom jumps back, eliminating its 2 jump chances, and the progression rate of the

25

26

Vacancies may tend to cluster at temperatures close to the melting point of the solid and speed up the diffusion. In real materials, line and plane defects, as well as grain boundaries, also contribute to diffusion. Do not confuse the Greek lowercase ν symbol for the frequency with the typographically similar italicized Latin lowercase v in the symbol vM for the vacancy.

3.3

Point Defects and Diffusion

103

original jump is affected by a factor of 1−2/7 = 0.714. This rough estimate, fc = 1−2/(Nn−1), of the correlation factor in Equation (3.10) agrees reasonably with the actual fc = 0.727 obtained by exact and involved derivation for Nn = 8 (see Mehrer in Further Reading). This approximation works well for Nn > 4. Instead of the metal atom M, let’s consider the vacancy jump. While the atom M jumping via the vacancy mechanism has pavail = Nn [vM], the vacancy is jumped into by surrounding M atoms, the availability of which at a selected neighbor site is pavail = 1−[vM] while pdir and fc remain the same. Now, what is the jump frequency of this vacancy? If it has Nn neighbors, it will get jumped into Nn times more often than by just one atom; hence the jump frequency of the vacancy is NnpBν instead of pBν for the atom M in Equation (3.10). While rprogression(M) = fc pdirNn[vM]pBν, we ﬁnd that rprogression(vM) = fc pdirNn(1−[vM])pBν. The ratio of these two jump progression rates is [vM]/(1−[vM]). In more general terms, the ratio of the atom- and vacancy-progression rates is a consequence of the jump balance: as 1 vacancy jumps 1000 times, 1000 atoms jump once. We’ll see soon that rprogression is directly proportional to the diffusion coefﬁcient D, and we anticipate: Datom ½vatom ¼ Dvacancy 1 ½vatom

(3.11)

For low defect fractions, this simpliﬁes to Datom = Dvacancy [vatom].

3.3.2 Random Hopping In the previous section, we realized that atoms in solids jump and move even without an external driving force. In isotropic solids, the movement has equal probability in all directions. The eventual probability distribution follows from a 2D thought experiment called a random walk: If you tag an atom on a plane by placing the coordinate cross at it, and let it “walk” n steps, it will end up some distance from the origin. Do the same with another atom, and it will end up somewhere else. If you mark the ends of very many such random walks, there will be no directional preference, only a radial distribution, in 1D.

number of atoms

σ

radial displacement

σ

0

radial displacement

Figure 3.8 Radial distribution of atoms after many long random walks from zero.

104

Defect Chemistry and Nonstoichiometry

The radial distribution is binomial, and becomes normally distributed for an inﬁnite number of steps. It can be shown that the mean square displacement σn2 after n jumps of equal length λ is equal to the sum of the squares of the individual jump vectors, σn2 = nλ2. Hence after n steps of random walk, the root mean square displacement pﬃﬃﬃ from the origin is σ = λ n. The distribution in Figure 3.8 shows that σ is a convenient measure of the progression of the atoms, only a tiny fraction of which will reach the maximum distance λn in the given time τ = n/rjump. Problem 3.20 explores these ideas further.

3.3.3 Hopping Under a Driving Force At thermal equilibrium, atoms and defects adopt local minima of the Gibbs energy. A typical energy proﬁle between two interstitial sites is shown in Figure 3.9. In the absence of any external force, jumps between the sites will occur at random. If, however, an external ﬁeld exerting a force F is applied, the jumps will develop a preferred direction. Such a ﬁeld may be due to a chemical-potential or an electricpotential gradient. In the direction of the force, the Gibbs-energy barrier for migration, Δ‡Gm, will be lowered (Figure 3.9, right) by an energy Em, while it will be increased in the opposite direction by the same amount. Em is equivalent to the work done by the force F along the corresponding path λ/2: Em ≡ ½λF

(3.12)

For a jump from site 1 to site 2, the barrier height becomes (Δ‡Gm−Em), and the progression rate r12 of this jump is r12 = pdir pavail ν exp{(−Δ‡Gm+Em)/kT} in analogy with Equation (3.10), or r12 = rprogression exp(Em/kT), where rprogression refers to the progression rate under

Gibbs energy

Em ∆‡Gm

λ

1

λ/2

2

1

2

Figure 3.9 Gibbs-energy proﬁle between two interstitial sites. Left: No external force. Right: Under an external force, the forward barrier is lower by Em.

3.3

Point Defects and Diffusion

105

random movement. When the force F is small, the exponential function can be approximated by a Taylor series with only the linear term27 retained, exp(Em/kT) ≈ 1+(Em/kT). The frequency of this jump then becomes r12 ≈ rprogression{1+(Em/kT)}. For jumps in the opposite direction, the Gibbs-energy barrier is higher by Em and accordingly r21 ≈ rprogression{1−(Em/kT)}. Combining these terms gives the net rate rnet = r12 − r21 = rprogression(2Em/kT). Substitution for Em from Equation (3.12) yields rnet = rprogression(λ/kT)F. The net ﬂux J (in s−1 m−2 ) in a given direction is obtained by multiplying rnet (in s−1) by the distance λ (in m) between the two sites and by the local volume concentration c of the atoms (in m−3): J ¼ rprogression

λ2 c F kT

(3.13)

This result provides two important conclusions: (1) The ﬂux depends on the probability of the random progression in the given direction modiﬁed by the effect of the external force. (2) The ﬂux is linearly proportional to the external force.28 In the following sections, we’ll consider two such driving forces—the entropy increase upon homogeneous distribution of defects and the drift of charged defects in an electric ﬁeld.

3.3.4 Hopping Under a Concentration Gradient When defects move in a concentration gradient to homogenize their distribution in a sample, the associated entropy increase decreases the Gibbs energy of the system. The driving force Fi per atom i migrating in direction y is given by the gradient of the partial molar Gibbs energy of that atom (gradient of that atom’s chemical potential µi): Fi ¼

dμi dy

(3.14)

The negative sign in Equation (3.14) means that the transport proceeds from higher values of the potential to lower values, i.e. down the (negative) slope of the potential. The chemical potential per atom i is deﬁned29 as: μi ¼ μ0i þ kTlnai

(3.15)

For a dilute ideal solution of the defect i, the activity ai can be replaced with the volume concentration ci of the defects (in m−3).30 Considering that dµi/dy = (dµi/dci)(dci/dy), the force Fi per atom is:

27 28 29 30

f(x) = f(0) + f 0 (0)x. For x = 0.1 in ex, the error is 0.47%, for x = 0.5 the error is 9%. As long as F is sufﬁciently small so that the linear term of the Taylor-series approximation is sufﬁcient. See any textbook on physical chemistry. If the concentration is expressed in mol/m3, the Boltzmann constant k is replaced with the molar gas constant R = NAk, where NA is Avogadro’s number (6.02214076×1023 mol−1 exactly).

106

Defect Chemistry and Nonstoichiometry

Fi ¼

1 dci kT dy ci

(3.16)

Substituting for F in Equation (3.13) gives: λ2 c i 1 dci dci 2 kT J ¼ rprogression ¼ rprogression λ kT ci dy dy

(3.17)

This reproduces the macroscopic Fick’s ﬁrst law, Equation (3.7), via microscopic atomic jumps. We see that the diffusivity Di (in m2 s−1) of the atom (defect) i in an ideal and dilute solution31 in the solid is Di ¼ rprogression λ2

(3.18)

where rprogression (in s−1) is the progression rate at a given site, Equation (3.10), under random movement, and λ is the jump length in the direction of the progression (in m).32 This is an important result and shows that diffusion under an applied force is controlled by the atom’s self-diffusion coefﬁcient.

3.3.5 Hopping Under an Electric Field From electrostatics we know that the force Fi acting on charge qi in an electric ﬁeld of intensity E is Fi = qiE.33 When the charged defect i moves down the gradient of the electric potential V (in volts),34 it experiences the electric-ﬁeld intensity E = −dV/dy and: dV Fi ¼ qi (3.19) dy Substituting for F in Equation (3.13) and converting the particle ﬂux Ji into the charge ﬂux ji by multiplying it with the charge (in C) per particle qi (hence ji = qiJi), we obtain

31

32

33

34

If the solution of the defect in the solid were ideal but not dilute, the backward ﬂux of the solvent (i.e. the solid host matrix) would have to be included with its own (intrinsic) diffusion coefﬁcient of the participating ﬂuxes. The e combined diffusivity is often called interdiffusivity, denoted as D. For isotropic cubic structures, the probability pdir that a vacancy jump moves a selected atom forward along the direction of the ﬂux, when multiplied by the square of the length λ of the projection of the jump onto that direction, equals ℓ2/6, where ℓ is the actual length of the jump. Furthermore, ℓ2/6 equals a2/Nn, where a is the unit-cell parameter and Nn is the number of nearest neighbors of the vacancy. These formulae can be conveniently used instead of pdir λ2 when D is calculated from the combined Equations (3.10) and (3.18). The unit of the electric-ﬁeld intensity is V/m. One V/m is the intensity of an electric ﬁeld where a point charge of 1 C (C ≡ A s) experiences a force of 1N (N ≡ J/m ≡ Ws/m ≡ VA s/m). 1 N of force per 1 C of charge then equals 1 V/m electric ﬁeld. Note that in this context we use the symbol V for the electric potential. Do not confuse with volume.

3.3

Point Defects and Diffusion

dV ji ¼ σ i dy

107

(3.20)

in which σi is the electrical conductivity due to defect i, σi ¼ rprogression

λ2 ci q2i kT

(3.21)

where rprogression is again the progression rate of Equation (3.10) under random movement. Electrical conductivity is an intrinsic material property and will be treated in more detail in Chapter 10. The conductivity σi represents a fraction ti of the total electrical conductivity σ of the solid due to defects, and ti is termed the transference number of the point defect i. For ﬂux of elementary charges under constant electric potential (a steady state), Equation (3.20) adopts the form j = σE that we’ll recognize in Chapter 10, Equation (10.2), as one possible expression of Ohm’s law.

3.3.6 Relationship between Conductivity and Diffusivity Whether the driving force is electrical or chemical, it produces a ﬂux. The ﬂux Ji of the defect i at a concentration ci under the general driving force Fi, Equation (3.13), can be expressed using the experimentally available35 random diffusivity Di from Equation (3.18): Ji ¼

Di ci Fi kT

(3.22)

It can also be expressed using the experimentally available36 electrical conductivity σi. This makes use of the Nernst–Einstein relation between σi (in S/m, 1 S ≡ 1 A/V) and Di (in m2/s),37 obtained when Equation (3.21) is expressed with Di of Equation (3.18) for a defect i of charge qi (in C ≡ A s) and carrier density ci (in38 1/m3):

35

36

37

38

Di is obtained by tracer-diffusion techniques with isotopes. An isotope is traceable either by mass spectrometry after sectioning the sample, or by measuring radioactivity along the diffusion path if a radioactive isotope is used. As noted earlier, for vacancy mechanisms the tracer-diffusion coefﬁcient is smaller than a purely random diffusion model by the correlation factor fc. For interstitial diffusion of dilute defects, fc = 1. σi is obtained by measuring electrical conductivity with electrodes that conduct speciﬁcally via the defect i. As an example, ZrO2 (Chapter 13) blocks electronic carriers while allowing oxide anions through. The Di thus obtained from conductivity (Dconductivity) will not necessarily be the same as the tracer-diffusion coefﬁcient for the same atom/defect. The ratio Dtracer/Dconductivity is then evaluated as the Haven ratio and reﬂects various movement correlations for the charged defects. When the amount of charge-carrying defects is expressed in moles, hence the carrier density is in mol/m3, we replace kT with RT, and the defect’s electric charge qi = zie with ziF. Here F is the Faraday constant (1 mole of elementary charges: NAe = 6.02214076×1023 × 1.602176634×10−19 ≈ 96485.3 C) and zi is the defect’s charge number (the integer charge in units of elementary charge e).

108

Defect Chemistry and Nonstoichiometry

Di σi ¼ 2 kT qi ci

(3.23)

Substituting from here for Di in Equation (3.22) yields the ﬂux in terms of σi: Ji ¼

σi Fi q2i

(3.24)

Returning to the Nernst–Einstein relation, we can perform one last step that will lead to the useful concept of mobility that we’ll encounter in Chapters 10 and 13. Mobility, μi, is the speed of a species i per unit intensity of the ﬁeld that moves it. It is obtained by multiplying Equation (3.23) with the charge qi in coulombs. Both sides of the equation then have units of m/s per V/m; the left-hand side μi = Diqi /kT expresses the mobility of the charged defect via its random diffusivity and the right-hand side μi = σi/qici via its electrical conductivity. Finally, we should note that transport of a single type of charged particle is rare. It is usually accompanied by transport of a compensating counter charge, forming two ﬂuxes that together appear as a total ﬂux of neutral atoms. This is explored in the following section.

3.3.7 Ambipolar Diffusion Transport of charged defects is not limited to situations where an electric ﬁeld is applied. In many cases, transport under a concentration gradient proceeds via charged defects. Clearly, the transport of a charged defect in the absence of an applied electric ﬁeld must maintain bulk neutrality. Consider the oxidation of YBa2Cu3O6 by O2 as discussed in Section 3.2. Chemically, a copper cation is oxidized while ½O2 is reduced to O2−. As O2− migrates into the center of the sample, the positive cation charges (holes) follow its motion; we thus have an inﬂux of both negative (O2−) and positive species (2h•), which together represent the ﬂow of oxygen as a neutral atom (O). This type of polar transport of nonpolar species is called ambipolar diffusion. Equation (3.4) describes oxygen transport in YBa2Cu3O7−δ in terms of defects. At the surface, O2 oxidizes copper (creates h•) and is reduced to O2− ions that ﬁll vO•• coming from the interior. The holes migrate inwards. Because these defects are charged, any non-uniform distribution not only creates a concentration gradient but also a local electric-potential gradient. A ﬂux under the combined chemical and electric potentials therefore requires a formal summation of the two forces Fi used separately in Equation (3.14) and Equation (3.19). The ﬂux of Equation (3.24) then becomes: σi ∂μi ∂V Ji ¼ 2 (3.25) qi ∂y ∂y qi

3.3

Point Defects and Diffusion

109

As stated above, there are two such ﬂuxes, an outward ﬂux of vO•• and a charge-compensating inward ﬂux of h•. The charge of one mole of oxygen vacancies is +2F, the charge of one mole of holes is +1F. The participating mole ﬂuxes are then: Jv••O

∂μv•• σv••O ∂V σh• ∂μh• ∂V O 2F F ¼ 2 and Jh• ¼ 2 ∂y ∂y 4F ∂y F ∂y

(3.26)

Electroneutrality requires the sum of charged ﬂuxes to be zero. The ﬂux of holes must therefore be twice the ﬂux of oxygen vacancies and run in the opposite direction: Jh• ¼ 2Jv••O

(3.27)

We cannot establish the actual electric potential created inside the solid, so a good way to proceed is to eliminate the ∂V/∂y terms from Equations (3.26).39 By taking the actual inward O ﬂux (see above) as the negative of the oxygen vacancy ﬂux, we obtain: JO ¼ Jv••O ¼

∂μv•• 1 1 ∂μh• O 2 1 ∂y ∂y 4F 2 1 þ σv••O σh•

(3.28)

The form of this equation suggests that the ﬂux of O behaves as if driven by its own chemicalpotential gradient—a sum of the gradients of the ionic- and electronic-defect ﬂuxes (of vO•• and h•, respectively):

∂μO ∂μv••O ∂μ • ¼ 2 h ∂y ∂y ∂y

(3.29)

Note that the combination of the ionic- and electronic-defect conductivities in Equation (3.28) appears in a mathematical form as if ionic and electronic resistivities40 were summed and then inverted into the total ambipolar conductivity σO. This can be interpreted as though the ionic and electronic resistors are connected in series in a circuit. When the O-ﬂux Equation (3.28) is formally rewritten in terms of ∂μO =∂y and σO, σO ∂μO JO ¼ 2 (3.30) 4F ∂y it becomes obvious that a diffusion coefﬁcient for the neutral species O (the chemical diffusion coefﬁcient DO) can also be deﬁned. At this point, we need to remember that diffusivities are normally expressed via gradients of concentrations c and not of chemical potentials (Section 3.3.4). Therefore a conversion ∂μO =∂y ¼ ð∂μO =∂cO Þð∂cO =∂yÞ is performed 39

40

For example by expressing the coulombic term ∂V/∂y from the equation for holes, substituting it into the equation for vacancies, substituting for the hole ﬂux from Equation (3.27), and rearranging. Resistivity is the inverse of conductivity.

110

Defect Chemistry and Nonstoichiometry

on Equation (3.30). In the result, we identify DO as the proportionality parameter between the ﬂux JO and the concentration gradient ∂cO =∂y: σO ∂μO DO ¼ 2 (3.31) 4F ∂cO Having deﬁned the chemical diffusion coefﬁcient DO, we can return to the individual point defects and their concentrations. From Equation (3.29), we see that ∂μO ¼ ∂μv•• þ 2∂μh• , and electroO neutrality dictates that ∂cO ¼ ∂cv••O ¼ ∂ch• =2 (there are two holes per vacancy). This gives: ! ∂μv•• σO ∂μ • O (3.32) DO ¼ 2 þ4 h 4F ∂cv••O ∂ch• For low concentrations of defects, activity depends on concentration via µ = µ0 + RT lnc; hence ∂μ=∂c ≈ RT=c, where c is the equilibrium steady-state concentration in mol m−3.41 Converting σO back to the defect conductivities, we obtain: ! RT 1 1 1 (3.33) DO ¼ 2 þ 1 1 F 4cv••O ch• þ σv••O σh• What remains is to express the separate diffusion coefﬁcients for the ionic- and electronicdefect components. This is done by substituting for each of the two defect conductivities from the Nernst–Einstein relation of Equation (3.23), which after rearrangement gives: ! 1 1 1 (3.34) þ DO ¼ 1 1 4cv••O ch• þ Dv••O 4cv••O Dh• ch• We see that the diffusion coefﬁcient of the chemical element transported depends on the participating electronic and ionic defects; their individual diffusivities/conductivities, their charge numbers, and their equilibrium concentrations. The diffusion of the neutral chemical element is largely controlled by the slower species,42 but the slower ﬂux is somewhat enhanced by the faster ﬂux. As an example, the enhancement factor for Equation (3.34) approaches a maximum of DO =Dv••O ¼ 1 þ ð4cv••O =ch• Þ ¼ 3 if Dh• ch• >> Dv••O 4cv••O . 41 42

For concentrations given in number of particles per m3, R is replaced by k, and F by e. Diffusion of neutral O through a purely oxide-ion conductor, such as Ca- or Y-doped zirconia, is limited by the material’s low electronic conductivity. It speeds up enormously when a metallic conductor is added to transport the electrons. That can be a Pt powder mixed with the doped-zirconia powder prior to sintering into the device form, or an external wire connecting porous Pt electrodes applied onto the two opposite surfaces along the diffusion path. In contrast, diffusion of O through a good electronic conductor, such as YBa2Cu3O7−δ, is controlled by the oxygen-ion conductivity of the material.

3.3

Point Defects and Diffusion

111

3.3.8 Temperature Dependence of Diffusivity As we have just seen, point defects are the vehicles of mass transport in crystalline solids. Diffusivity depends on temperature via the energetics of their movement. The energetics may have two contributions—the cost of making the vehicle and the cost of running it. Both costs can be expressed in terms of the free-energy change ΔG (the ability of a system to do work), and the common approximation is to consider the enthalpy and entropy terms in ΔG = ΔH − TΔS to be independent of temperature. The making costs are the total Gibbs free energy of formation for the defects relevant in the particular transport. This is derived in Section 2.3, where Equation (2.3) gives the equilibrium fractional concentration of the defect as a function of the changes in atomic vibration entropy (ΔSvib) and enthalpy (ΔHf) upon defect formation. The running costs stem from Equation (3.9), which represents the increasing Boltzmann probability that at higher temperatures the atom will be more likely to overcome the Gibbs-energy barrier for migration: Δ‡Gm = Δ‡Hm − TΔ‡Sm. Let’s consider a metal atom M diffusing by a vacancy mechanism in its own cubic structure where it has Nn nearest neighbors. Substituting Δ‡Gm in Equation (3.9) with Δ‡Hm − TΔ‡Sm, considering that pavail = Nn[vM] in Equation (3.10), expressing [vM] with Equation (2.3), replacing k with R so that the enthalpy and entropy are per mole, and plugging the result into Equation (3.18), yields: DM ¼ λ2 fc pdir Nn ν expðD‡ Sm =R þ DSvib =RÞ expðD‡ Hm =RT DHf =RTÞ

(3.35)

Here DM has the temperature dependence of the Arrhenius equation, D = D0exp(−EA/RT), in which the activation energy EA combines the enthalpy contributions, and the preexponential term D0 includes everything else. EA can therefore be obtained from experimental data by least-squares ﬁtting of the linear slope of lnD versus 1/T. In some cases, the making costs do not apply and only running costs need be considered. This is the case for the diffusion of foreign or extrinsic interstitial atoms in low concentrations, for example of solid-solution carbon atoms in iron. Here the vehicle is simply the extrinsic defect itself, pavail ≈ 1, and the equivalent expression becomes: Dinterstitial;extrinsic ¼ λ2 fc pdir ν expðD‡ Sm =RÞ expðD‡ Hm =RTÞ

(3.36)

3.3.9 Diffusivity and Redox Defect Equilibria Let’s now consider diffusion in a metal oxide via a metal- or oxygen-vacancy mechanism. Here, we’ll have to take into account how the vacancy fraction depends on the equilibria we explored in Section 3.1. The constituent atom i (metal or oxygen) at its regular lattice site will not migrate unless it has an adjacent vacancy. The probability of this is pavail = Nn [vi], and we modify the previous result (take fc = 1 for simplicity) to

112

Defect Chemistry and Nonstoichiometry

Di ¼ Nn ½vi λ2 pdir ν expðD‡ Sm =RÞ expðD‡ Hm =RTÞ

(3.37)

The vehicle production costs not-yet-included concern the vacancy fraction [vi] and follow from energetics of the point-defect equilibria the vacancy is involved in. Let’s consider three cases where this [vi] = f(T) function is straightforward. The ﬁrst is when the high-temperature vacancy fraction [vi] in the material becomes “frozen” at lower temperatures when kinetic factors prevent further redox exchange with the reaction atmosphere to establish a new equilibrium. The second is when [vi] is independent of temperature because it is ﬁxed by aliovalent dopants around the point of integer valence (oxygen vacancies in Figure 3.4 and nickel vacancies in Figure 3.5). The third case is when the vacancy is the dominant defect and [vi] can be expressed via the temperature dependence of the equilibrium constant K for the defect-formation reaction in terms of the reactionenthalpy and -entropy change as K = exp[(ΔS/R)−ΔH/RT].43 As an example, when NiO is oxidized, holes are compensated by nickel vacancies (Figure 3.2). The electroneutrality condition simpliﬁes to 2[vNi 0 0 ] = [h•], and from Table 3.4 we see that [vNi 0 0 ] = (pO2Kox/16)1/6. Substituting into Equation (3.37) and rearrangement gives the random diffusion coefﬁcient of Ni in oxidized nonstoichiometric NiO via a vacancy mechanism as ! ! p 16 DSox þ 6D‡ Sm DHox þ 6D‡ Hm O2 2 DNi ¼ exp (3.38) Nn λ pdir ν exp 16 6R 6RT where both the Arrhenius activation enthalpy and the pre-exponential factor have two components—one from the defect formation and one from the defect mobility. As stated earlier, ν is the (essentially constant) vibration frequency of the atom and pdir is the probability that the jump occurs in the ﬂux direction, advancing the atom by the distance λ. See Footnote 32 in this chapter for alternative expressions of λ2 pdir.

3.3.10 Outline of Non-Steady-State Diffusion Fick’s second law, Equation (3.8), expanded into three dimensions, has analytical solutions for time-dependent concentrations of diffusing species across simple shapes such as a plate of inﬁnite thickness (termed a half-space; diffusion enters from one side only), a plate of ﬁnite thickness (diffusion enters from both sides), a parallelepiped, a cylinder, or a sphere, all provided D is constant. The principal solutions are in the literature on either particle diffusion [like Crank or Mehrer in Further Reading] or heat conduction. When D depends on the concentration c, this must be properly included in the treatment. As an example, we’ll calculate oxygen-content proﬁles in a half-space of YBa2Cu3O6 exposed to O2 at 350 °C (Figure 3.10). In this arrangement, the oxygen ﬂux has one direction. Assuming that the surface reduction of O2 is instantaneous and D is independent of 43

Since ΔG = −RT lnK.

3.3

Point Defects and Diffusion

y

O2(g)

113

Figure 3.10 Set-up sketch of oxygen diffusion into half-space of YBa2Cu3O6.

concentration, Equation (3.8) is simpliﬁed, and the solution starts by introducing the dimensionless (half) length, y=2 u ¼ pﬃﬃﬃﬃﬃﬃ ; Dτ

(3.39)

as a new variable.44 This replaces the two variables (τ and y) in Fick’s second law 2 2 ∂c ∂c ∂c ∂c ∂u ∂c ∂2 c ∂u 2 . ¼D ¼ and with one. Given the new variable u, ¼ ∂τ ∂y2 ∂τ ∂u ∂τ ∂y2 ∂u2 ∂y ∂u u ∂u 1 ¼ and ¼ pﬃﬃﬃﬃﬃﬃﬃﬃ are obtained by differentiating u. In the latter two expressions, ∂τ 2τ ∂y 4Dτ 2 dc dc This yields the differential equation 2 þ 2u ¼ 0. Substituting z ¼ dc=du simpliﬁes it to du du dz 1 þ 2uz ¼ 0. Separation of variables gives dz ¼ 2udu that is integrated to du z 2 2 lnz ¼ u þ const, from which z ¼ C expðu Þ. Putting back z ¼ dc=du yields pﬃﬃﬃ π dc ¼ C expðu2 Þdu. The integral of expðu2 Þdu equals erfðuÞ, expressed with the 2 Gaussian error function (erf).45 Given the boundary limits of erf(0) at the concentration pﬃﬃﬃ c = 1 at u = 0 at any time and erf(∞) = 1 when c = 0 at u = ∞ at any time, C ¼ 2= π. Integration of the left-hand side of the differential equation gives c = −erf(u) + K. The initial condition of c = 1 at u = 0 yields K = 1 and the relative concentration change cr: cr ¼ 1 erfðuÞ

(3.40)

In Figure 3.11 (left), our solution of Equation (3.40) is illustrated for DO = 7.144×10−13 m2/s at 350 °C. The concentration proﬁle is linear close to the interface pﬃﬃﬃﬃﬃﬃ as erf(u) ≈ u for low u. Even at u = 0.5, erf(u) is 0.5205, which happens at the distance Dτ; see Equation (3.39). This distance is called the penetration depth (Figure 3.11). It is a characteristic value indicating the extent of penetration of the diffusant. For diffusion solutions based on the erf function, it is close to the diffusion half length; a length where a 50% concentration change occurs in 44 45

This is possible only if both initial and boundary conditions are functions of u only. The erf(u) is the integral of the normal probability distribution from its center at 0 to u. That distribution is the limiting large-numbers envelope for the discrete binomial distribution, Figure 3.8.

114

Defect Chemistry and Nonstoichiometry

600 500

0.8 0.6 0.4 10

40

90

160

250

360

0.2 0.0 0.0

0.5

1.0

1.5

log D (m2/s)

cr or x in YBa2Cu3O6+x

Relative concentration profile

300 t (°C)

400

1.0 -8 -10 -12 -14 1.0

1.2

distance (mm)

1.4

1.6

1.8

2.0

1000/T (K−1)

Figure 3.11 Left: Proﬁles of oxygen-content increase inpﬃﬃﬃﬃﬃ a thick layer of YBa2Cu3O6 exposed to O2 at ﬃ 350 °C, after 10, 40, 90, etc. hours. Penetration depths Dτ are marked by dots. Right: Arrhenius-type temperature dependence of the diffusion coefﬁcient over temperature range 350 to 600 °C.

a given time. Note also that the penetration depth doubles in 22 times that time, triples in 32 times that time, etc. Equation (3.40) is derived for a plate of inﬁnite thickness. It can also be used for the initial stages of diffusion into a ﬁnite or thin plate, but only until the concentration starts to change signiﬁcantly at half the plate thickness. The D values for temperatures of interest are easily evaluated from published Arrhenius-type temperature dependencies. The D dependence for our example is plotted in Figure 3.11 (right) and has an activation energy of 129.2 kJ/mol and D0 of 4.808×10−2 m2/s.

3.3.11 Cautionary Note on Diffusion in Real Materials Caution needs to be applied when investigating diffusion in real oxides and other binary compounds with high ionicity. In addition to possible computational difﬁculties, problems may be encountered either due to the diffusion model or due to the sample. The model-related problems concern the assumption of single point defects being the transport vehicles. In many oxides, these are in reality aggregated defect clusters, the simplest of which are dimers of interstitials or vacancies. Other model-related problems include disregarding ambipolar diffusion, and, in variable-temperature studies, the fact that D may depend on some defect concentration that is chemically variable due to reaction with the measurement atmosphere. There are also the practical difﬁculties of arranging the experiment in a manner that correctly approximates the initial and boundary conditions of the model. Sample perfection and morphology is also of concern—in single-crystal measurements, line defects can lead to short-circuit diffusion; in polycrystalline materials, a similar rapid transport can occur at grain boundaries. Last, but not least, omnipresent aliovalent impurities will increase diffusivity by creating point defects as vehicles for the mass transport.

3.4

3.4

Problems

115

Problems 3.1 Write Kröger–Vink symbols for the following fully charged point defects in NiO: metal vacancy, oxygen vacancy, lithium acceptor, aluminum donor. 3.2 Name the following defects in TiO2 and write their Kröger–Vink symbols: Al and Nb dopants at the Ti site; F and N dopants at the O site; oxygen and titanium atoms out of their regular sites. 3.3 State the type of intrinsic defects would you predict in ﬂuorite-type CeO2 and UO2. 3.4 Recast Table 3.4 into one valid for a hypothetical MO oxide with cation-Frenkel intrinsic defects. 3.5 Use chemistry or physics to suggest whether ionic or electronic defects will dominate in pure ZrO2 at high temperatures. 3.6 Consider pure PbO with anion-Frenkel compensation and dominant ionic defects. What are the slopes of the essentially linear dependences in the three limiting regions of the plot of defect fractions versus pO2? Sketch the Brouwer diagram. 3.7 In fact, pure PbO may show an anti-Schottky disorder. What differences does this bring to the results of Problem 3.6? 3.8 Consider an idealized pure CuO with anion-Frenkel compensation and dominant electronic defects. What are the slopes of the essentially linear functions in the three limiting regions of the plot of defect fractions versus pO2? Sketch the Brouwer diagram. 3.9 State the limiting slope of the metal-vacancy fraction versus pO2 in the oxidativenonstoichiometry range for (a) Cu2O and (b) Cr2O3, both of Schottky intrinsic defects. 3.10 Consider a stoichiometric metal oxide of dominant Schottky defects in equilibrium. Which of these two defects will increase its fraction upon either an acceptor or donor doping under the same conditions? 3.11 Consider a stoichiometric metal oxide in equilibrium with its dominant electronic defects. Which of these two defects will increase its fraction upon an acceptor or donor doping under the same conditions? 3.12 Sketch the Brouwer diagram for Li-doped NiO with dominant electronic defects. 3.13 Sketch the Brouwer diagram for Al-doped NiO with dominant ionic defects. 3.14 Write down the dissolution reaction of ZrO2 in Cr2O3 and state how the solid solubility will depend on pO2: (a) about the point of integer structure, (b) about the point of integer valence. 3.15 The equilibrium constant in Equation (3.5) for oxidation of the oxygen vacancy in YBa2Cu3O7−δ at 500 °C is Kvox = 55 bar−½. (a) State the equilibrium composition of YBa2Cu3O7−δ at 500 °C in a ﬂow of Ar gas containing 100 ppm O2 and in air, both at 1 bar. (b) State the pO2 at which you would anneal YBa2Cu3O7−δ in order to obtain an average oxidation state of CuII.

116

Defect Chemistry and Nonstoichiometry

3.16 Derive the simpliﬁed expression for gross oxygen nonstoichiometry in NdBaFe2O5+δ as a function of pO2 assuming that Fe3+ deﬁnes the point of integer valence. 3.17 Water ﬂows from a 0.2 cm2 hose at 6 kg per minute. State the mass, volume, mole, and molecule ﬂux of H2O in SI units. 3.18 Calculate the mass ﬂux of carbon under steady-state diffusion through a steel plate separating carbon-rich and carbon-poor gases at 700 °C if subsequent analysis gives carbon concentrations of 1 kg/m3 and 0.5 kg/m3 at the respective depths of 0.5 mm and 1 mm below the surface. Assume 10−11 m2/s as the diffusion coefﬁcient of C in the iron matrix at this temperature. 3.19 An oxygen-permeable YBa2Cu3O7−δ membrane 1 cm thick operates at 700 °C between pressurized air at 11 bar and pure O2 at 1 bar. The steady-state O2 gas production is 0.84 mL at atmospheric pressure and 20 °C (molar volume 24 L/mol) per square meter every second. Calculate the O2 ﬂux, O atom ﬂux, and, ﬁnally, DO with Kvox = 4.3 bar−½ (to obtain the O gradient across the membrane) and with molar YBa2Cu3O7−δ volume of 10−4 m3/mol. 3.20 Consider a random 1D walk of n equal steps of length λ originating at zero. (a) What is the probability of deviating by 4λ from the origin in 4 steps? (b) Construct a table of probabilities of reaching points −nλ . . . + nλ for up to n = 4. (c) Calculate the variance (i.e. the mean squared deviation from the mean) and its root after 4 steps of unit length. (d) Derive a formula for the variance σn2 after n steps of length λ and for its root σn. 3.21 Calculate the jump frequency of interstitial carbon in bcc iron at 800 °C, assuming a vibration frequency ν = 1013 s−1 and an activation energy for hopping Δ‡Gm = 62 kJ/mol. On average, every x-th carbon vibration overcomes the jump barrier; determine x. 3.22 Assume that bcc iron at 1800 K has a fraction of vacant Fe sites of 0.0001, an Fe atom vibration frequency ν = 1013 s−1 and an activation energy for hopping Δ‡Gm = 29 kJ/ mol. What is the jump frequency of Fe atoms? On average, how many vibrations are there between jumps? What is the Fe progression rate at each site? 3.23 Calculate the self-diffusion coefﬁcient of Fe in Problem 3.22, given the unit-cell parameter a = 2.87 Å. 3.24 Given the diffusivity DC = 10−10 m2/s for interstitial carbon in bcc iron at 800 °C of a = 2.87 Å, estimate the activation energy Δ‡Gm for hopping of the C atoms (ν = 1013 s−1) via interstitial sites. 3.25 The self-diffusion coefﬁcient in Al (fcc; a = 4.05 Å) at 600 K is DAl = 2×10−16 m2/s. Assuming an atomic vibration frequency ν = 4×1013 s−1 and an activation energy for hopping Δ‡Gm = 58 kJ/mol, calculate the site fraction of Al vacancies. 3.26 Verify the statement in this chapter’s Footnote 32 that pdirλ2 = ℓ2/6 = a2/Nn, in which the distance a is the unit-cell edge, ℓ the actual jump length, λ its projection onto the unitcell edge direction, and Nn is the number of nearest neighbors of the vacancy, for (a) primitive cubic, (b) bcc, and (c) fcc packing of spheres.

3.4

Problems

117

3.27 Calculate the self-diffusion coefﬁcient in the primitive cubic α-Po (Figure 1.23; a = 3.36 Å) at 500 K via vacancy mechanism, assuming 0.001 vacant sites, ν = 1013 s−1, Δ‡Gm = 36 kJ/mol. Estimate the diffusivity of the vacancy. 3.28 Calculate the self-diffusion coefﬁcient of α-Po along the direction of the cell edge (Figure 1.23; a = 3.36 Å) at 500 K via an interstitial mechanism with full availability of interstitial sites, fc = 1, ν = 1013 s−1, and Δ‡Gm = 40 kJ/mol. Verify the result by orienting the cube to yield three equivalent jumps for positive progression direction and three for negative progression direction. 3.29 A single crystal of fcc iron (a = 3.6468 Å) having a few ppm of interstitial carbon is kept at 1000 °C and isolated from its surroundings. Assume DC = 2.217×10−11 m2/s for the self-diffusion coefﬁcient of interstitial carbon along a via octahedral holes, site availability pavail = 1, correlation factor fc = 1 for the interstitial, and atomic vibration frequency ν = 1013 s−1. (a) State the probability of a vibration of C becoming a jump. (b) State the total length of the path a carbon atom travels in one minute. (c) State that atom’s root mean square displacement from its position a minute earlier. (d) Calculate the hopping activation Gibbs energy per mole of interstitial carbon defects. 3.30 Conﬁrm by dimensional analysis in SI that multiplying Equation (3.23) with the charge qi yields mobility. 3.31 A rectangle of calcium-stabilized zirconia Zr0.85Ca0.15O1.85 (a = 5.13 Å) is covered with porous platinum electrodes on its opposite faces, heated to 1100 °C in air, and an electrical conductivity of 6 S/m is measured. Assuming t(vO••) = 1, calculate the diffusivity D(vO••) and mobility μ(vO••) of the oxygen vacancies in the bulk of the sample, neglecting kinetics of surface recombination. 3.32 Assuming that oxide-ion conductivity of YBa2Cu3O7−δ at 500 °C in air is σ(vO••) = 10−2 S/m and the ionic transference number t(vO••) = 10−6, what is the total electrical conductivity? 3.33 Calculate the enhancement factor DO/Dh• for Equation (3.34). 3.34 Use Equation (3.34) to generalize the value of the limiting ambipolar enhancement for DA of a neutral atom A, the ﬂux of which consists of a ﬂux of a z-charged ionic defect and a much faster ﬂux of singly charged electronic defects. 3.35 Figure 3.2 suggests that oxidative nonstoichiometry of NiO at high temperature is achieved via formation of nickel vacancies and holes. The following data have been measured [5, 6] at 1100 °C in O2: coefﬁcient of (tracer) random diffusion for nickel atoms DNi = 10−15 m2/s, total electrical conductivity σ = 65.5 S/m, site fraction 0.0001 of nickel vacancies. Assuming that Ni diffuses with a vacancy mechanism via nickel sites (never at O site), and given a = 4.20 Å for the NaCl-type cell, calculate for each of the two majority defects: (a) Concentration per m3, (b) diffusivity, (c) ionic electrical conductivity and ionic transference coefﬁcient in order to determine whether NiO is an ionic or electronic conductor, (d) mobility. 3.36 Set up the equation for the temperature dependence of DCr in oxidized Cr2O3 where chromium vacancies dominate.

118

Defect Chemistry and Nonstoichiometry

pﬃﬃﬃﬃﬃﬃ 3.37 Check that u = (y/2)/ Dτ of Equation (3.39) is dimensionless. 3.38 A steel blade has been nitridized by exposure to ﬂowing NH3 at 700 pﬃﬃﬃﬃﬃﬃ°C for 1 hour. The hardened layer, estimated from the penetration depth Dτ of the nitrogen atoms, is 20 μm. In what time would the penetration depth reach 0.1 mm? 3.39 Nitridized steel is hard yet brittle, and this means that the bulk of a steel object must remain free of nitrogen. Assuming D = 10−9 cm2/s for interstitial diffusion of nitrogen in steel at 700 °C, estimate the minimum thickness of the above steel blade such that the nitrogen concentration at its center would increase by no more than 0.005 of the surface change under 1 (alternatively 25) hour(s) of nitridization. Assume for simplicity that the concentration at the center is twice the concentration that would be caused by nitridization from one side only (in reality it will be less than twice due to decreasing gradient after the two ﬂuxes penetrate each other). 3.40 At 700 °C, an YBa2Cu3O7−δ sphere of 2 cm radius is abruptly exposed to 1 bar O2 gas. Assuming DO = 10−5 cm2/s and diffusion as the rate-controlling process, calculate how long it will take before 90% of the total oxidation change occurs 1 mm below the surface. Under these conditions, the sphere center will oxidize by less than 1%, so that the sphere can be approximated as an inﬁnite half-space.

3.5

Further Reading P. Kofstad, “Non-Stoichiometry, Diffusion and Electrical Conductivity in Binary Metal Oxides” (1972) Wiley. J. Crank, “The Mathematics of Diffusion” 2nd edition (1975) Clarendon Press. S. Mrowec (translated to English by S. Marcinkiewicz), “Defects and Diffusion in Solids” (1980) Elsevier. D.M. Smyth, “The Defect Chemistry of Metal Oxides” (2000) Oxford University Press. D.S. Wilkinson, “Mass Transport in Solids and Fluids” (2000) Cambridge University Press. J. Maier, “Physical Chemistry of Ionic Materials” (2004) Wiley. H. Mehrer, “Diffusion in Solids” (2007) Springer. J.-M. Missiaen, “Solid-state spreading and sintering of multiphase materials” Mater. Sci. Eng. A 475 (2008), 2–11. P. Heitjans, J. Kärger (editors), “Diffusion in Condensed Matter, Methods, Materials, Models” 3rd edition (2011) Springer.

3.6

References [1] G. Brouwer, “A general asymptotic solution of reaction equations common in solid-state chemistry” Philips Res. Rep. 9 (1954), 366–376.

3.6 References

119

[2] J.C. Schön, I.V. Pentin, M. Jansen, “Ab initio computation of low-temperature phase diagrams exhibiting miscibility gaps” Phys. Chem. Chem. Phys. 8 (2006), 1778–1784. [3] P. Karen, “Nonstoichiometry in oxides and its control” J. Solid State Chem. 179 (2006), 3167–3183 (and references therein). [4] P. Schleger, W.N. Hardy, B.X. Yang, “Thermodynamics of oxygen in YBa2Cu3Ox between 450 °C and 650 °C” Physica C 176 (1991), 261–273. [5] W.C. Tripp, N.M. Tallan, “Gravimetric determination of defect concentrations in NiO” J. Am. Ceram. Soc. 53 (1970), 531–533. [6] M.L. Volpe, J. Reddy, “Cation self-diffusion and semiconductivity in NiO” J. Chem. Phys. 53 (1970), 1117–1125.

4

Phase Diagrams and Phase Transitions

In this chapter we will consider two separate but related topics; phase diagrams and phase transitions. Phase diagrams are used throughout materials chemistry to guide the synthesis of known and new materials. Electronic and magnetic phase diagrams are used to help summarize the properties of functional materials under different conditions. We’ll see throughout the later chapters of this book that many functional materials undergo structural phase transitions that are intimately linked to their properties. The second half of this chapter will introduce the fundamental concepts needed to understand these.

4.1

Phase Diagrams Phase diagrams provide a graphical summary of the behavior of chemical systems at equilibrium as a function of external variables. In materials chemistry, these variables are usually composition, temperature, and pressure, but could also include effects such as electric or magnetic ﬁeld. These diagrams are based on the phase rule ﬁrst proposed by Gibbs, which states that for a system in equilibrium: PþF ¼Cþ2

(4.1)

where P is the number of phases, F the degrees of freedom or variance, and C the number of components.1 We can deﬁne the system as being the part of the universe that we’re interested

1

120

The derivation of this rule is relatively straightforward and is covered in many physical chemistry texts. Brieﬂy, to describe the state of a system consisting of P phases, you need temperature, pressure (two variables), and (P·C) − P mole fractions for P phases of C components each (−P appears because the sum of mole fractions of each phase is one, hence one fraction per phase is redundant). There are then a total of 2 + (P·C) − P variables. For phases at equilibrium, chemical potentials for each component must be equal. This gives C(P − 1) independent equations (conditions). The number of variables that still remain free to vary is F = 2 + (P·C) − P − C(P − 1), which can be rearranged to the equation given.

4.1

Phase Diagrams

121

critical point

pressu re (ba r)

220.5

Solid e

d b c

Liquid a

normal boiling point

1.01 normal melting point

Vapor

-3

6x10

triple point 0 0.0098 temperature (ºC)

100

374.4

Figure 4.1 Schematic phase diagram of water.

in, anything else is the surroundings. It is easiest to understand the various terms in the phase rule through examples. Gibbs deﬁned a phase as a state of matter that is uniform throughout in terms of both its chemical composition and its physical state. It thus represents a homogeneous part of the chemical system that is bounded by a surface such that it can, at least in principle, be separated from other parts of the system. To take the simple example of H2O (Figure 4.1) ice, water, and steam are individual phases—each is homogeneous and each could potentially be separated from the other; crystals of ice dispersed in liquid water is therefore a twophase system.2 If we consider a mixture of two metals A and B where A forms a dispersion of droplets within B, it is a two-phase system. If A and B form a solid solution in which atoms are homogeneously mixed on an atomic length scale, it is a one-phase system. For a material such as SiO2, which displays polymorphism and has more than one structural form in the solid state (e.g. the quartz, tridymite and cristobalite modiﬁcations), each form is a different phase. We can deﬁne the components of a system as the minimum number of independently variable chemical constituents that we need to deﬁne the overall composition. The H2O phase system, for example, contains a single component because H2O has a ﬁxed chemical formula. Our two metals A and B would be a two-component system. Al2O3 and SiO2 can also be considered a two-component system if we take Al2O3 and SiO2 as having ﬁxed composition (no nonstoichiometry).3 This particular two-component system contains three phases: Al2O3, SiO2, and the compound Al6Si2O13 (often expressed as 3Al2O3·2SiO2 on phase diagrams). 2 3

Throughout this chapter, for reasons of pedagogical clarity, single-phase areas in phase diagrams are shaded in gray. With nonstoichiometry considered, Al2O3 and SiO2 would become part of a three-component system; Si, Al, O.

122

Phase Diagrams and Phase Transitions

The number of degrees of freedom can be formally deﬁned as the number of variables (pressure, temperature, concentration of components) that need to be speciﬁed to fully deﬁne the condition of the system. This can be understood with reference to the phase diagram of water (a one-component system) in Figure 4.1. If we consider a general point on the phase diagram, we have a single phase (P = 1) present—liquid water for the point labeled a, ice at point e. For a one-component system, C = 1. The phase rule tells us that the number of degrees of freedom, F, is C − P + 2 = 2. At a point like a, we can thus vary both the temperature and the pressure of the system independently of each other, meaning both have to be speciﬁed to deﬁne the system. We therefore see that on a single-component phase diagram like this, a single phase exists over an area.4 If we cool the system until we reach point b, which is the freezing point of water at the pressure under consideration, we reach the phase boundary between water and ice represented by the almost vertical solid line. At this point, two phases (liquid water and ice) are in equilibrium and will remain so indeﬁnitely. The phase rule says that F = 1 + 2 − 2 = 1, and we therefore need to specify only one variable to deﬁne the system. We can change pressure and temperature and retain two phases but we can’t change them independently without destroying one phase or the other. If we increase T, we must decrease p to compensate (i.e. move to point c); if we decrease T, we must increase p (i.e. move to point d). We can see from the phase rule why, when water freezes to ice at constant pressure, the temperature of the system remains constant as long as both ice and water are present and in equilibrium.5 At the so-called triple point, one has three phases (ice, liquid water, and water vapor) in equilibrium, and F = 1−3 + 2 = 0. If one changes either p or T, one phase will disappear, so no variables have to be speciﬁed to deﬁne the system. This is an example of an invariant point; one with no degrees of freedom. A line on the H2O phase diagram thus represents the presence of two phases, and a point where three lines intersect represents three phases. The ﬁnal point to mention on the water phase diagram is the critical point, which occurs at the critical temperature and critical pressure. Beyond this point, liquid and vapor have the same density and can’t be distinguished—a supercritical ﬂuid is the only phase present. A practical consequence is that above the critical temperature, gas can’t be liqueﬁed by application of pressure alone. As the focus of this text is on solid state materials, the majority of the chemical systems that we’ll consider will be condensed systems, i.e. ones in which the vapor pressures of the substances involved are negligible compared to atmospheric pressure. The pressure can therefore be considered as constant, and one degree of freedom is removed from the system. The phase rule for a condensed system becomes:

4

5

Note that this is not the case in a phase diagram with two or more components. In a two-component diagram, a single solid phase is represented by a line and in a three-component diagram by a point. In practice, remaining at equilibrium means using a slow cooling rate. With more rapid cooling, one may not allow time for crystallites of ice to nucleate and thus obtains a supercooled state. This, however, is not an equilibrium state of the system.

4.2

Two-Component Phase Diagrams

123

PþF ¼Cþ1

(4.2)

This is the form of the phase rule that will apply for the rest of this chapter.

4.2

Two-Component Phase Diagrams

4.2.1 Without Compound Formation Figure 4.2 shows one of the simplest phase diagrams for a two-component (A and B) or binary condensed system, a system in which A and B form no compounds AmBn. Components A and B form no solid solutions (x is either zero or one in A1−xBx) but are completely miscible when molten. The y axis represents the temperature of the system and the x axis the composition. Composition throughout this chapter is expressed in mole fraction (0 to 1), though mole percents are also in common use.6 The left-hand y axis of Figure 4.2 then corresponds to pure A, and we can read from this axis that A melts at T4; the right-hand axis represents pure B, which melts at T5. There are four main regions on this phase diagram. At low temperature, as A and B form no compounds and no solid solution, one has a two-phase region consisting of a mixture of pure A and pure B solids. When the solid two-phase mixture is heated to temperatures just above T1, one obtains a mixture of either solid A and liquid, or solid B and liquid, depending

T4

temperature

Liquid A + Liquid

B + Liquid

a q p

c

A 1.0

0.2 0.4 0.6 mole fraction B, xB 0.8

0.8

0.6 0.4 0.2 mole fraction A, xA

(a)

1.0

A

e

F

b T5

m

T3 l

j solidus

f

A+B 0.0

liquidus k

g

E K

J

T2

d T 1

B

B 0.0

(b)

Figure 4.2 (a) The phase diagram for a binary system of A and B that form no compounds and no solid solution. (b) The same phase diagram but with labels for speciﬁc points discussed in the text. Single-phase areas are shaded, two-phase areas unshaded. 6

Mole percents are just mole fractions ×100. In some ﬁelds (particularly phase diagrams used industrially), the composition axis may be expressed in weight percent.

124

Phase Diagrams and Phase Transitions

on whether the composition lies to the left or right of composition E. At composition E, the solid mixture melts directly to form a liquid at point e, called the eutectic point, which represents the lowest melting temperature in the system. Line cd (Figure 4.2b) where the ﬁrst liquid appears is called the solidus. At temperatures above those deﬁned by the line aeb (called the liquidus), one enters a region where the system is fully molten into a single-phase liquid. When interpreting such phase diagrams, it is crucial to realize the difference between a two-phase and a one-phase region. For a one-phase region (shaded), each point on the diagram represents a certain state of the phase in terms of composition and temperature. For example, one can form a liquid with any desired composition at any temperature above the liquidus. For two-phase regions the situation is very different. An arbitrary point in a twophase region does not represent an actual state of a phase, but corresponds to the overall composition of two phases in equilibrium. At point f in Figure 4.2b (whose composition is marked as F on the composition axis), one has a two-phase mixture of pure A and pure B. The relative amount of each phase present can be read directly from the composition axis. Equivalently (and to prepare ourselves for later diagrams), we can see that the mole fraction of A present, xA, is given by (distance F to B)/(distance A to B) (i.e. FB/AB) and xB as AF/ AB. Similarly, point j on the diagram contains a mixture of pure B and a liquid. The composition of the liquid present is given by point k on the diagram (i.e. xA ≈ xB ≈ 0.5). The solid present is pure B and represented by point l. The relative amounts of liquid of composition K and pure B present can be determined straightforwardly by the lever rule. Let’s label the fraction of pure liquid present as xL and the fraction of pure B as xB. The lever rule7 states that: xL kj ¼ xB jl

(4.3)

i.e. the relative amount of B and liquid is given by: xB =xL ¼ kj=jl

(4.4)

Since we know xL + xB = 1, we can eliminate xL from Equation (4.3) to give the mole fraction of B as: xB ¼ kj=ðjl þ jkÞ ¼ kj=kl

(4.5)

Note again that the amount of B present is proportional to the distance (kj) further from pure B. Let’s consider what happens when you cool a liquid of a given composition. Firstly, let’s consider a liquid of composition E (xA ≈ 0.6, xB ≈ 0.4) on our diagram. This liquid has the special property of transforming directly to two solids on cooling at the eutectic point e. No region of mixed solid and liquid phases exists. Since three phases (A, B, and liquid) are 7

This can be likened to balancing two masses at different distances from a pivot. At balance, m1d1 = m2d2 where m1 and m2 are the two masses and d1 and d2 the distances to the pivot.

4.2

Two-Component Phase Diagrams

125

present at e, the number of degrees of freedom is zero (F = C + 1 − P = 2 + 1 − 3 = 0), and this tells us that the eutectic point e is invariant.8 The behavior of other compositions is more complex. Consider the composition J (xA ≈ 0.35, xB ≈ 0.65) initially at point g. When the liquid is cooled to T3, one meets the liquidus curve at point m where an inﬁnitesimally small amount of pure B will form. Solid B will be in equilibrium with liquid of composition J at this point. On further cooling to T2 we reach point j. One still has a liquid in equilibrium with pure B, but the composition of the liquid has changed to K—it has become richer in A. The relative amounts of solid and liquid present are given by the lever rule as kj/jl as discussed above. Note that although the liquid and solid have different compositions, the overall composition of the system does not change. As one continues to cool, the liquid composition follows the line ke until at temperature T1 the ﬁnal liquid of composition E crystallizes. Below T1 one forms a solid mixture of A and B of the original overall composition. The system will follow this pathway if cooled under equilibrium conditions. If the system is rapidly cooled, it may follow a different pathway, but the ﬁnal phases present would be the same. We can also use Figure 4.2 to understand the effect that solid impurities have on melting points. A sample of pure B at temperature T3 will be a solid (B doesn’t melt until the higher temperature T5). However, if a small amount of A is added, the solid will be in equilibrium with a small amount of liquid at point m (composition J, xA ≈ 0.35, xB ≈ 0.65); i.e. a small portion of B will have dissolved in the liquid. If sufﬁcient A is added so that the overall composition becomes J, then all of B will dissolve. The impurity A has lowered the melting point from T5 to T3. Since at this point B has just dissolved, we have a saturated solution of B in A. As we continue to add A at this temperature, we retain a single-phase liquid until we reach point p on the liquidus. At this point, a small amount of solid A will form. As more A is added, the amount of solid will increase and liquid decrease until at point q we have pure solid A present. The point p represents a saturated solution of A in B. Since ae and eb represent saturated solutions of A and B, respectively, point e represents a liquid saturated in both solids. The use of one solid to lower the melting point of another is the reason why salt is spread on roads to prevent ice formation. It’s also of great practical use in the growth of crystals from a ﬂux at lower temperatures than would otherwise be required. Fluxes are chosen to be easily separable from the crystals of interest, for example by dissolution in water in the case of NaCl/KCl ﬂuxes.

4.2.2 With Compound Formation Most of the systems we’ll meet in materials chemistry will be more complex than Figure 4.2— components that undergo reactions in the solid state leading to new materials are far more interesting and exploitable than those that don’t! Figure 4.3 shows three possible phase 8

Terms univariant and bivariant are used for F = 1 and F = 2.

126

Phase Diagrams and Phase Transitions

diagrams in which A and B can react to form an intermediate phase AB2. This phase occurs as a vertical solid line on the phase diagram at xA = ⅓, xB = ⅔. Note that for composition calculations it is often more convenient to express the formula of AB2 as A1/3B2/3 (a normalized or pseudoatom formula). Figure 4.3a shows the most straightforward system. Each of the solid phases A, AB2, and B melts to form a liquid without decomposition (at temperatures T2, T1, and T3, respectively, on the diagram); they are said to have a congruent melting point. The phase diagram is then very similar to that of the simple eutectic system in Figure 4.2. In fact, it can be considered as two eutectic systems placed side by side. Figure 4.3b shows a situation in which the compound AB2 is only stable up to a temperature T1 above which it decomposes without melting to solid A and B. Above this temperature, the diagram is again essentially identical to Figure 4.2. Other systems show the reverse behavior, i.e. compounds are only stable above a certain temperature. ZrW2O8 of Figure 4.8 is one such example (see later). Figure 4.3c represents a more complex situation in which AB2 has an incongruent melting point, that is, it melts to give a solid and a liquid of different chemical compositions. On heating AB2 to T2, it decomposes to give a liquid of composition corresponding to point p and pure B; the relative amounts are given by the lever rule. On further heating, B will gradually dissolve in the melt and the liquid will move in composition from p to r. At point r, all the solid dissolves/melts and a single liquid phase results. At point p, three phases are in equilibrium (liquid, AB2, and B), F = C − P + 1 = 0, and p is therefore an invariant point. As can be seen from Figure 4.3c, the composition of point p lies outside the composition range of AB2 to B. The composition of the liquid phase therefore can’t be expressed in terms of positive quantities of the solid phases with which it is in equilibrium. Such a point is called a peritectic point. At a peritectic point there is no minimum in the melting curve as there is at the eutectic point, only a kink. Systems in which a compound melts incongruently follow relatively complex pathways on cooling. Consider a liquid at point s on Figure 4.3c. On cooling, the liquidus is met at t, and liquid and solid B will be in equilibrium. As cooling continues towards T2, the liquid will move in composition from t to p. At temperatures just below the peritectic point p, the stable solid phase becomes AB2. To form this solid, a peritectic reaction must occur, in which all the solid B present must react with the liquid to form solid AB2. A drastic change in the composition of solids present will therefore occur for a very small temperature change. The amount of liquid present also changes dramatically at T2. Just above T2 the lever rule shows the system will contain largely liquid (xL ≈ 0.86 given by uB/pB) and just below T2 far less liquid (~0.36, uAB2/pAB2). On further cooling, the liquid composition follows curve pe, and, at temperatures below T1, solid A forms along with solid AB2. From the complexity of this behavior, it should not be surprising that systems containing phases that melt incongruently frequently show non-equilibrium behavior. If liquid at point s is cooled rapidly and/or if solid B falls to the bottom of the crucible during cooling such that it is essentially removed from the system, the peritectic reaction may not have time to occur completely and one would therefore observe a non-equilibrium mixture of A, AB2, and B at

4.2

Two-Component Phase Diagrams

(a)

127

T3 T2

temperature

Liquid T1

B+ Liquid

A + Liquid

AB2 + Liquid AB2 + B

A + AB2

0.0

0.2

0.4 xB

A

0.6

0.8

1.0

B

AB2

(b) t empera tur e

Liquid A + Liquid

B + Liquid

A+B T1

A + AB2 0.0

0.2

0.4 xB

A

AB2 + B 0.6

0.8

1.0

B

AB2

(c) s

t empera tur e

Liquid r

t p

A + Liquid

u

e

AB2 + B

A + AB2

A

T2

AB2 + Liquid

T1

0.0

T3

B + Liquid

0.2

0.4 xB

0.6

0.8

AB2

1.0

B

Figure 4.3 Two-component phase diagrams containing an intermediate phase AB2: (a) AB2 stable to its melting point. (b) AB2 decomposes to solid A and B before melting. (c) AB2 decomposes on melting.

128

Phase Diagrams and Phase Transitions

low temperature. It should also be clear that if one wants to grow crystals of composition AB2 from the melt under equilibrium conditions, one should start with a liquid composition between e and p.

4.2.3 Solid-Solution Formation We learned in Chapters 2 and 3 that solid solutions are ubiquitous. A schematic phase diagram for a two-component (C = 2) system that shows complete solid solution in both the liquid and solid states is shown in Figure 4.4. At high temperature (above the liquidus), one has a single liquid phase and F = C + 1 − P = 2; at low temperature (below the solidus), one has a single solid phase and F = 2. In both regions, either temperature or composition can be varied without changing the number of phases present. Between these two extremes, one has a two-phase region in which (since F = 1) the composition of the liquid and solid phases is ﬁxed by the temperature of the system. Consider what happens when a liquid with composition and temperature corresponding to point c is cooled under equilibrium conditions. At point dℓ, the liquid of composition dℓ will be in equilibrium with a solid of composition ds, one richer in B than the starting composition. On cooling to T3, the liquid will have composition eℓ (richer in A) and the solid es (richer in B); the relative amounts of solid and liquid will be given as eℓe/ese by the lever rule—approximately equal amounts as drawn. As one cools further, the liquid becomes progressively richer in A (it follows curve dℓ fℓ), and the amount of liquid relative to solid decreases. Simultaneously, the solid composition changes from ds to fs. At T1, one has a single solid phase with the same composition as the original liquid. The description above again holds only under ideal equilibrium conditions, which would be very hard to achieve in practice. On more rapid cooling, it is very likely that the B-rich

c

Liquid

dl

temperature

el

liquidus

fl

solidus

T4 T3

ds

e

es

T2

fs

Solid g

0.0

A

0.2

0.4

0.6

mole fraction B, xB

T1 0.8

1.0

B

Figure 4.4 Phase diagram for a two-component system showing complete solubility in both solid and liquid states.

4.2

Two-Component Phase Diagrams

129

tempera ture

Liquid

Ass

Ass + Liquid

Bss + Liquid Bss

f g

d

e

T1

h

Ass + Bss c 0.0

A

0.2

0.4 0.6 mole fraction B, xB

0.8

1.0

B

Figure 4.5 Phase diagram for a two-component system in which a limited range of solid solutions is formed.

crystals formed initially wouldn’t have sufﬁcient time to fully equilibrate with surrounding liquid. One would then expect crystals whose core is rich in B (compositions as high as ds) and outer shell rich in A (compositions as A-rich as fℓ). Such effects are frequently observed in mineralogy. For many applications, the range of compositions from the core to the outside of the crystal may give rise to deleterious properties, and extended annealing periods may be required to homogenize samples. A full range of solid solutions as shown in Figure 4.4 would only be expected for components that are chemically very similar, and few phase couples have full thermodynamic miscibility at very low temperatures.9 In most systems at equilibrium, one observes partial solid solution; there is a limit of solubility at a given temperature. Figure 4.5 shows a typical phase diagram for a two-component system in which no compounds form but there is solid solution at either end of the composition range. The diagram is directly related to Figure 4.2a. At the left-hand side of the diagram, we have a region in which A will dissolve B to form a single-phase solid solution A1−xBx (labeled Ass). The range of solubility generally increases with temperature (curve cdf ) and reaches a maximum at the solidus temperature T1. A similar region exists at the B-rich side of the diagram (Bss). At temperatures below T1, these regions are separated (the boundary is called the solvus) by a two-phase region containing a mixture of Ass and Bss. The composition corresponding to any point on this diagram can be found using the same rules we’ve used above. Point g, for example, has an overall composition of xA ≈ 0.7, xB ≈ 0.3; there will be two phases present, Ass and Bss. As drawn, Ass will have composition d (A0.9B0.1) and Bss composition h (A0.05B0.95). The mole fractions of each of the two phases as given by the lever rule are gh/dh for Ass and dg/dh for Bss

9

Many solid solutions can be quenched from high temperatures and remain stable at low temperatures because of slow kinetics of demixing.

Phase Diagrams and Phase Transitions

c

Single Liquid temperature

130

T1

e

f

g

T2

Two Liquids

Ass

Ass + Liquid

a

B + Liquid

d

b

AASS++BB

0.0

A

0.2

0.4

0.6

mole fraction B, x B

0.8

1.0

B

Figure 4.6 Phase diagram for a two-component system with limited solid-solution range for A and liquids rich in A and B immiscible under certain conditions.

(~0.765 A0.9B0.1 and ~0.235 A0.05B0.95). Note that (0.765 × 0.9) + (0.235 × 0.05) = 0.7 and (0.765 × 0.1) + (0.235 × 0.95) = 0.3, as expected for the overall composition. In the two examples described above, the components have been fully miscible when molten and therefore form a single liquid phase. This is not, however, always the case, and we’re familiar in everyday life with oil and water forming two-phase liquid systems. Liquid immiscibility is also encountered in ceramic phase diagrams. The example in Figure 4.6 shows an immiscibility dome inside which two liquids exist as separate phases. Point e, for example, will correspond to a mixture of two liquids of compositions corresponding to f and g. Temperature T1 is called the upper consolute temperature. Along the line abd, two liquids (compositions at a and b) and a solid (pure B) are in equilibrium. Point b is an invariant point (three phases are present) called a monotectic point. It is similar to the eutectic point, except that one of the phases that forms is a solid (here pure B) and the other a liquid (composition at a). When we discussed the formation of compounds in Section 4.2.2, we moved from simple eutectic phase diagrams such as Figure 4.2 to the more complex diagrams of Figure 4.3. Each of these diagrams can be readily extended to allow for the formation of solid solutions in the same manner as described above. For example, the incongruently melting system of Figure 4.3c becomes Figure 4.7. While they appear complex at ﬁrst glance, we can use the same ideas as described above to read such phase diagrams. A real-world A–B binary system that combines many of the ideas discussed above is shown in Figure 4.8 for ZrO2–WO3. The system exhibits two structural forms of ZrO2 (monoclinic and tetragonal structures) over the temperature range depicted, each of which shows a small range of solid solution. There is a single AB2 compound ZrW2O8 that is only thermodynamically stable above 1105 °C, melts incongruently, and has a peritectic point at 1257 °C. This system is discussed further in the end-of-chapter problems.

4.3

Three-Component Phase Diagrams

131

tempera ture

Liquid Bss + Liquid Ass + Liquid

AB2 ss + Liquid

Ass

Ass + AB2 ss 0.0

0.2

AB2 ss

Bss

AB2 ss + Bss

0.4 0.6 mole fraction B, xB

A

0.8

1.0

B

Figure 4.7 Phase diagram for a simple binary system with one intermediate phase AB2 and a range of solid solutions for each solid phase.

ZrO2 tempera ture (ºC)

1400 1300

1200 1100

ss tet

ZrW2O8 + Liquid ZrO2 ss tet + Liquid

ZrO2 ss tet + ZrW2O8 ZrO2

ss mon

Liquid

WO3 + Liquid

ZrW2O8 + WO3

+ ZrW2O8

1000 900 0.0

ZrO2

ZrO2

ZrO2

ss mon

+ WO3

ss mon

0.2

0.4 0.6 mole fraction WO3

0.8

1.0

WO3

Figure 4.8 Partial phase diagram for the ZrO2–WO3 system at ambient pressure, after [1].

4.3

Three-Component Phase Diagrams For a three-component or ternary system, we would need ﬁve axes (one for each composition and one each for p and T ) to draw a general phase diagram. In practice, an equilateral triangle is used to represent the composition of the system, and temperature is represented by an axis normal to this triangle, forming a prismatic diagram (Figure 4.9). One such prism is required for each pressure of interest. The side faces of the prism represent the binary phase diagrams we’ve already discussed. Due to the complexity of drawing and reading such diagrams, it is far more common

Phase Diagrams and Phase Transitions

tem per atur e

132

A +L

liquidus surface

C +L

B+ L B +L

A+B B+C A

C

B

Figure 4.9 A phase diagram for a three-component eutectic system.

to depict an isothermal section of the prism (Figure 4.10), which represents the phases present at a speciﬁed temperature and pressure. In this chapter, we will only discuss sub-solidus ternary diagrams and not address crystallization pathways for these systems. The reason for using an equilateral triangle for such phase diagrams is that its geometry provides a natural way of expressing mole fractions xA, xB, xC of the three components, which must, by deﬁnition, sum to 1. This arises from the fact that if you take any point in an equilateral triangle and draw lines from it to intercept each edge at right angles then the sum of the length of these lines is equal to the height of the triangle (Viviani’s theorem). If, as in Figure 4.10a, we draw such a triangle and call its height 1 then the distances marked xA, xB, and xC will always sum to 1. One corner of the triangle represents pure A (the others are B and C), and lines drawn parallel to the opposite edge moving towards that corner represent increasing mole fractions of A. This is shown in Figure 4.10a where each of the dashed lines represents a constant mole fraction of A, with the amount of A increasing as one moves from edge CB towards corner A. If we consider point d, it lies on the line representing xA = 0.6. If we were to draw lines parallel to the other edges, d would lie on lines corresponding to xB = 0.3 (lines parallel to the AC edge) and xC = 0.1 (lines parallel to AB). A second way of determining composition is to use the triangle rule, which is the equivalent of the lever rule we used for binary systems. In Figure 4.10b we draw lines from each corner of the triangle through d to the opposite edge. The amount of each component is given by: xA ¼ q=ð p þ qÞ; xB ¼ s=ðr þ sÞ ¼ 0:3; xC ¼ u=ðt þ uÞ ¼ 0:1:

4.3

A

(a)

Three-Component Phase Diagrams

A

(b) 0.8

cC

s u

0.4

0.6

d

fra cA

0.4

0.8

p

mo le

fra

0.6

xC

d

0.2

le mo

xB

0.6

0.4

xA

t 0.2

C

B

133

q

r

0.8

0.2

C

0.2

0.4

0.6

B

0.8

mole frac B

A

(c)

0.8

fra mo le

mo le

d

0.4

xC

0.6

cA fra

cA

0.6

xB

0.4

le mo

0.6

fra

d

f

cC

e 0.4

0.8

0.2

le mo

cC

0.2

fra

A

(d)

0.6

AC2

0.4

xB'

h 0.8

0.2

0.8

e

xC'

0.2

g

C

0.2

0.4

0.6

mole frac B

0.8

B

C

0.2

0.4

0.6

0.8

B

mole frac B

Figure 4.10 Isothermal sections for a three-component system; (a) shows how the mole fraction of a phase increases as one moves towards the corresponding corner, (b) illustrates the triangle rule for determining composition, (c) illustrates how composition can be read from a single axis, and (d) shows a line corresponding to a constant B:C ratio.

A third way of reading compositions, which is often the most useful in practice, is to read the amount of each component directly from one axis. To do this, we take point d in Figure 4.10c and draw dashed lines through it parallel to each edge of the triangle and look where these lines intercept any edge. If we consider edge AB, then the mole fraction of A is given by f B (as in two-component phase diagrams, the length “furthest” from pure

134

Phase Diagrams and Phase Transitions

A gives its mole fraction), xB as Ae, and xC is the remaining portion of the axis, namely ef. This method is particularly useful as it also applies to scalene10 triangles. If, in the system of Figure 4.10c, A and C can react to form an intermediate phase AC2 (or A1/3C2/3 when normalized), then we might want to consider just the subsystem formed by A, B, and AC2. This is represented by the triangle A–B–AC2 in Figure 4.10c. We could redraw this subsystem as an equilateral triangle to read off the composition of point d in terms of A, B, and AC2. However, our original diagram lets us read this information directly. To do this, we can use edge B–AC2 as we already have construction lines (eh and dg) drawn parallel to the other two edges, and composition can be read from the interception of these lines with B–AC2. The mole fraction of AC2 is given by Bg/(B–AC2), the mole fraction of B by (h–AC2)/(B–AC2) and the mole fraction of A by gh/(B–AC2). These can be measured from the diagram as xA1/3C2/3 = 0.15, xB = 0.3, xA = 0.55 (using the normalized formula for AC2). Note that multiplying each mole fraction with the phase composition gives an overall A:B:C ratio of 0.6:0.3:0.1, as expected. One can see intuitively from these diagrams that the closer a point lies to a given corner, the richer the composition is in that component. In fact, for points d and e of Figure 4.10d, which lie on a straight line Ade, the ratio xB/xC = xB 0 /xC 0 , and the dashed line Ae therefore shows the effect on a system of increasing the amount of A at a ﬁxed B:C ratio. This is true for any set of compositions that lie on a straight line linking them to a corner. The sub-solidus phase diagrams in Figure 4.11 are for the relatively simple Al2O3–TiO2 –ZrO2 system and the more complex Y(O)–Ba(O)–Cu(O) system,11 in which the famous YBa2Cu3O7 superconductor is found. In the second system, the (O) brackets imply that the oxygen content in some phases on the diagram can be variable (redox behavior of Cu). In Figure 4.11a, only binary and ternary oxides are formed (all compounds are points on the edges of the main triangle); in Figure 4.11b quaternary oxides also form. The phases present for any overall composition can be read in a similar way as for binary phase diagrams. A point within any single triangle represents a mixture of the three solid phases at its corners (the amounts of which can be found using the rules above). The edge of any triangle represents a mixture of the two phases at the corners it links, and a vertex represents a single phase. Thus under the conditions corresponding to Figure 4.11b, a certain amount of the YBa2Cu3O7 phase12 (labeled 123 for the Y:Ba:Cu ratio) will be formed from starting compositions anywhere within the triangle enclosed by points labeled CuO, 211, and BaCuO2. Pure material will only be formed using the correct 1:2:3 Y:Ba:Cu ratio. In practice, as we discussed for binary phase diagrams, many systems form solid solutions. These would be represented by an area located around an ideal stoichiometric point.

10 11

12

A scalene triangle is a triangle with no equal sides. Note that in Figure 4.11a the compositions are in mole fractions of Al2O3, whereas in Figure 4.11b in mole fractions of YO1.5. Al2TiO5 (2:1 Al:Ti) therefore lies halfway along the edge joining Al2O3 and TiO2 in Figure 4.11a, whereas Y2Cu2O5 (1:1 Y:Cu) lies halfway along the edge joining Y(O) and Cu(O) in Figure 4.11b. Though the oxygen content may not be exactly 7; see Chapters 3 and 12.

4.4

(a)

ZrO2

TiO

le mo

2

CuO

fra c

c fra

ZrTiO4

Y2Cu2O5

123

ZrO

mo le

a

2

e

BaCuO2 143 Ba2CuO4

211

f

135

Cu(O)

(b)

c b

Structural Phase Transitions

163

d Al2TiO5

Y2O3

Al2O3

TiO2

Y(O)

BaO BaY2O4

Ba3Y4O9

Ba(O)

mole frac Al2O3

Figure 4.11 Isothermal sub-solidus phase diagrams (neglecting minor solid solubilities) for (a) TiO2–Al2O3–ZrO2 below 1580 °C [2] and (b) Y(O)–Ba(O)–Cu(O) at 900 °C in O2 [3].

4.4

Structural Phase Transitions In the ﬁrst half of this chapter, we have explored the phase diagrams of a number of simple systems. The concept of phase transitions was implicit to this discussion. In Figure 4.1, for example, as we heat from point e to point a, there is a phase transition from solid ice to liquid water. Many materials undergo phase transitions in the solid state where their structure changes. For example, when α-quartz13 is heated, it undergoes a series of phase transitions. At 573 °C (the transition temperature or critical temperature, Tc), a relatively subtle transition to β-quartz occurs, in which the connectivity of the SiO4/2 tetrahedra is unchanged (i.e. no chemical bonds are broken or formed), but the tilting pattern of tetrahedra changes and the symmetry increases from trigonal to hexagonal. On further heating, more drastic modiﬁcations occur in which the bonding pattern changes; at 870 °C, a transition to β-tridymite and, at 1470 °C, to β-cristobalite. The α- to β-quartz transition can be classiﬁed as a displacive phase transition, because no bonds are broken or formed. The higher temperature transitions are classiﬁed as reconstructive because they entail a major reorganization of the structure involving bond breaking and formation.14 The ﬁnal category of phase transition we’ll encounter is order‒disorder transitions. Order‒disorder transitions can be further 13 14

Polymorphs are often distinguished by Greek letters α, β, γ, etc. These different classiﬁcations aren’t used uniformly in the literature. For example, we describe a transition as displacive if atoms only move a short distance, no chemical bonds need to be broken to achieve the conversion, and there is a group–subgroup relationship (Appendix B) between the two space groups, regardless of whether the process occurs in an abrupt or continuous fashion. Others choose to restrict the term displacive to continuous phase transitions.

136

Phase Diagrams and Phase Transitions

subdivided into substitutional disorder (for example atoms ordering on speciﬁc lattice sites such as the FePt example in Section 4.4.2) and orientational disorder where atoms or groups of atoms change their positions without breaking the fundamental bonding pattern of the material (such as the phase transitions of C60 described in Chapter 13). We’ll see throughout the later chapters of this text that structural phase transitions are closely associated with changes in the physical properties of materials.

4.4.1 Classiﬁcation of Phase Transitions The traditional way of classifying phase transitions was suggested by Paul Ehrenfest based on how chemical potential (which is simply the Gibbs free energy G per mole) changes at the phase transition. From thermodynamics we know that (∂G/∂p)T = V and (∂G/∂T)p = −S. Since entropy and enthalpy changes at a phase transition are related by ΔS = ΔH/Tc, it follows that for a phase transition such as melting or boiling, in which there are abrupt changes in both volume and entropy/enthalpy, there will be a discontinuity in the ﬁrst derivative (or slope) of the free energy with respect to temperature (and pressure). Such a transition is therefore called a ﬁrst-order transition. Since constant-pressure heat capacity, Cp, is deﬁned as (∂H/∂T)p, it will be inﬁnite at the phase transition. The existence of a signiﬁcant latent heat (ΔH) means that ﬁrst-order transitions display a hysteresis, a difference in phase-transition temperature on warming and cooling. We can understand this through a simple thought experiment: if a sample is warmed to Tc and held at precisely this temperature, the phase transition will not initially occur as there is no temperature gradient between the surroundings and sample to allow the ﬂow of latent heat. It is only when the surrounding temperature is raised above Tc that latent heat ﬂows and nuclei of the new phase begin to form. A ﬁrst-order solid state transition will therefore lag behind the temperature change causing it in any real experiment. The sample remains at temperature Tc during the transformation while the heat supplied feeds the higher entropy of the product (drives the transition). This means that the presence of two phases in coexistence is a criterion for the ﬁrst-order phase transition. To obtain any hysteresis intrinsically associated with a ﬁrst-order transition, this kinetic factor has to be eliminated by extrapolating temperaturedependent measurements to the zero rate of temperature change. A second-order phase transition is one in which there is a discontinuity in the second derivative of the free energy with respect to temperature or pressure. The volume and the entropy (and therefore the enthalpy) do not change abruptly at the phase transition, but quantities such as the volumetric coefﬁcient of thermal expansion or heat capacity do.15 The dependence on temperature of various thermodynamic quantities for classical ﬁrstand second-order transitions is shown in Figure 4.12.

15

The volumetric coefﬁcient of thermal expansion, αV, as αV ¼ ð1=VÞ∂V=∂T ¼ ð1=VÞ∂2 G=∂P∂T and Cp as Cp =T ¼ ð1=TÞ∂H=∂T ¼ ∂S=∂T ¼ ∂2 G=∂T 2 .

4.4

H

S

V

G

Structural Phase Transitions

Cp

137

first order

V

G

T

T

T

T

Cp

H

S

T

second order

T

T

T

T

T

Figure 4.12 Variation in thermodynamic quantities at ﬁrst- and second-order Ehrenfest phase transitions. The vertical dashed line corresponds to the transition temperature.

W1

W2

W3

W3

Figure 4.13 The Euler strut. When the load on the strut is increased (weights W3 > W2 > W1), the system will eventually buckle causing a reduction in symmetry.

It is now more common to categorize phase transitions as discontinuous or continuous with reference to the behavior of entropy or another order parameter (see below) at Tc. At a discontinuous transition, the order parameter changes abruptly. All discontinuous phase transitions are ﬁrst-order in the Ehrenfest classiﬁcation. During a continuous phase transition, the order parameter changes in inﬁnitesimally small steps, as in a second-order transition. These concepts are developed further in the following sections.

4.4.2 Symmetry and Order Parameters We can deﬁne many of the phase transitions we’ll encounter in terms of the changes in symmetry that occur. Figure 4.13 illustrates the relevance of symmetry using a simple mechanical model, the Euler strut. If we place increasing weights on top of a ﬂexible plastic rod, the rod will buckle or bend at some point. When this occurs, the symmetry of the system is lowered or broken. We can see from the ﬁgure that the system could choose to buckle to the right or the left. Even if the mass was loaded perfectly centrally on the rod, the system would “choose” one direction or the other—ultimately decided in this ideal scenario by random thermal displacements of the system. An analogy to the Euler strut example in materials

138

Phase Diagrams and Phase Transitions

Box 4.1 Characterizations: Differential scanning calorimetry (DSC) Everyone enjoying an iced drink on a hot summer day exploits the fact that latent heat is needed to melt the ice before the drink’s temperature starts rising. If you plotted the temperature evolution of a freshly iced cup versus an identical standard second cup where the ice has just melted, the area between the two time-dependence curves would be proportional to the latent heat of the ice in the ﬁrst cup. This is the principle of DSC: a sample and a standard are warmed at a constant rate, and the temperature of both is “scanned” at regular time intervals, for example every second. One patented DSC method adopts a smart twist. It measures the latent heat directly in terms of the electrical power to supply it. The sample in a tiny aluminum pan, and an equivalent empty pan for comparison, are each placed in their own tiny thermostat, each having a miniature hot plate and a temperature sensor; the total of about 1 gram weight. The electronics is wired up to keep their heating rate constant during the “scan”. The extra power (J/s) needed for the sample is recorded every second upon heating through the phase transition. When summed per unit mass of the sample, it gives the latent heat. The apparatus is usually calibrated using a phase change of a standard of known latent heat and weight. This DSC method is termed a power-compensation DSC. sample thermostat

reference thermostat

Pt resistance thermometer heater He

He

He

He

power diﬀerence

The advantage of the method is a quick thermal equilibration that gives a fast response needed for high rates of heating or cooling, as well as sharp peaks that make it possible to separate closely occurring transitions. In addition to the latent heat of a discontinuous transition, it is possible to determine the heat capacity of the individual phases upon heating or cooling beyond the transition peak.

chemistry could be the phase transitions between perovskite tilt systems outlined in Chapter 1. In the ideal perovskite structure, one has 180° M–O–M bond angles (this ideal structure would normally be the high-temperature, low-pressure limit), which can bend away from 180° on cooling, lowering the symmetry of the system. As a second model of broken symmetry, consider a simple single-headed arrow that can ﬂuctuate between pointing to the left and pointing to the right. If it switches between these two orientations very rapidly, it would appear as a double-headed arrow to an observer. If, however, its rate of switching was gradually reduced, there would come a point when the

4.4

Structural Phase Transitions

139

Figure 4.14 Order‒ disorder transition in FePt alloy. cooling Pt

Fe

disordered, fcc

ordered, tetragonal

observer would see it “frozen” into one of two possible orientations. Once the arrow adopts one of the two possible orientations, it changes from appearing double-headed to singleheaded and its symmetry is reduced.16 A structure with an atom dynamically disordered over two closely separated sites at high temperature (for example, an atom in a double-well potential), which chooses one of the two sites and orders on cooling, is one example of this type of behavior. Phase transitions in ferroelectric perovskite materials such as BaTiO3 and PbTiO3, which are discussed in Chapter 8, can also be understood in a similar way. As the material is cooled from high temperature, Ti moves away from a position on a dynamic average at the center of the BO6 octahedron, freezes in an off-center position, and the material develops a spontaneous polarization. Again, this is associated with a lowering of symmetry at the phase transition on cooling. Symmetry changes leading to phase transitions can also be brought about by atomic ordering. One important example is found in FePt 1:1 alloys. At high temperatures (above ~1300 °C), FePt has the face-centered cubic structure shown on the left of Figure 4.14, in which Fe and Pt atoms are randomly distributed over all sites of the structure. On cooling, it is thermodynamically favorable to order Fe and Pt atoms in layers perpendicular to the original c axis, and the stable room-temperature structure is tetragonal (this is the so-called L10 phase). Once again we see that ordering of atoms on cooling lowers the symmetry. This particular transition is of technological relevance as the ordered material has a high magnetocrystalline anisotropy, making it possible to produce magnetically hard nanoparticles with a range of potential applications. In each of these examples it is useful to introduce an order parameter, η, to describe the distortion of the structure relative to the high-symmetry case.17 This is particularly true when the distortion involves movement of groups of atoms or molecules. In the case of octahedral tilts in perovskites, the tilt angle can be used to deﬁne the order parameter. For B cations moving off-center in a BO6 octahedron, the shift in fractional coordinate of the metal might 16

17

Note that the point at which the transition is deemed to have occurred might be inﬂuenced by the experimental method used to observe it. For example, if one used a photographic technique, a camera with a high shutter speed would record the freezing transition before one with a low shutter speed. The symbol Q is also commonly used for order parameter.

140

Phase Diagrams and Phase Transitions

be the order parameter. For the FePt transition, if we deﬁne one lattice site on the right of Figure 4.14 as being the Fe site and the second as being the Pt site, we can deﬁne the order parameter in terms of the fractional occupancy of each site by “right” and “wrong” atoms. In a perfectly ordered structure, occPt(Fe) (the fractional occupancy of Pt at the Fe site) would be 0, and occFe(Fe) = 1; in the fully disordered occPt(Fe) = occFe(Fe) = 0.5. An order parameter could therefore be deﬁned as η = 2[occFe(Fe) − 0.5] and would vary from 0 to 1 for a disordered to fully ordered material on cooling. Finally, entropy change itself is an order parameter, such as (Sliquid − S)/(Sliquid − Ssolid) for H2O freezing. Many readily measurable macroscopic quantities also show a simple dependence on η and can be used to monitor a phase transition. For example the distortion of cell parameters as a perovskite changes from cubic to lower symmetry can be expressed as a spontaneous strain,18 ε = (a − acub)/acub, and it typically depends on either η or η2.19 It’s worth noting that although the examples described above have an order parameter that could potentially vary continuously (though we’ll see that it needn’t in practice) from the high- to low-symmetry situation, symmetry itself always changes abruptly—a symmetry element is either present or absent in the structure. A continuous transition concludes when the ﬁnal inﬁnitesimal heating step causes the order to ﬁnally disappear, at which point the new symmetry emerges. For the vast majority of transitions, the high-temperature form has the higher symmetry.

4.4.3 Introduction to Landau Theory One of the advantages of introducing the order parameter to describe phase transitions in solids is that it allows one to use Landau theory20 to describe their thermodynamics. The basic assumption used in this approach is that the Gibbs free energy of the phase can be approximated as a simple power series in terms of the order parameter η: 18

Strain (ε, the proportional displacement in shape or volume) is the deformation that occurs when a material is subjected to a mechanical stress (σ, a force per unit area). For small deformations where materials behave in an elastic manner, the stress tensor of rank 2 (a 3X × 3 matrix; diagonalized in engineering to have six non-zero terms) is related to the strain tensor of rank 2 by σi ¼ cij εj where cij are elastic stiffness coefﬁcients (originally a tensor of j

19

20

nine 3 × 3 matrices; in engineering simpliﬁed to 36 cij parameters relating the stress and strain matrices) and subscripts refer to different directional components. For a uniaxial stress and isotropic body, this simpliﬁes to Hooke’s law σ = Eε where E is Young’s modulus. See, for example, Elliott [Physics and Chemistry of Solids (1998), J. Wiley and Sons] for more detail. Transitions that keep group–subgroup relationships can be categorized according to how the translational symmetry of the lattice changes at the transition: if the lattice centering changes or a superlattice is formed, the transition is called a zone-boundary transition, otherwise it is called a zone-center transition. Here the “zone” refers to the Brillouin zone introduced in Chapter 6 as the volume in reciprocal space that lies closest to each reciprocal lattice point; if lattice points are added or diluted, the zone boundaries change. Zone-boundary transitions (such as the SrTiO3 perovskite tilting discussed in Section 4.4.6) generally have ε proportional to η2 and zone-center transitions to η. We call this a phenomenological theory as it explains experimental results mathematically without using a rigorous fundamental physical law.

4.4

Structural Phase Transitions

1 1 1 GðηÞ ¼ G0 þ Aη2 þ Bη4 þ Cη6 þ . . . 2 4 6

141

(4.6)

where G0 represents the part of the free energy that does not change at the phase transition. The term G(η) − G0 thus represents the excess free energy compared to one that the unchanged form would possess if no phase transition occurred. Additional terms can be introduced to this equation if, for example, the order parameter is coupled to properties such as strain. Usually G is independent of the sign of η such that only even powers are needed, as in Equation (4.6), and it’s common to adopt the smallest number of terms required to describe a system.

4.4.4 Second-Order Transitions Let’s consider the phase transition shown schematically in Figure 4.15, which involves an oxygen atom being continuously displaced from an ideal site midway between two metal atoms—this could represent a tilting transition of octahedra in a perovskite. We can deﬁne an order parameter η in terms of the oxygen displacement from the ideal site. At high temperatures, the oxygen vibrates around its M–O–M midpoint, maintaining high symmetry (η = 0). At low temperature, the oxygen vibrates around a position displaced to the left or to the right (η ≠ 0). For this situation, oxygen displacements to the left or right (±η) are equivalent, justifying the use of even powers of η in Equation (4.6). Since the linear M–O–M arrangement is stable at high temperature (T >Tc), G(η) at η = 0 must be a minimum. The simplest expression that would produce this has to have a term in Equation (4.6) dependent on η2 with a positive A coefﬁcient. Below the phase-transition temperature Tc, the linear M–O–M is no longer stable, implying that G(η = 0) becomes a local maximum (Figure 4.15). This change requires that A changes sign from positive to negative at the phase transition. The simplest way to express this is to give A a temperature dependence such as: AðTÞ ¼ aðT Tc Þ

(4.7)

with a positive. This means that A(T) is positive for T >Tc and negative for T < Tc. In order to produce minima in our free-energy curve at η ≠ 0 below Tc, it is now necessary to include a term in the G(η) series with a positive coefﬁcient, such as one depending on η4. The Gibbs free-energy expression becomes: 1 1 GðηÞ ¼ G0 þ aðT Tc Þη2 þ Bη4 2 4

(4.8)

We can see from the form of G(η) curves in Figure 4.15 that because A(T) changes smoothly with temperature, G(η) also changes smoothly, and the phase transition occurs in a smooth or continuous fashion. At the transition temperature Tc, the state of both phases is identical, and

Phase Diagrams and Phase Transitions

M

M G( )

142

O

O M

M

T>Tc

M O

M O

T=Tc

G0

M −

T 0. Differentiating Equation (4.8) gives: ∂G ¼ aðT Tc Þη þ Bη3 ¼ 0 ∂η

(4.9)

The three solutions to this equation are:

rﬃﬃﬃ a η ¼ 0 and η ¼ ðTc TÞ1=2 B

(4.10)

For T >Tc, η = 0 represents the minimum in Gibbs energy, and there are no other real solutions. For T < Tc, this solution (η = 0) is a local maximum in Gibbs energy, and the other two solutions represent minima. The way in which η varies with temperature can be expressed even more succinctly than pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Equation (4.10). If we make const ¼ aTc =B then:

4.4

143

first order order parameter, η

order parameter, η

second order

Structural Phase Transitions

Tc

Tc

temperature

temperature

Figure 4.16 Schematic temperature dependence of the order parameter η in the Landau description of a second- and ﬁrst-order transition.

η ¼ const½ðTc TÞ=Tc β with β ¼ 1=2:

(4.11)

The parameter β as a general variable is called the critical exponent. Under the Landau approximation, the full structural order of η = 1 is acquired at T = 0 such that const = 1 and η = [(Tc − T)/Tc]½. This simple dependence of the order parameter η on temperature (Figure 4.16, left) is followed by many second-order transitions, at least close to Tc. The transition thermodynamics can be derived as follows. Substitution of the non-zero η from Equation (4.10) into Equation (4.8) gives the excess Gibbs energy acquired by the transition on cooling from Tc to T as: DG ¼ G G0 ¼

a2 ðT Tc Þ2 4B

(4.12)

Since G = H − TS, we can use S = −dG/dT to derive the excess entropy and enthalpy acquired by the phase transition on cooling from Tc to T. The full-transition values can be determined by setting T = 0 into the temperature-based terms for ΔS and ΔH below, or by setting η = 1 with Tc = B/a into their η-based terms:21 DS ¼ DH ¼ DG þ TDS ¼

a2 1 ðT Tc Þ ¼ aη2 2B 2

a2 a2 T 1 1 ðT Tc Þ2 þ ðT Tc Þ ¼ aTc η2 þ Bη4 4B 2B 2 4

(4.13) (4.14)

The derivations are explored in the end-of-chapter problems. Equation (4.14) shows that the excess enthalpy of the system is a double-well function, and the positive sign of a and B in Equation (4.13) means that entropy, as a measure of disorder, decreases as the system distorts (orders) below Tc. 21

Transition entropies and enthalpies are always reported upon heating, hence would have opposite signs to those suggested by Equations (4.13) and (4.14).

144

Phase Diagrams and Phase Transitions

The effect of the phase transition on the heat capacity can be found using the relationship Cp = T(∂S/∂T)p. Below Tc, differentiating Equation (4.13) gives: DCðT < Tc Þ ¼ T

∂DS 1 ∂η2 a2 T ¼ ¼ aT ∂T ∂T 2 2B

DCðT > Tc Þ ¼ 0

(4.15) (4.16)

We see that the heat capacity changes abruptly by a2Tc/2B at Tc. Since B is positive, and we are considering the cooling process, heat capacity shows a positive jump at Tc on cooling to the low-temperature phase (see Figure 4.12), consistent with Ehrenfest’s deﬁnition of a second-order transition. Note from this analysis that once a and B are known, all the thermodynamic quantities associated with the phase transition can be calculated. The values of a and B can be obtained by measuring Tc and one of the excess thermodynamic quantities. The way in which an orderparameter approach can be used to describe magnetic transitions is explored in the end-of-chapter problems.

4.4.5 First-Order and Tricritical Transitions We can apply similar arguments to investigate a discontinuous or ﬁrst-order transition, provided we can relate the two structures by an order parameter. Here, the high- and lowtemperature phases coexist in equilibrium at Tc. This coexistence requires that equal minima in G(η) occur for different absolute values of η; one at the order parameter η = 0 of the disordered phase and two at non-zero ±η of the ordered phase.22 The simplest Gibbs freeenergy function that will allow this coexistence has a fourth-order term negative and a sixthorder term positive: 1 1 1 GðηÞ ¼ G0 þ aðT T0 Þη2 Bη4 þ Cη6 2 4 6

(4.17)

where a, B, and C are all positive quantities as written. T0 is a temperature slightly lower than Tc, and we will derive their relationship shortly. This function has a single minimum at high T, three minima at intermediate temperatures above T0, and two minima at temperatures below T0, as depicted in Figure 4.17. As in the second-order case, differentiating Equation (4.17) with respect to η will tell us the order parameter values that give rise to minima in the free energy. Depending on temperature, there are up to three minima at:

22

Note that in the Landau model, the order parameter η is often used in a somewhat relaxed way as a transition parameter and allowed to exceed the value of 1.

T>T1

Structural Phase Transitions

145

G( )

4.4

T1 Tc G0

T